Dr. Charles Mueller ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH Impact of Atomic Effects Corrosion on Material Sustainment POTOMAC INSTITUTE PRESS P O T O M A C I N S T I T U T E F O R P O L I C Y S T U D I E S B G
POTOMAC INSTITUTE FOR POLICY STUDIES901 N. Stuart St, Suite 1200Arlington, VA, 22203www.potomacinstitute.orgTelephone: 703.525.0770; Fax: 703.525.0299Email: [email protected]
This book contains information obtained from multiple sources, including interviews. The author and publisher gratefully acknowledge the permission granted to reproduce copyrighted material in this book and have made every effort to trace copyright holders and to obtain their permis-sion for use of this material. The author and publisher apologize for any omissions and would be grateful if noti ed of any corrections that should be incorporated in future reprints or editions of this book. Government-produced materials are not copyright protected (17 U.S.C. § 105). The author and publisher do not hold the copyright to works of the United States government appearing in this publication. The author and publisher do not hold the copyright to works licensed through Creative Commons appearing in this publication. The author and publisher cannot assume responsibility for the validity of all materials or the consequences of their use; the view and opinions expressed do not necessarily re ect those of the Institute and publisher.
This is a product of the Potomac Institute for Policy Studies. The conclusions of this study are our own and do not necessarily represent the views of the sponsors or participants.
Note: All images included abbreviated citations in text – full attributions are provided for all images and can be found under Image Credits, page 171. All hyperlinks current as of November, 2015.
ALTERNATIVE FUTURESFOR CORROSION AND
Impact of Atomic Effects Corrosion on Material Sustainment
FOREWORDThe e e e e e i i e e i he i hi the e the e et e e e i t t te ti i e -
ti te i i e h v i it e i e t the i t t e ith hi h e e e t i it e ti t the -te
t te te i e the e t i h e t i te e e h eve e t the eve ti iti ti i th e i e t
i t t e
Many research efforts in the corrosion revention enter rise have een an re ain foc se on s eci c in ivi a echanis s of corrosion These efforts have tra itiona y foc se on
e ra ation fro the che ica environ ent an che ica reactions at the o ec ar eve M ch oo science has een eve o e an that science has res te in any ne corrosion revention an iti ation etho s an a ications ith the rea th of techno o ica iscovery e an in ho ever e are certain that echanis s eyon che ica reactions are ca sin ateria s to e ra e s a res t e have eco e con-vince that a roa er research a en a is nee e to a ress ateria s e ra ation ef-fects in ne areas s ch as ato ic effects an io o ica inc in acro o ec ar an
icro io o ica effects corrosion
n a ition to the roa er a en a e e ieve a ore coor inate cross- o n ary ti-isci inary a roach is re ire to iscover the n er yin echanis s of e ra ation
effects s ch as tin his ers on icroe ectronics in hich ea -free so er is se rther-ore in or er to coor inate this roa er research a en a e e ieve there are acco -anyin o icy an strate y initiatives that nee to e i e ente
The ateria in this oo a es the case for a roa er e nition of corrosion to encompass all mechanisms of materials e ra ation e to environmental effects e they chemi-cally in ce atomic or thro h other iolo ical mechanisms e nee to n erstan these mechanisms a ress their effects an miti ation an evelop etter metho s for preventin etectin pre ictin an mana in e ra ation n a ition this oo e -plores atomic effects corrosion in etail an recommen s initiatives to stren then o r na-tion s efenses a ainst emer in mechanisms of materials e ra ation loo for ar to contin in to or on innovative material s stainment ase on the ri oro s science an analysis in: Impact of Atomic Effects Corrosion on Material Sustainment
Daniel J. Dunmire
PREFACEThe p rpose of this oo is t o-fol :
• irst to ar e for a roa er e nition of corrosion rather than the tra itional e nition that is limite to chemical reactions only peci cally e call
for e pansion of the e nition to incl e materials e ra ation an an approach to com attin e ra ation that e call material sustainment
• econ to escri e one of the elements of that roa er e nition: speci cally that of e ra ation at the atomic level hich e call atomic effects corrosion (AEC).
ince efore recor e history man in has een concerne a o t materials e ra a-tion n prehistoric times people s concern as ith e ra ation of simple tools fashione from materials fo n in nat re for e ample a oo en cl co l e ra e very ic ly thro h iolo ical mechanisms s ch as rot s society a vance the search for thin s that last an conse ently material s stainment too on ifferent imensions The ron e for e ample intro ce a ne ilemma: tools an eapons ma e of iron ere m ch stron er than those ma e of ron e t iron o ects ere also more prone to r st (corrosion s a res lt rin the ron e people ha to consi er tra e-offs: o se a stron er iron tool that e ra es more ic ly or eep the ea er t less li ely to corro e
ron e tool t is not har to ima ine ho that choice as ma e rather ramatically after the rst ht et een s or smen ith iron an ron e eapons o ever ith the chan e to stron er iron eapons an other tools the iss e of chemical corrosion ecame a m ch more important consi eration
s man in a vance thro h the a es the a ility to a ress material e ra ation im-prove as scienti c no le e of the associate mechanisms increase an en ineers
evelope co nters s ch as coatin s to re ce the impact of corrosive effects ith the a n of atomic eapons an po er an h man e ploration of space e iscovere
ne mechanisms of materials e ra ation eyon chemical reactions at the molec lar level t the nat re of atomic effects associate ith n clear eapons po er an aste pro cts ere often hi hly classi e an to a lar e e ree ept separate from the main-stream of corrosion science o that e have entere the nformation e e are see-in atomic effects in other areas s ch as microelectronics that cannot e e plaine y the classic chemical e nition of corrosion ome of these effects s ch as tin his ers ( hich occ r in applications in hich lea -free sol er is se for e ample have not een e plaine other than it s not chemical or electrochemical n a ition ne plaine effects in micro iolo ical environments are emer in e call these iolo ical effects cor-rosion an intro ce them rie y in this vol me ltimately to effectively ht corrosion in all its forms e nee to a opt the concept of the corrosion spectr m
The categories in the
• Atomic effects corrosion (AEC) describes atoms degrading; that is mechanisms ithin the atom that ama e or estroy the atomic str ct re There are several ays can occ r s ch as hi h-ener y collisions et een atomic particles that split the atom
• Classical corrosion describes molecules degrading; that is interactions et een atoms an molec les s ch as the chemical ionic reactions that form r st an other types of visi le corrosion
• Biological effects corrosion describes complex degradation beyond the scale of simple atomic decay or molecular chemical reactions; that is interactions et een iolo ical comple es incl in comple or anic macromolecules that e ra e comple systems
Title of the o e c rrently e nes corrosion as the eterioration of a material or its properties e to (em-phasis a e 1 e conten that in the mo ern a e the tra itional application of this
e nition is too restrictive n or er to properly con ct the roa -spectr m research nee e to n erstan the mechanisms of materials e ra ation an then evelop effective metho s for miti atin these effects a roa er e nition is nee e This oo proposes e pan in the e nition to incl e effects other than chemical reactions recommen s a comprehensive spectr m of coor inate research escri es atomic effects corrosion ( an recommen s strate y policy an research initiatives to a ress these effects
trate y policy an research are all relate in fact o r propose strate y an policy recommen ations are so closely relate that e isc ss them to ether in essence o r recommen ation is that the orrosion olicy an versi ht f ce ( nee s a stra-te ic plan to coor inate the policy initiatives nee e to achieve material s stainment thro ho t the corrosion spectr m
The orrosion pectr m rro
ma e cre it: le Taliesen
1 Develop a comprehensive policy for the corrosion spectr m
sta lish a roa er coor inate research pro ram that crosses o n aries in the corrosion spectr m
entify an ma e speci c policy chan es ithin the comprehensive policy ase on research o tcomes
esearch n erpins an s pports the strate y policy o ectives so that the has a rm scienti c asis for initiatives thro ho t the corrosion spectr m
Initial Research Directions
1 il for elia ility meanin con ctin research that ena les n erstan in of physical phenomena an interaction
mechanisms thro ho t the corrosion spectr m in or er to improve systems esi ns from the ottom p (from f n amental-level n erstan in of material properties
entify Threshol s meanin eterminin hen matters to material s stainment in terms of oth n m ers of events an time
This oo is the secon in a series p lishe thro h the otomac nstit te for olicy t ies a ressin lternative t res for orrosion an De ra ation esearch n the rst oo Dr o ert mmel a resse the topic of alternative f t res n this oo
Dr harles M eller rills into the etails of follo -on oo is plane to a ress iolo ical effects corrosion
ACKNOWLEDGEMENTSThe a thor o l li e to e press his sincere appreciation to his mana ement an col-lea es at the otomac nstit te for their i ance an assistance rin the research an preparation of this oo n partic lar he o l li e to than Mr Michael etnam an Dr ennifer ss for their patience an i ance in completin this comple tas n a ition he o l li e to than his collea es Ms ennifer ato an Dr a l yers
itho t hose assistance the research references an man script for this oo co l not have een complete in time
Charles Mueller, PhD otomac nstit te for olicy t ies
CHAPTER I: INTRODUCTIONorrosion is a national pro lem estimate to cost ta payers each
year 1 veryone no s hat happens if yo leave a steel shovel o t in the rain: it r sts st is an e ample of classical corrosion hich occ rs hen the iron molec les in
the shovel react chemically ith the ater molec les in the rain formin hat chem-ists call ferro s o i e hich is r st orrosion ca ses pro lems oth in Department of Defense (DoD an society an the DoD orrosion olicy an versi ht f ce (
as esta lishe ithin the f ce of the ecretary of Defense ( D to prevent miti ate an mana e corrosion in o r systems an infrastr ct re To e ne the s mission a (Title 1 e nes corrosion as the eterioration of a material or its properties e to
a reaction of that material ith its environment (emphasis a e hile this e nition serve s ell in the n strial e this e nition is no lon er s f cient
There are m ltiple ays materials can e ra e e to interaction ith their environment sho n in the Corrosion Spectrum elo These types of e ra ation are not ne t in the past their effects ere seen mainly in speciali e areas s ch as n clear eapons or space satellites s technolo y contin es to a vance these e ra ation mechanisms are sprea in into a roa er ran e of systems or e ample as microchips have prolifer-ate thro h many systems an those chips are ecomin more sophisticate atomic effects corrosion is e pan in eyon the speciali e realm an into common systems
The orrosion pectr m rro
ma e cre it: le Taliesen
14 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The categories in the
• Atomic effects corrosion (AEC) describes atoms degrading; that is mechanisms ithin the atom that ama e or estroy the atomic str ct re There are several ays can occ r s ch as hi h-ener y collisions et een atomic particles that split the atom
• Classical corrosion describes molecules degrading; that is interactions et een atoms an molec les s ch as the chemical ionic reactions that form r st an other types of visi le corrosion
• Biological effects corrosion describes complex degradation beyond the scale of simple atomic decay or molecular chemical reactions; that is interactions et een iolo ical comple es incl in comple or anic macromolec les that e ra e comple systems
Title 1 c rrently limits the s a thority to classical chemical corrosion only on ress nee s to chan e the la hich can e accomplishe y simply removin the or chemical from the e nition This chan e ill ena le the to p rs e an coor-inate research policy an strate y across the corrosion spectr m to stren then o r
nation s efense a ainst materials e ra ation
This intro ctory chapter rie y escri es o r previo s research in the corrosion arena then e intro ce the concept of material s stainment as a str ct re iscipline approach for a ressin corrosion across the spectr m ith the conte t of material s stainment thro ho t the spectr m e ne t e plain in etail hy the c rrent Title 1
e nition of corrosion is ins f cient The chapter concl es y overvie in the str ct re of the remain er of the oo
n 1 the tas e the otomac nstit te for olicy t ies ( to evelop a co-or inate research an evelopment pro ram for the prevention an miti ation of corrosion for ne an e istin military e ipment an infrastr ct re The st y title
lternative t res for orrosion an De ra ation esearch ( D 4 recommen e a lon -term strate y to prevent etect pre ict an mana e corrosion so as to a ress the effects of corrosion an e ra ation on e istin systems an ne ac isitions
15CHAPTER I: INTRODUCTION
ccor in to the D st y the tas of pre-ventin an miti atin corrosion an e ra a-tion is est approache n er the r ric of ma-terial s stainment That is esi nin il in maintainin an shepher in systems s ch that the materials an components f nction for their e pecte lifetimes s a iscipline material s s-tainment foc ses on the life cycle of str ct ral an constit ent materials an a resses the ca ses of e ra ation in all forms n the recom-men ations portion of the D st y the st y team recommen e that the el of ma-terial s stainment sho l e enhance ith lon term coor inate research o ectives to com-plement c rrent research hich primarily foc s-es on speci c shorter-term o ectives n s m the D st y intro ce the concept of material s stainment hich e e plore an e -plain in the ne t section
ne research o ective intro ce in the D st y as investi atin the ant m effects that in ence corrosion an e ra ation of evices an systems s ch as micro-electronics at the atomic an s -atomic scales se ently the st y team i enti-e the applica le mechanisms that res lt in corrosion e to ant m an relate
effects hich the st y team has rephrase as atomic effects corrosion ( ll cor-rosion involves events that chan e the properties of materials an materials are f n a-mentally ma e p of atoms lassical corrosion typically involves chan in the n m er of electrons s rro n in an atom (for e ample y chemical o i ation an re ction reactions tomic effects corrosion is ifferentiate y the mechanism that ca ses the chan e to in ivi al atoms lassical corrosion encompasses e ra ation interactions
et een m ltiple atoms an molec les a resses e ra ation atoms
That is classical corrosion arises e to chemical reactions et een molec les normally at l level (many atoms or molec les atomic effects are those phenomena that ca se chan es to the n clei of atoms f n amentally chan in the atomic properties of the in ivi al atoms affecte tomic effects can e ca se y spontaneo s ra ioac-tive ecay an hi h-ener y collisions of li ht pac ets (i e photons or matter particles (e ne trons n a ition atomic effects encompass other phenomena s ch as el effects that ca se atoms to chan e or move for reasons other than the chemical ef-fects a resse in classical corrosion st ies n terms of material s stainment atomic effects corrosion can have impacts that are as important as classical corrosion an the t o are at times co ple (e an atomic effect can ca se a chan e that res lts in chemical reactions the atomic effect there y ecomes the initiatin mechanism for classical corrosion
16 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
hile classical corrosion is ell- evelope scienti c el atomic effects corrosion an its impacts on materials an systems of interest to the DoD are not yet ell an i ely
n erstoo To increase n erstan in of corrosion mechanisms an then improve o r a ility to ens re the material s stainment of systems ith implications for national sec rity re ires a ressin the effects of corrosion across the spectr m not st one part of it (classical corrosion The conte t for accomplishin this oal is a resse in the ne t section hich a resses material s stainment as a iscipline
the discipline of material sustainment
mans il thin s ith the intention that they sho l last Thro ho t the transition from h nter an atherers to a ric lt ral comm nities an societies ase on pop la-tion centers h mans have evise tools e ipment an ellin s to perform thro h a lifetime an eyon
s a res lt h mans fo n lon a o that certain materials are etter s ite at ma in thin s that last (for instance the re elo sho s the evelopment of lon er lastin
etter arti cial li hts or e ample the earliest e amples of ceramics are fo n in -rines from at least 5 5 ottery se for coo are an vessels ates from
6 Metals came later ith ol se for e elry appearin aro n 6 an s -se ent metals s ch as copper silver an lea appearin more than 5 years a o 7
17CHAPTER I: INTRODUCTION
The opper e is ascri ed to the period to 4 8 which transitioned to the ron e e wherein tin was added to copper to form an alloy that is more easily worked and fashioned into tools and implements. The introduction of the ron e after the ron e e around 1 is most si ni cant.1 ron is more a undant and more easily smelted and when com ined with car on it can produce stron er and etter tools (and weapons . owever it can deteriorate and of course rust.11
y the way to determine the a e of the ancient artifacts mentioned a ove scientists use radiocar on datin which is ased on an atomic de radation effect: the amount of the car on-14 isotope remainin in an o ect. s o ects row older the car on-14 in them decays y measurin the amount of car on-14 relative to the other (more sta le car on isotopes scientists can estimate an ancient artifact s a e. o atomic ef-fects de radation is not always a ad thin and radiocar on datin is one of the est mechanism we currently have for determinin the a e of ancient items. hat we are concerned a out in this ook is atomic effects that do indeed have deleterious effects.
The ultimate cost of a tool or o ect is the amorti ation of its cost of construction over its period of service. ccordin ly the lon er the service life the lower the overall cost. There are multiple ways to uarantee a lon er useful life span. ne of the most impor-tant is to employ materials that resist corrosion and de radation.
nterestin ly the development of improved tools in the ron e coincided with a lar e increase in the development of weapons that used steel which included chariots armor and shields swords and da ers and spears.1 hether it was the need for etter tools or an arms race to produce stron er weapons the military has consistently een at the forefront of the ac uisition of o ects that have su stantial permanence. n part the military value of new weapons in the ron e was a conse uence of steel s stren th and hardness. To this day the military is interested in ac uirin thin s that will last in stora e or in use for known and predicta le lifespans (e. . sophisticated military air-craft such as that depicted in the ure on pa e 18 . f weapons or military e uipment fail prematurely due to de radation our military capa ility will e adversely affected. Therefore stren th remains a ma or performance oal of materials used in military appli-cations. Today however material sustainment is not merely a direct result of the stren th of the constituent materials ecause weapons have ecome more sophisticated and
11. . 1 .1 . 1 1 . .
1 1 .
18 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
dependent on complex su systems such as microelectronics. ustainment remains an important oal for military e uipment oth in terms of cost control and sustained readi-ness and accomplishin that oal is ettin more complex as technolo ies ecome more sophisticated.
s a discipline the oal of material sustainment is to ensure that thin s have reason-a le predicta le lifespans with minimal maintenance re uirements. Therefore material sustainment must address causes of all forms of de radation in all technolo ies y virtue of usin materials and construction techni ues that prevent or miti ate de radation due to external environmental causes. There are multiple ways of cate ori in causes of de radation. s we have already discussed classical corrosion often arises from chemi-cal or electrochemical action y the environment that causes de radation on materials used in DoD systems.
There are other causes of corrosion that are less common or less visi le ut can still cause premature a in and failure. or example some materials simply under o disso-lution for example y dissolvin in water. Mechanical wear is enerally not considered corrosion in and of itself ut is often a component of de radation that can involve multiple causes. ndeed metal fati ue involves structural chan es to the or ani ation of rains in metal and is enerally caused y mechanical stresses and cycles imposed
y purely physical (as opposed to chemical phenomena. n 1 54 the conse uences of metal fati ue were dramatically demonstrated with the failure of two de avilland aircraft.1
13. 1 1 . .
1 . .
Nuno Andre /www.shutterstock.com
1CHAPTER I: INTRODUCTION
adiation that impin es on materials is another cause of de radation. or example polymers su ected to ultraviolet li ht ( will eventually ecome rittle crack or
reak.14 ther kinds of radiation: -rays amma eta and alpha radiation can also cause various kinds of material chan es from ioni ation of molecules to causin nuclei of atoms to transmute throu h fusion or ssion. Microelectronics in particular (see ima e
elow are suscepti le to chan es induced y radiation. As feature si es (the si e and spacin of electronic components in a microchip decrease and component densities increase in microchips radiation-induced effects can ecome even more pronounced.
n the other hand for some atomic-level mechanisms decreasin feature si es increas-es chips radiation tolerance. As we ll explain later in the ook the impact of radiation on microchips is a complex topic.
Materials can also e su ected to elds that cause de radation. ravity slowly causes the atomic structures of silica molecules in lass to deform over time. lectrical elds in semiconductors and electronic circuits can cause atoms to ecome displaced causin de radation. ven ma nets can de rade over time due to thermal effects that cause
14. 4 .
ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
their magnetic strength to wane these effects are particularly important for motors that depend on compact powerful magnets.
A material s properties are determined y the composition and arrangement of its su -stances. hen the material experiences a change in its composition or molecular ar-rangements that material has degraded from its original state. or many materials a large num er of atomic changes must take place efore the properties we tend to care a out start to ecome compromised. owever this does not change the fact that any one change might e the initiating event that ena les additional or more rapid degra-dation of that material. nowing the full spectrum of processes that lead the changes in a materials property is critical to a truly successful material sustainment strategy.
e use the term material sustainment as opposed to corrosion and degradation pre-vention and mitigation in order to emphasi e the primary goal: to ensure that systems function as designed for their designed lifetimes. During its lifetime the system should not suffer from unexpected loss of functionality or the need for unexpected servicing due to deterioration from external (environmental effects. nstead systems should have pre-dicta le performance and maintenance costs re uired y degradation from external in uences should e minimi ed. Accordingly from the standpoint of developing good policy and directing research in areas that have the greatest impact it is important to understand the road set of environmental in uences and physical phenomena that can cause degradation to materials and thus the functionality of a system.
The reason that corrosion is traditionally restricted to causes attri uted to external in-uences is the perception that the external environment is less controlla le whereas
internal effects are more an issue of design and use which are under the developer s and user s control. This perception is true only to a certain extent. ometimes internal in uences have to do with re uired design elements. or example radioactive materials will degrade according to their half-lives and that might e an internal design element that is re uired for functionality as noted in the use of radiocar on dating for ancient artifacts sometimes radioactive decay is key to the use of such techni ues. n other cases the internal components might show incompati ilities that are not expected or known when the system is designed and as a result these components cause degrada-tion in functionality that is not controlled y the user. alvanic corrosion in which two or more metals in contact corrode due to electrochemical reactions etween the metal interfaces is a common example of incompati le materials corroding.
hat is normally omitted from the study of corrosion is degradation that is due to wear and tear. ear and tear is usually considered to e an internal effect in the sense that the system operates under normal conditions and that expected degradation effects occur independent of the external environment. Metal fatigue would generally e considered an example of wear and tear. f course wear and tear can also cause unexpected failures. Thus wear and tear should not necessarily e omitted from the
roadened eld that we are calling material sustainment. nexpected failure can e the result of the lack of a good prediction model of how wear and tear will degrade a
1CHAPTER I: INTRODUCTION
system or failures increase ecause the system is used in unexpected ways. n essence a well-designed material sustainment approach not only addresses individual effects
ut the relationships of multiple potentially coupled effects.
urther wear and tear effects can work in con unction with corrosion and degrada-tion that does involve the external environment. To the extent that systems interact with in uences from the external environment corrosion prevention and mitigation gener-ally involves proactive defense mechanisms including defenses against wear and tear along with com atting corrosion due to the environment. nvironmental in uences can include weather temperature physical stresses electromagnetic elds magnetic elds radiation or other effects. ome of these effects could e generated through the in-teraction of materials within the system as in galvanic corrosion from contact etween dissimilar metals and others can e strictly dependent on external in uences.
To promote material sustainment and the associated research and policies to address degradation effects that cut across chemical and other effects the distinctions etween wear and corrosion should e viewed as exi le. The intent of material sustainment is that systems designed and ac uired y the military or any ranch of government should have predicta le life spans that are free from surprise premature degradation whatever the cause.
Thus the uest for material sustainment involves com atting myriad causes of degra-dation. These causes often act in compound ways and sometimes in ways that are not yet fully understood. lassical corrosion as we might call it has een a ma or hin-drance since the ron Age and therefore chemical and electrochemical causes are relatively well understood. owever other types of degradation are less o vious and in some cases less understood and the conse uences of these types of degradation can
e more dif cult to prevent or mitigate. rom a strategic perspective a champion is needed to coordinate the research and policy needed to com at degradation and we argue that the is ideally and uni uely positioned to e the champion of mate-rial sustainment.
articularly in the area of microelectronics with increasing design complexity and com-ponent densities degradation may e caused y relatively few single events that sig-ni cantly impact performance and therefore degradation of microchips is ecoming increasingly important. To assist in identifying the research policy and strategy issues associated with the less well-understood degradation mechanisms related to material sustainment this ook focuses on atomic effects corrosion (AEC) which is corrosion at the atomic level. The third volume planned for the ook series featuring Alternative u-tures for orrosion and Degradation esearch will address iological effects corrosion which involves even less well-understood complex degradation mechanisms including micro iological and macromolecular effects.
ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
n the next section we complete the case for adopting the discipline of material sustain-ment and the role of as its champion y explaining why the current de nition of corrosion is inade uate. These concepts are fundamental to improving material sustain-ment across the corrosion spectrum. imply put limiting corrosion to a single part of that spectrum is insuf cient.
the current definition of corrosion – and why it is inadequate
The . . ode Title 1 u title A art hapter 1 1 section 8 su section (f (1 de nes corrosion as follows:15
The term “corrosion” means the deterioration of a material or
This same law states that the DoD has a responsi ility for the prevention and mitiga-tion of corrosion of military e uipment and infrastructure of the DoD. As such the clear intention is to prevent or mitigate degradation as de ned y the term corrosion. (The photographs on the next page depict mulitple cases of classical corrosion. The is ased within DoD ut since corrosion and degradation affect all aspects of society their oversight of solution paths impacts all levels of government and society. owever the current notion of chemical environment is too limiting. hemistry is ust one of the processes y which material properties change and the prevention detection pre-diction and management of materials degradation y any mechanism is part of the
s mission. n order to implement material sustainment as a discipline the needs to e a le to address corrosion across the spectrum from atomic to classical (chemical to iological effects.
The degradation of materials due to environmental effects depends on the kinds of en-vironments and their conse uent effects in which we operate and on the materials we are using in those environments. n the prehistoric (and thus pre-science era the relevant environmental effects were often primarily iological. hen a caveman (let s name him g selected a stout tree lim and made it into a clu he knew nothing a out the scienti c mechanisms of the environment in which he was operating. hat
g did care a out was the integrity of that clu : if it rotted it was no longer useful to him. hether it rotted due to chemical corrosion (e.g. molecular changes caused y chemical reactions induced from soaking the clu in water for example or iological activity (e.g. acteria/mold eating the wood did not matter: what g knew was that he needed a strong clu to survive. f course we are well eyond the prehistoric era and we can use science to systematically investigate the underlying mechanisms of degradation and develop measures to prevent or mitigate degradation.
15. 1 . . . . 1 .
CHAPTER I: INTRODUCTION
4 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
o why is our current de nition limited to chemical effects e surmise that until recently these were the effects that caused the most prominent degradation of materials. n the various metal ages ( ron e iron etc. chemical reactions were the primary and cer-tainly resulted in the most o serva le degradation effects. As we moved into the ndus-trial Age our tools and our e uipment were ased mainly on metals and other materials that corroded due to chemical reactions. Most are familiar with the rust that forms on iron or steel o ects or the green patina that forms as copper corrodes. ocieties are af-fected y infrastructure degradation such as ridge structures crum ling and ultimately collapsing. All of these effects can e explained as the deterioration of a material or its properties due to a reaction of that material with its chemical environment.
The pro lem with limiting corrosion to the chemical environment is that even the common terminology of corrosion of metals involves multiple in uences including the environment that are not strictly speaking exclusively chemical in nature. or ex-ample stress corrosion cracking involves the con uence of physical material stress as well as chemical interactions. ltraviolet radiation can cause ioni ation of polymeric materials that can cause degradation in the properties of polymers such as coatings or plastics. The proposed discipline of material sustainment cannot e reali ed if we are interested in degradation solely due to a chemical environment. f radiation or an electromagnetic eld causes degradation that reduces a system s useful life cycle due to interaction with the external environment a material sustainment approach must e concerned with those mechanisms too. ince the intent is to provide material sustainment in DoD systems and infrastructure consideration of all external environ-ments and physical processes that can cause degradation of systems is of importance to DoD when designing elding and maintaining systems. n short material sustain-ment must address degradation across the spectrum not limit itself ust to classical chemical-reaction ased corrosion. ee The orrosion pectrum gure page 5.
As technology advances the importance of mechanisms in addition to chemical re-actions is increasing. or example we already know a out degradation affects at the atomic level that occur in nuclear materials: weapons power plants nuclear waste and the nuclear waste storage containers. urthermore we understand many of the com inations of effects that can occur in for example nuclear waste storage con-tainers that deteriorate due to oth chemical and atomic effects.16 Atomic effects cor-rosion in the nuclear arena falls under the purview of the Department of nergy (Do and Do has an extensive research and monitoring program to detect and mitigate A in nuclear programs.
owever nukes are not the only arena in which atomic effects are o served. or ex-ample the tin whiskers that occur in electrical devices were rst o served in the vacu-um tu e era of the 1 4 s and 1 5 s. Though tin whiskers have een studied extensively no one is certain what causes them. n addition as microelectronics ecome more so-phisticated a few atomic-level events can result in signi cant degradation effects that
16. . 14 .
5CHAPTER I: INTRODUCTION
are discerni le at the macro level in terms of a microchip s a ility to function properly. The point is that materials degradation can occur in numerous modern technologies y mechanisms that are de nition of classical corrosion.
Though this ook does not explore macromolecular iological effects in detail it is ap-parent that atomic effects are not the only new (relatively speaking mechanisms y which materials degradation occurs. Micro iological effects have een o served in numerous areas and these mechanisms are also not fully understood. or example it appears that there are iological mechanisms causing even synthetic materials such as tents to rot even though the tents are not constructed of iologically- ased cloth. These mechanisms are not yet fully determined they may e purely chemical they may e chemical reactions induced or cataly ed y micro iological agents or they may e com inations of multiple-cause mechanisms in the macromolecules that we increasingly use in synthetic materials. e call these iological effects corrosion and plan to address them in the third ook in this series Alternative utures for orrosion and Degradation esearch.
mage credit: Alex Taliesenorrosion pectrum Diagram
6 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The ottom line is that identifying chemical reaction mechanisms is no longer suf cient for dealing with materials degradation and promoting the discipline of material sustain-ment. or this reason we propose that the de nition of corrosion needs to e roadened. t should not e limited to deterioration due to reactions with the chemical environment it should include degradation due to all environmental effects. Therefore we propose
that the de nition of corrosion should e updated to:
Corrosion means the deterioration of a material or its properties
n short corrosion should e roadened to include materials degradation throughout the spectrum and include A classical corrosion and iological effects corrosion. n concert with this de nition we further recommend the adoption of the term material sustainment to descri e the coordinated research policy and strategy for prevent-ing detecting predicting and managing materials degradation. The remainder of this
ook focuses on A ut as we address this non-classical corrosion mechanism the reader should keep in mind that iological effects are also important. hether A or
iological effects limiting material sustainment to classical chemical-reaction effects is .
organization of the book
The main ody of this ook is designed to e reada le y reasona ly educated non-scientist laymen trying to understand A its impacts and the research policy and strategy implications associated with a coordinated approach to material sustainment. Therefore the main ody comprises two additional chapters.
hapter provides a description of the various kinds of A . The description egins with the phenomenology of A degradation mechanisms: high-energy collisions elds and spontaneous decay (for context we also rie y address the low-energy collisions associ-ated with classical chemical corrosion . The phenomenology overview is followed y speci c applications in which signi cant A impacts can occur. These applications include speciali ed applications such as space and nuclear systems ut also increas-ingly common widely proliferating microelectronics. This ook is unclassi ed which limits the discussion of some nuclear system details we can however descri e many of the phenomena that take place in these systems. or example the rst ook in the Alterna-
series descri ed atomic effects in nuclear systems at the unclassi ed level.17 n this ook we summari e these effects only: further detail a out the speci c mechanisms of A and how they affect speci c systems could move into the classi ed arena and we purposely avoid that possi ility.
hapter provides our recommendations for the in the areas of strategy policy and research. These three topics are closely interrelated and in fact we discuss strategy and policy together ecause in the area of material sustainment these topics are inter-twined. esearch underpins strategy and policy and we segment it from strategy and policy only to present the recommendations in a logical order.
1 . . 14 .
7CHAPTER I: INTRODUCTION
This nal chapter egins with an overview of strategy policy and strategic planning for policy identi cation and implementation and recommends strategic and policy initia-tives we elieve the is ideally suited to implement. The research recommendations that follow the strategy/policy section are intended to support the development of othpolicy and strategy. hapter also includes descriptions of DoD interests to include interests in areas that other agencies own (e.g. NA A for space Do for nuclear sys-tems . These recommendations are in no fashion an attempt to roaden DoD s control:they are simply factual descriptions of the interests DoD has in the systems and associat-ed material sustainment of those systems in these arenas. The purpose of including themis to provide context for the recommendations. ith regard to research recommenda-tions we reinforce the need for a coordinated research agenda. This is not a criticism ofthe extensive and excellent research oth completed and ongoing in speci c areas. t is ased on an o servation that stove-piped research alone is insuf cient to fully inform the policy and strategy associated with the complex mechanisms associated with mate-rial sustainment in the modern age. e also provide examples of research to prime thepump for research in support of speci c strategy and policy changes.
All three chapters of the main ody of this ook are structured so that an interestedreader can complete them in a single sitting. or the reader interested in more depthand additional scienti c/technical detail the ook includes two appendixes. The rstappendix contains additional material on the classi cation structure of materials. This ap-pendix is not intended as a text ook ut an introductory compilation of the materialscience associated with the corrosion spectrum. The second appendix provides morescienti cally oriented descriptions of examples of A in DoD. oth appendixes are tar-geted to the more scienti cally inclined reader who wants to dig into the details in moredepth than the main ody of the ook.
8 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH8 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Image Credit, Alex Taliesen
CHAPTER : THE SCIENCE OF MATERIALS DEGRADATIONThis chapter provides a rief description of materials degradation effects and the as-sociated science. The science is descri ed so that a reasona ly educated non-scientist can understand it: its purpose is not to delve into the details of the science (which are overviewed in Appendix 1 ut to ena le the reader to understand the various effects what is known a out them and to point out some of the unknowns. e do descri e some of the mechanisms using scienti c terms ut we keep those descriptions at a rela-tively high level.
To provide a proper context for understanding A the chapter egins with a reprise to the corrosion spectrum which includes atomic effects (i.e. A chemical reaction (e.g. ionic effects which is classical corrosion and iological effects (i.e. complex corrosion . Next the chapter descri es the various forms of degradation within this spec-trum how A is uni ue and the way A affects nuclear weapons nuclear power nuclear waste disposal space and perhaps most signi cant of all: microelectronics. As technology continues to develop and ecome increasingly dependent on microelec-tronics A associated with microelectronics has implications across the information technologies control monitoring and other systems in oth the DoD and in roader society.
introduction – the corrosion spectrum
The corrosion spectrum (see gure at the top of the next page descri es the various contexts of materials degradation. ts intent is to provide a way to classify the distinct pathways the different facilitating causes and the diverse impacts of degradation. The underlying physical processes ehind materials degradation de ne the corrosion spec-trum. e propose that this spectrum egins at the atomic level which we categori e as atomic effects corrosion (i.e. A where su atomic particles and spontaneous decay cause degradation of material properties. As we move across the spectrum the si e of the degradation particles increases to that of atoms ions and small molecules ringing us into the realm of classical chemical corrosion (e.g. ionic effects . The corrosion spec-trum ends as the si e of the degradation particles reaches that of macromolecules such as those produced y iological organisms leading to complex interactions that facili-tate the degradation of micro- and macrostructures in materials (i.e. iological effects .
The underlying physical processes
behind materials degradation de ne
the corrosion spectrum.
ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
iven the topic of this ook it is reasona le to uestion why we claim A is a different mechanism than classical chemical-reaction ased corrosion. The term A identi es the class of mechanisms y which a material can ecome degraded or dysfunctional
ecause of changes in its properties rought a out through processes resulting from interactions with su atomic or force carrying particles that affect the uilding locks of the atoms in the material. These processes are distinct from the traditional chemical cor-rosion processes of degradation considered y the DoD and include nuclear chemistry radiation effects and spontaneous decay. The common thread etween all of these A processes is that they impact individual atoms through non-chemical means.
ecause the properties of individual atoms do not characteri e most of the things that are important to us it is easy to think physical changes to an individual atom can have no impact on our daily lives. owever diseases like cancer remind us that when things degrade on the smallest scale the result can e serious. A cancer that egins in an individual cell degrades the nucleus of that cell which can spread to other cells which collectively degrade the tissue or organ which degrades the human eing that is made up of cells tissues and organs. undamentally the same effect can happen via A if for example a neutron collision alters an atom in a transistor within a microchip which degrades the surrounding material lattice which sets off a degradation cascade that impacts the functionality of the transistor the chip the computer and ultimately the en-tire system (e.g. weapon system . n oth examples the types of degradation descri ed here . Thus A is a out studying and understanding what makes atomic-level degradation of materials different than classical corrosion effects.
mage credit: Alex Taliesen
orrosion pectrum Arrow
1CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
This is not to say that the transistor descri ed a ove (and the chip/computer/weapon system of which it is a part cannot also undergo classical corrosion. f the transistor were placed in the ottom of the ocean it would degrade through classical corrosion processes. The designers of the transistor understand this and thus go to great lengths to control the environment around the transistor to ensure it will not e exposed to phe-nomena that can cause classical corrosion. They do not however design the transistor to e safe from atomic reactions and thus our transistor represents a material that while resistant to classical corrosion processes is suscepti le to A .
The goal of material sustainment should e to design materials so that all degradation processes are accounted for as est as possi le. DoD and society in general do not want to uild essential technology and infrastructures that are only protected from a fraction of the processes that can cause them to fail. t is therefore necessary to under-stand and make sense of all material degradation processes especially in cases where A (or other processes such as those caused y iological effects can ecome signi -cant. This is what the term corrosion spectrum is intended to convey.
The corrosion spectrum provides context to the uestion of what it means when we say a material has een degraded. t points out that classical corrosion is ust one type of degradation process that can cause systems and infrastructures to fail due to interaction with their environments which means that we need to understand the other mecha-nisms. n order to address corrosion in any part of the spectrum it is necessary to start y understanding the science of matter and how the ehaviors of materials are dependent on the properties of the individual atoms that make them up. ith a more complete understanding of the uilding locks of materials a discussion a out the properties of materials and the ways they can degrade incorporates not ust chemical reactions ut also the atomic molecular and larger-scale macromolecu-lar components that comprise materials. The corrosion spec-trum addresses all these mechanisms and in doing so the difference etween atomic effects classical and micro- or macro- iologically induced degradation ecome appar-ent. The goal is to ensure that the materials the DoD ac uires are capa le of withstanding all degradation pathways. To
egin understanding the corrosion spectrum let s start with the fundamentals: the science of matter.
the science of matter
tarting with fundamental particles such as uarks scale (physical si e increases from fundamental particles to atoms to simple molecules and ions to complex molecules and ions to macromolecules. As these uilding locks aggregate into micro and macrostruc-tures they can e further classi ed into four common material classi cations: metals ce-ramics polymers and composites. ith each type of classi cation we can thus descri e
The goal is to ensure that the
materials the DoD acquires are capable
of withstanding all degradation
ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
the mate-rial that results from the assem ly of these uilding
locks. Metals are large aggregates of me-tallic atoms held together into precise atomic geom-etries y special metallic onds and this gives rise to the properties we associate with metals. olymers are aggregations of car on- ased molecules held together through com-plex molecular onding schemes that lead to the molecular structures upon which poly-mer properties depend. Technologies such as a laptop computer incorporate many different uilding locks and it is the com ination of all the uilding locks working in concert that gives the laptop its functionality (see image a ove . A laptop depends on more than a single transistor to give it the capa il-ity of accessing the nternet.
CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
The laptop however still needs the individual transistors inside it to correctly execute their limited functions to e a le to perform its more complex functions. t may e a le to continue working if one transistor fails ut how many transistors need to fail efore the laptop is critically impaired xpanding from this example to the larger uestion the answer changes for different devices and different functions of a single device especially with more complex pieces of technology. This is key to understanding the corrosion spectrum.
4 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
nderstanding materials on a fundamental level ena les us to systematically investigate and understand the types of degradation pathways possi le throughout that material s lifetime. e will continue to have gaps in our material sustainment strategies if we fail to address the science of all degradation mechanisms associated with the materials we use to uild systems. This is why it is important to recogni e that chemical degradation also known as classical corrosion is only one of many degradation mechanisms. Many claim that the chemical/ionic mechanisms of degradation are well understood and we agree. hat is less well understood are the degradation mechanisms caused when su atomic particles smash into the atoms of a material (i.e. A : there is a lot of sci-ence that addresses individual mechanisms ut less recognition of how and when these degradation mechanisms reach the point where degradation matters to the materials we use. To lay the foundation for understanding the distinctions etween A and clas-sic corrosion we will rie y focus on the differences etween atom ions and molecules.1
The anatomy of the atom includes a central structure called the nucleus which is sur-rounded y electrons. hile an electron is a fundamental particle (it is indivisi le the nucleus is made up of protons and neutrons. These protons and neutrons are them-selves aggregations of other fundamental particles we call uarks. The nucleus of the atom is held together y the nuclear strong force (an attractive force etween nuclear particles which manifests from the ehaviors of uarks. The nuclear weak force (which allows uarks to transmute into other uarks which can change nuclear particles which can in turn reak up the nucleus resulting in radioactive decay also affects the e-havior of uarks and so it plays a role in A as well. More speci cally it plays a role in the spontaneous decay of atoms associated with radioactivity. rotons and electrons carry opposite electric charges ( y convention the proton is positively charged and the electron is negatively charged and the neutron carries no charge. The particle s electric charge interacts with electromagnetic forces and these interactions are critical to understanding how and why chemical reactions occur.
5CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
The anatomy of the atom includes a central structure called the nucleus which is sur-rounded y electrons (see the gure on page 4 . hile an electron is a fundamental particle (it is indivisi le the nucleus is made up of protons and neutrons. These pro-tons and neutrons are themselves aggregations of other fundamental particles we call
uarks. The nucleus of the atom is held together y the nuclear strong force (an attrac-tive force etween nuclear particles which manifests from the ehaviors of uarks. The nuclear weak force (which allows uarks to transmute into other uarks which can change nuclear particles which can in turn reak up the nucleus resulting in radioactive decay also affects the ehavior of uarks and so it plays a role in A as well. Protons and electrons carry opposite electric charges ( y convention the proton is positively charged and the electron is negatively charged and the neutron carries no charge. The particle s electric charge interacts with electromagnetic forces and these interac-tions are critical to understanding how and why chemical reactions occur.
An atom s properties depend on the num er of protons and neutrons in its nucleus (see the gure elow . An element is de ned y the num er of protons (and e ual num er of electrons an atom has and the various isotopes of a single element are distinguished
y changing the num er of neutrons in the atom. Deuterium for example is an isotope of hydrogen. maller lighter elements such as hydrogen ( and helium ( e have few protons and neutrons larger heavier atoms such as uranium ( have more protons and neutrons giving them a higher atomic weight. The neutron is necessary to overcome the repulsive forces ( like charges repel that occur as protons aggregate within the nucleus. To alance out the electromagnetic forces each atom has one electron for every proton. lements such as hydrogen helium or iron therefore represent a speci c sta le arrangement of protons neutrons and electrons.
The three isotopes of hydrogen
6 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
owever not all atoms are sta le for very long. arge atoms like uranium have isotopes such as uranium- 5 that can decay spontaneously through a process known as s-sion leading to a large release of energy and two new elements (Kr- and a-141 in this case that are more sta le. This phenomenon is what nuclear power and weapons depend on. Depending on the element and the associated isotope these con gura-tions can have varying half-lives (the time it takes for half of the atoms in a collection to come apart or decay into different more sta le isotopes . The reason for this phe-nomenon is that for elements with nuclei larger than iron the strong and weak nuclear forces egin to fail in their a ility to keep the nucleus together as more and more pro-tons aggregate into the nucleus. A contri uting factor is that elements larger than iron contain so many electrons that the nucleus struggles to keep them close to the atomic core. This reduces the inding effect of the electrons and thus adds to the desta ili ation of larger atoms.
nderstanding this factor is important ecause we have to e careful when general-i ing matter. t is incorrect to say that all atoms are sta le and will not degrade even the atoms of lighter elements. ome isotopes are very unsta le and exist for only fractions of seconds. ther isotopes are very sta le and take much longer (on average to de-grade. till others are so sta le that to date we have een una le to measure decay rates or determine half-lives for them. Then again we ve only een investigating atomic decay for a relatively short time. n sum when any atom degrades it is a conse uence of the same phenomena: the alance of strong weak and electromagnetic forces that hold a nucleus together is lost resulting in a repulsive force that e ects particles away from the atom. hether we have o served descri ed or understand it a pro a ility exists that any atom may decay.
The periodic ta le of elements descri es the con gurations of atoms. t provides a struc-tured asis for understanding the trends and ehaviors associated with atoms. The peri-odic ta le is arranged so that anyone who understands the asic properties that make up an element (atom can predict with some degree of certainty the ehavior of that element (see gure next page . This predicta ility is ased on an understanding of what changes when an atom adds an electron proton or neutron.
As one marches across the periodic ta le ( eginning in the top left corner the elements add more and more protons to their nuclei meaning they also have more and more electrons surrounding those nuclei. The electrons that surround the nucleus of an atom occupy special regions called or itals. ach or ital can contain a limited num er of electrons in it. There are four different types of or itals named P D and . The num er of electrons they can hold as well as their si es and shapes distinguishes them. As more electrons are added to an atom this increases the amounts of energy called energy levels that the electrons of an atom hold. lectrons will occupy energy levels of the same or ital until the or ital can no longer t any additional electrons. The next electron added to the atom then occupies a different or ital at the next highest energy level. The rows of the periodic ta le order the elements y the energy levels that re ect the most sta le regions for the electrons to arrange themselves around the atom. The sta le con gurations minimi e the repulsive forces of other electrons and maximi e attractive forces with the positive charge of the nucleus. The shape of the or itals descri es the lo-
7CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
cations and distances at which we expect to nd an electron most often (on average . The more electrons there are in an atom the more energy levels are involved and the higher-energy electrons are on average farther from the nucleus. Thus the reactivity (i.e. ehavior of an atom is re ected y the sta ility of the particular atomic arrange-ment of the atoms protons neutrons and electrons.
or an atom of a given element the highest energy level of the or ital and the last electron occupies determines its or ital. The electrons that occupy these outer or ital shells are called valence electrons. alence electrons are the most important electrons when it comes to chemical reactivity and thus classical corrosion events (e.g. ionic effects occur when su stances exchange possession of valence electrons. ven though atoms are electrically neutral when they have the same num er of electrons as protons they are more sta le when all of the valence energy levels are full. The forces keeping valence electrons attached to an atom are small enough that they can leave an electromagnetically alanced atom to occupy another atom that has a more favor-a le empty valence energy level. The principles ehind this are descri ed y thermo-dynamics and uantum mechanics. r itals that don t have any empty energy levels are said to e fully occupied and the electrons within those or itals called core electrons do not participate in any chemical reactions: the reason the no le gases are so non-reactive is ecause their outer electron shells are full. The trends on the pe-riodic ta le are a re ection of the desire for atoms to o tain the most sta le electron con guration. Thus understanding what controls the ehavior of valence electrons is critical to understanding the ehavior of atoms molecules and as we scale up materials.
Diagram of the arious Periodic Trends.
8 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
hen an atom either gains or loses an electron its charge ecomes im alanced and we call it an ion. The relative tendency for an atom to take on an extra electron can e calculated as electronegativity. The closer an atom is to having its valence electron shell full the more electronegative that atom is ecause o taining an extra electron puts it one electron closer to a more sta le con guration. Additionally the smaller an atom is the more electronegative it is ecause smaller atoms have a stronger nuclear pull on their electrons. f two atoms are close to each other and an electron is placed in e-tween them the one that is more electronegative will tend to capture that free electron.
f all the trends the periodic ta le helps us understand the trend of electronegativity is the most important when it comes to understanding chemical reactivity.
ons tend to form when elements dissolve in a solvent. The most common solvent is water for example when common ta le salt (Na l is added to water the Na (sodium and l (chlorine tend to separate into positive and negative ions respectively. The rea-son that common ta le salt dissolves in water into ions (sodium ion Na and chlorine ion
1. Sodium, which has one extraelectron from an ideal energycon guration, collides with chlorine,which needs one more electron tohave an ideal energy con guration.
2. Upon collision, the sodium atom begins to share its extra electronwith the chlorine atom.
3. If dissolved in an aqueous solution,the sodium gives up its extra electron to the chlorine atom, formingsodium (+) and chlorine (-) ions.
orming and dissolving of table salt
Image credit: Alex Taliesen
3CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
l-) is because the loss of an electron from sodium gives it the electron con guration of a noble gas and the gain of an electron from chlorine gives it the electron con guration of a noble gas. y splitting as they do, ions ll their valence shells. Understanding this trend explains why we see the presence of certain stable ions. The difference between ions and noble gas atoms is that ions have unbalanced charge which makes ions more chemically reactive than noble gases. All simple ions that exist in nature are a re ection of the general trends we see on the periodic table, and re ect a more stable arrange-ment of their electrons than existed when the atom was neutral.
The gure on page 38 describes what happens when sodium and chlorine combine to form table salt (middle picture in the gure). The bottom picture shows what happens when table salt dissolves in water: the sodium separates from the chlorine, but in the process leaves an electron with the chlorine. oth ions now have more stable electron con gurations and as long as the water molecules keep them suf ciently separated, they do not recombine. If the water evaporates, the positive and negative ions will be attracted to each other and reform table salt.4
The term oxidation describes the process of an atom/ion giving up an electron to an atom of higher electronegativity (typically oxygen) and is a common process that oc-curs in various metals. ust as with ioni ation in general, a metal oxidi es because the metal s valence electrons are more stable on the atoms of the oxidi ing agent. The atom that gains the electron, in most cases oxygen, is said to undergo reduction (see gure page 4 ). hen iron reacts with oxygen, iron oxide ( e 2), commonly known as rust, forms. At the molecular level, e 2 is more stable but at the macroscopic level on which we experience it rust is annoying.
Molecules are slightly larger in scale than atoms and consist of two or more atoms locked into a particular geometry through electrostatic interactions. The forces that hold these atoms into their geometries are called bonds and these bonds give molecules their struc-ture. The structures of molecules help give rise to new properties that individual atoms do not possess.
onds, like orbitals, come in different, unique types. As stated before, all bonds are elec-trostatic in nature and represent an interaction between two atoms. No matter what type, a bond exists because the two atoms involved experience an attractive force based on charge separation5 (a phenomenon commonly observed in static electric-ity ). These charge separations can be transient or permanent.
The ionic bond is the strongest type of bond. These bonds occur when ions exist in close enough proximity to become strongly attracted to each other (i.e., form a bond).
ovalent bonds are strong, but weaker than ionic bonds, and involve the sharing of electrons between two atoms. These bonds occur between two atoms that have similar
4. . . 3
. .5. .
4 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
electronegativity properties and the sharing of electrons allows them to feel like they have lled their valence shells. Metallic bonds are weaker than both ionic and covalent bonds and involve the delocali ation of electrons among many metallic atoms aggre-gated together. There are also secondary bonds, such as dipole or van der alls inter-actions, that involve transient changes in a molecule s or atom s charge polarity. These are much weaker than ionic, covalent, or metallic bonds, but collectively can have a tremendous in uence on a material s structure and properties.
The properties of bonds are the basis for chemical reactions. These reactions are, for the most part, well understood. Depending on the particular electronegativity proper-ties of an atom it will tend to engage other atoms, ions, or molecules through ionic, covalent, metallic or other secondary bonding schemes. lassical corrosion is focused on understanding why atoms, ions, and molecules exchange electrons to form new
bonds and take on new structures. Although the atoms in-volved in chemical reactions become more stable, these reactions lead to changes in the atomic or molecular ge-ometries. The properties of a particular material depend on the atomic and molecular structures that make it up. Ac-cordingly, chemical reactions that change these structures are degradation events that lead to changes in the materi-al s properties. hen iron is exposed to water it loses some of its valence electrons to oxygen. This forces iron to stop bonding with the other iron atoms around it and this of
course effects the structure of the other iron atoms. Thus, while the formation of iron oxide (i.e., rust) might be more stable, it weakens the iron metal because it causes degradation of the underlying metallic structure. This is why classical corrosion is con-cerned mainly with the chemical reactions of ions and molecular level effects. ith a basic understanding of atoms, ions and molecules as a basis, let s move on to the various roles they play in materials degradation.
Classical corrosion is focused on understanding why atoms, ions, and molecules exchange electrons to form new bonds and take on new structures.
xidation and eduction/Alex Taliesen
41CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
the science of degradation
Moving from a summary of the foundational concepts of atoms and chemistry, we need to examine the speci c processes that cause degradation. It is clear that there are ma-terials that degrade through mechanisms different than those traditionally associated with classical chemical corrosion. In this section, we categori e the different processes that can disrupt the properties of materials, resulting in degradation via chemical and non-chemical reaction mechanisms. These categories include low-energy collisions, high-energy collisions, the effects of eld forces, and spontaneous degradation, also known as radioactive decay.
Traditional chemical (classical) cor-rosion is caused by what we call low-energy collisions. These colli-sions are the common chemical re-actions that occur between atoms, ions, and molecules (see the gure to the right). xidation-reduction reactions occur because atoms and molecules collide with enough energy to exchange electrons, but not with enough energy to alter their nuclear properties. Additionally, lower-energy light photons, such as those in the visible or infrared spectra, can play a role in these chemical reactions. Photons can also collide with matter, but these interactions only have enough energy to excite valence electrons to a higher energy state. The collisions do not transfer enough energy to e ect a valence electron. owever, when these electrons occupy a higher energy level, the atom itself is inherently less stable and is thus potentially more reactive. ow-energy col-lisions cause atoms, ions, or molecules to exchange electrons.
As stated, low-energy collisions are the primary mechanism of classical corrosion. e de-scribe it here only to provide a context for addressing the differences between classical corrosion and A . A occurs due to high-energy collisions, eld forces, and spontane-ous decay all of which act on an atom s nucleus (the nuclear level).
hen matter travels at extremely high velocities and collides with other matter, it can cause changes to the nuclear properties of that matter. Due to the high energy associ-ated with these collisions, the participating particles can overcome the electronic repul-sive forces caused when the electron clouds get too close, and thus penetrate to the nucleus of an atom. This is the fundamental difference between nuclear and chemical reactions: nuclear reactions involve smashing into the nucleus and chemical reactions involve smashing into electron orbitals. hen an event result causes changes to the nucleus of an atom in a material, we call it atomic effects corrosion (A ). Subatomic
42 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
particles, such as a proton or neutron, can be e ected from the nucleus of an atom when a gamma photon (light packet) carrying large amounts of energy collides with the atom. In its extreme form, mechanisms such as this lead to what is referred to as splitting the atom. ast neutrons
or other particulate radiation, such as that found in a cosmic ray, can smash into the atoms of a material like a bowling ball wrecking pins (see gure to the right). These high-energy
collisions often cause changes to the atomic properties of atoms within a material, as well as forcibly displac-ing them from their previous location within a material s atomic or molecular structure. These are the degradation events we typically associate with A . igh-energy collisions that destroy chemical bonds and/or cause the e ection of valence electrons from atoms (i.e., another mechanism for ioni a-tion) are more associated with classical corrosion as these are essentially changes in the electronic con gurations of atoms.
In addition to interactions with par-ticles, atoms, and photons, there are environments that can produce strong electromagnetic elds (i.e., force particles) that can attract or repel matter in ways to cause serious damage to the structure and proper-ties of a material. There are natural and arti cial sources of these strong electromagnetic elds. Arti cial sources arise from a wide range of phenomena (see gure to the right), from small electromagnetic elds around power lines and within elec-tronics that cause electromigration, to large elds like those produced in medical instruments such as nuclear magnetic resonance imagers (M I). Such large elds can cause changes in atomic con gurations at the nuclear and electron shell
levels. ield forces, therefore, can both cause A and in uence the rate at which clas-sical corrosion occurs.
MS: Simulated iggs to two ets and two electrons. Image creator : ucas Taylor N
43CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
Spontaneous degradation oc-curs when an unstable nucleus decays and emits radiation in most cases, at the same time its nucleus splits into two or more smaller atomic nuclei. Sponta-neous degradation is a stochas-tic, or random process in the sense that we cannot predict when a particular atom is go-ing to decay. The most familiar type of spontaneous degrada-tion process is radioactive de-cay. Spontaneous degradation processes are a consequence of the second law of thermo-dynamics, which describes the process known as entropy. The concept of entropy describes the natural tendency of matter to fall apart, resulting in more disorder in the universe. It is a misconception that only radioactive atoms and molecules are susceptible to spontaneous decay. Any atom within a material can fall apart, and thus any mate-rial can degrade in this way at any moment in time. or most non-radioactive atoms, however, spontaneous degradation is such a low-probability event that at it has no real effect on the macroscopic scale. Aside from atoms falling apart, atomic and molecular structures can degrade due to entropy caused by phenomena like diffusion. ntropy guarantees that anything with order, be it an atom or a tank, has a chance to sponta-neously lose that order.
Degradation Mechanisms: Summary
In summary, the four broad categories that describe the various mechanisms by which materials can degrade are summari ed as follows.
• Chemical reactions
• xidation- eduction
• lectron excitation
• Particulate radiation
• lectromagnetic radiation
• adioactive decay
• Spontaneous bond breaks
• lectromagnetic elds
• ravitational elds
A hypothetical nucleus which can undergo many forms of radioactive decay/Kieran Maher
44 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
f these categories, classical corrosion studies only address speci c types of low-energy collisions, such as those associated with oxidation-reduction reactions, and some associ-ated with eld forces (e.g., electromigration) and spontaneous decay (e.g., electron dif-fusion). hat is clear is that there are other phenomena and processes that can cause materials to degrade. hat is less well known is: when is it important, and what can we do to prevent it from causing unwanted degradation
To highlight the importance of these distinctions among types of degradation, let s return to the dilemma associated with microchips described above: manufacturing micro-chips. e are developing microchips with increasing numbers of nanometer-si ed com-ponents, yet we counter that advantage by having to design redundancies into those chips. e an un er an e e i me ani m e ra a i n an eir im li a-i n n m ern em en a e n l a an e e ma e a le er me
eir e e an n l n er nee re r uil in in numer u re un an ie . This is the motivation behind addressing A C as a degradation/corrosion mechanism and it is why this non-classical degradation phenomenology is important to understand so as to overcome materials degradation and promote improved material sustainment policies.
Many materials that are involved in discussions of classical corrosion do not fall into the A C category because most materials function depends on an atomic/molecular structure composed of an astronomical number of atoms. A change in one atom s atomic properties is not going to impact the overall functionality of the material. et, as technology advances, A C is likely to become more important in materials where a few A C events degrade the material. Now, let s address the different types of A C and their potential impacts.
atomic effects corrosion implications
In the remainder of this chapter, we move beyond the scienti c description into the practical considerations of A C impacts on and their importance to a variety of DoD and other systems. e do not mean to suggest in this section that any part of the spectrum of corrosion/degradation has been neglected. Indeed, much physics and chemistry research in the area of atomic effects corrosion has been completed. ow-ever, A C and other corrosion mechanisms have, to date, been largely separated into different elds, with little collaboration or cross-fertili ation. e argue that there are rea-sons to increase collaboration in the scienti c investigation of materials degradation and
material sustainment. urther, we argue that even if the mechanisms and effects are not causing signi cant problems today, it is likely that (a) their importance will increase in the future as technology develops, and (b) identifying new ways to prevent materials degradation offers opportunities to develop more reliable, longer life systems. Chapter 3 provides recommendations in the areas of DoD interests, and the associated research ar-eas, along with policy and strategy development. et us now continue with the importance of A C.
If we can understand the speci c mechanisms of degradation and their implications on modern systems, then as technology advances, we may be able to overcome their effects and no longer need to resort to building in numerous redundancies.
45CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
the increasing importance of aec
As technology and applications develop, speciali ed systems will operate in new envi-ronments, and consequently new material sustainment requirements will be identi ed. y anticipating problems that could emerge in the future, we can avoid being reactive to materials degradation problems, and instead design new applications beforehand, with the supporting science and policy associated with material sustainment capabilities. The emerging A C issues arise in part due to the scale at which systems are constructed.
hile classical corrosion science focuses on the transfer of ions and electrons and the associated chemistry that affects materials at the molecular level, radiation and nuclear effects cause degradation from atoms emitting subatomic particles or radiation. These atomic effects are in the realm of nuclear physics. As a result, as our systems become more sophisticated, atomic effects cause various problems within varying environments.
hen (not if) the atomic effects start affecting the functionality of our systems, we will need to nd different solutions not solely based on classical corrosion chemistry. e ex-pect impacts in the areas of microelectronics, nuclear weapons, nuclear waste storage, materials in radioactive environments, and materials in space.
In microelectronics, as spacing or feature si es between processors or components get smaller (see gure below), the effects of quantum events and other atomic processes become more impactful, and the consequences of even single events might have long-term effects on system reliabilities. The impact of cumulative nuclear effects has not been the sub ect of prominent microelectronics research because to date, it has not yet resulted in noticeably harmful degradation. This will soon no longer be the case.
Comparison of si es of semiconductor
manufacturing process nodes with some microscopic
ob ects and visible light wavelengths/Cmglee
46 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
A great deal of research has been performed on single event effects (S s), which can cause microelectronics to experience a temporary change that causes a digital error, or permanent changes that can damage circuit components. As of 2 15, microelectronic feature si es will soon descend to single digit nanometer ranges. ield densities will also increase, which means that A C is likely to become important in microprocessors and sensor systems in the very near future.
The eld of modeling microelectronics reliability is well established, and has progressed from empirical models to physics-based analysis of component reliabilities.6,7 Some of the principle effects modeled that lead to microelectronic degradation include electromi-gration, hot carrier in ection, lattice degradation, dielectric breakdown, and negative
bias temperature instability (see appendix 1 for more detailed descriptions of some of these effects). hile these models take into account some basic quantum effects, they are based on a macroscopic perspective and do not necessarily scale down to feature si es that are only a few tens of atoms in width. Many challenges remain, including improving modeling and valida-tion of atomic-level effects, and accounting for the dependen-cies of voltage and temperature.
Microelectronics is the main forum where we currently encounter nanotechnology ( nanotech ). The future will bring nanotech robots, structural materials involving nano-tech, nanosensors, and nanobiologics. The effects of degradation of individual atoms due to A C will become important in these and other, as yet unforeseen, areas.
Atomic effects corrosion is already an important consideration to the U.S. nuclear stock-pile. As our nuclear weapons age, it becomes a graver issue, in terms of the costs for maintenance and the eventual need for new designs. urthermore, our nation does not currently test nuclear weapons, so a new design would have to be deemed reliable, and monitored, through virtual validation (i.e., by science based modeling instead of
direct empirical testing). ithout testing, we cannot col-lect new empirical data, meaning it is increasingly impor-tant to understand the science in depth in order to build adequate validation models. Accordingly, a detailed un-derstanding of the degradation processes, including those due to nuclear effects in proximity to various radioactive elements, is critical.
6. . . . .
14 4 1 1 5. .. 5 14 14
. 5 .
Microelectronics is the main forum where we currently encounter nanotechnology (“nanotech”).
As our nuclear weapons age, AEC becomes a graver issue, in terms of the costs for maintenance and the eventual need for new designs.
47CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
The medium and long-term storage of radioactive waste also continues to be a national issue. Although the topic has been heavily studied, there is still no consensus on the best policy for long-term disposition of such materials. hether from new weapons programs or new atomic energy production plants, the long-term storage of waste, and the ef-fects of waste material and the containers that store them degrading over time, remain important questions for both DoD and society.
adioactivity and nuclear events pose degradation ha ards in nuclear power plants. or example, control electronics must be protected from radiation in nuclear power plants. ailure to do so could result in sensor failures and in ability to properly characteri e and
respond to nuclear reactor changes in states. adiolysis of water is also a serious concern for nuclear plants. adiolysis is the dissociation of molecules a chemical process caused by nuclear radiation. The radiation basically breaks chemical bonds in molecules, separating them into chemically reactive pieces that readily react with their sur-roundings. This is an example of a process caused by A C that results in classical corrosion. A coordinated research program focused on both nuclear physics and chemistry may offer im-proved solutions to this compound degradation process.
inally, activities in outer space expose systems (and humans) to radiation and environ-ments that are outside of the shielding protection of our planet s magnetic eld and atmosphere. Interest in mining asteroids and exploiting other celestial bodies for re-sources will almost certainly lead to expanding our use of orbital assets for bene ts on arth. e have a lot of experience with assets in space, however, degradation pro-
cesses in systems and people in space will become more signi cant as our use of space expands and as the microelectronics and other systems that are sent into space be-come more miniaturi ed.
hile the areas of concern for A C may seem esoteric, these are areas of interest for the DoD, and in the future they are likely to be more impactful in terms of cost and national needs. hether addressing the lifespan of microelectron-ics, the reliability of our nuclear deterrent, or the longevity of power plants fueled by nuclear materials, it is in our national interests to do the research, develop the science and thus have the knowledge and means to prevent and/or mitigate degradation by A C mechanisms.
A coordinated research program
may offer improved solutions
to compound degradation.
... it is in our national interests to do the research, develop
the science and thus have the knowledge
and means to prevent and/or mitigate degradation by
48 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
current research in aec fields
There is a large and vibrant research enterprise in various speci c aspects of A C, and some of that research is classi ed. urthermore, the research in this area is largely separate from other branches of corrosion and degradation research. This section surveys what is known about A C, based on current and ongoing research, at the unclassi ed level.
1 eliability of weapons due to materials degradation in nuclear environments.
2 Medium and long-term containment of nuclear waste materials from nuclear power plants and from weapons development.
3 Degradation of components in current and future nuclear power plant environments.
4 Degradation of materials in outer space intended for long service lives.
hile various organi ations are addressing traditional corrosion issues, we propose that there is a need to develop a coordinated, collaborative research environment to ad-dress the multidimensional issues associated with A C, as well as A C leading to classical corrosion. The goal of the coordinated research program we recommend in the next chapter is to ensure that the eld of material sustainment is proactive in responding to advancing technology and its application in different environments, as opposed to re-acting to failures and sustainment surprises that show up as effects become more serious.
Nuclear weapon systems, a crucial piece of U.S. national defense, are among the most complex systems devised by mankind. Creating fusion and ssion reactions are simple, compared to the task of creating systems that constitute safe and reliable weapons that can be secured and maintained for years. All modern nuclear weapons include com-plex microelectronics systems, other materials, and radioactive elements that change over time. All of these components are sub ect to degradation, and thus require main-tenance. The weapons in the U.S. nuclear stockpile were designed for 2 to 25 year life spans but some are now over 4 years old.
. . . . 3 . .
4CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
The Do Stockpile Stewardship Program is executed primarily by the D National ab-oratories and administered by the National Nuclear Security Administration (NNSA).1 . The purpose of the program is to understand and analy e the reliability of the nuclear stockpile, and to ensure said reliability through analysis and experiments. The program was developed in response to the 1 2 decision that the United States would cease all nuclear detonations, including underground nuclear testing. The NNSA Stockpile Stew-ardship program includes the ife xtension Programs ( P) for inspecting, recondition-ing, and maintain our nuclear stockpile. Independent review of these efforts is conduct-ed regularly for example, the AS Ns (a scienti c advisory group named after ason, the Argonaut of reek mythology) regularly review components of the P for technical and policy soundness.11 The science that has been developed to understand stockpile degradation is extensive and complex. The scientists performing these analyses are ded-icated to achieving the stewardship and maintenance of viability, and to understanding in detail the modalities that cause degradations.
• There have been open reports of defects and degradation within nuclear weapons on several instances throughout their history.
• Tritium triggers must be replaced regularly, but the United States ceased production of tritium in 1 88.12 Since then, replacements have been made with recycled tritium.13
• In addition to nuclear decay, nuclear pits (the ssile material) can corrode. Plutonium pits degrade when exposed to humidity, and other materials and alloys employed in the ssile pit are sub ect to normal corrosion.
• adioactive materials can cataly e the corrosion of surrounding materials.
• The corrosion of core material can result in the deformation of the nuclear pit, which can rupture the storage container.
• adiation from the ssile material within the device can cause damage to surrounding components.
• Microelectronics in devices with nuclear material can degrade due to the highly radioactive environment.
1 . 1 15. . .
11. 61 1 . 61 . .
1 . . 3 .
5 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The interactions of radiation with matter are heavily researched. ven so, important questions remain. or example, how con dent are we in our modeling capabilities As-sessing con dence levels based on failure trends requires scienti c understanding of the state of analysis, but in areas where the science is not fully developed, this assessment can also involve udgments based on the expertise of directors and executives in the convoluted and dif cult area of weapons stewardship.
nuclear power facilities
Nuclear reactors (see gure below) consist of relatively few components: reactor core, control rods, heat transport system and nuclear fuel, almost all of which undergo serious degradation due to A C.14 The intensity and forms of radiation depend on the fuel type, moderators, and materials used for transporting the thermal energy out of the reactor core. Most nuclear power plants currently use enriched uranium. Some plants also use plutonium, and the interest in developing thorium plants is increasing.
oiling water reactor system diagram/Image credit: obert Steffens
The main degradation processes induced by radiation in a nuclear power plant involve stress corrosion cracking and corrosion byproduct buildup.15 Some of these processes are well understood, having received research attention for many years, particularly due to the known increased likelihood of corrosion in the aqueous (meaning water contain-ing ) environments.16 igh temperatures and pressures exacerbate the development of
14. 11 .15. 46.16. 11
1 15 . . . .
51CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
corrosion. owever, the corrosive effect of decay byproducts is a complex issue that is not as well understood. The radioactive decay of the fuel results in the degradation of metals and materials in the vicinity of the core.17 The nature of a material itself may be altered by exposure to radioactivity.18 Research on the impact of radiation on the met-als comprising the heat transport systems in nuclear power plants, in particular in light water reactors with an aqueous environment,1 has determined that nuclear activity not only impacts the rate of corrosion, but also the deposition of byproducts on the metal surfaces and these byproducts must be removed. 2
Thorium fueled reactors have been touted as cleaner, safer reactors. They may become more prevalent in the future, but as thorium reactors come on line, the ways in which they cause corrosion will need to be studied to determine and overcome the effects.
The corrosion rate of components in a nuclear power plant generally increases with dosage of radiation, but other conditions such as temperature and concentration of oxygen also impact the problem.21 Corrosion from ioni ing radiation, for example, is en-hanced by elevated temperatures as well as other factors.22 Stress corrosion cracking is a particular concern due to the physical pressures that the surrounding materials place on the pipes and containers. The impact of radiation on carbon and stainless steel has been studied for decades, and when exposed to even a small amount of water, corrosion is accelerated by radiation due to radiolysis.
Degradation processes also affect the microelectronics in a nuclear power plant, which must be able to withstand continuous exposure to a relatively highly radiation environ-ment. The functionality of microelectronic controls is also critical in the event of a melt-down, and so they must also be able to withstand the potentially extreme amounts of radiation such a scenario entails. As a result, the microelectronics within current nuclear power plants are hardened against radiation and in some cases, able to survive levels of radiation hundreds of thousands of times greater than what a human can survive.23 Due to the additional engineering demands, radiation hardened devices are often two to four generations behind commercial electronics. As commercial designs advance, even if power plant microelectronics are generations behind, we need to understand the effects of A C on the increasingly sophisticated microelectronics that will be used in future power plants.
1 . . . 1 . 11 1 1 1 4 .
1 . . . . . 15
11 4.1 . . .
1 . . . . 4 4 . .
11 1 15 . .1
1 11 . .1.
1 .. .
3. 1 1 11 1 15 . .
52 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
nuclear waste disposal
The nuclear enterprise consists of nuclear power plants and suppliers to those plants, nuclear weapons manufacture and maintenance, and research reactors and suppli-ers of nuclear materials for medicines and other applications. ach of these sources produces waste products (see gure above) that require handling and disposal. urther-more, each source has previously produced waste that is in short or intermediate term storage awaiting longer-term solutions.
Nuclear power facilities produce three types of waste: high-level waste, mill tailings and low-level waste. This waste is currently stored in water pools at nuclear facilities or in tem-porary dry surface storage.24 Some of this fuel has been in storage as long as 3 years, yet a permanent long-term storage site has not been identi ed.25
The waste from nuclear weapons development has been accumulating for decades. More than a hundred sites around the country contain waste products that will need even-tual disposal. urthermore, facilities are needed to cleanse contaminated groundwater.
Much of the study of nuclear waste storage degradation has focused on the impact of ioni ing radiation on metals in an effort to nd a safe and effective way to store and dis-
4. . . .4 15 . . 153 3 6. .
5. . 1314 15 . . 13 6
NucNucNucucNuNNN leaealealear Wr Wr Wr WWaastaa e Barra els/ Fliclicckr/kr/kk IwaIwaan Gn Gn GGaboaaboboa vitvitvitvv chchhc
53CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
pose of nuclear waste long-term. As we have noted, there are a variety of waste types, including spent fuel from nuclear power plants, and the byproducts of both power plants and nuclear weapons factories. Spent nuclear fuel and its byproducts can be reprocessed to recover unspent fuel, or to develop new material from certain radioac-tive waste products such as plutonium. Reprocessing reduces the volume of waste, but nevertheless leaves residual waste that must be handled. Similarly, waste from nuclear weapons development and production includes materials from the enrichment of ura-nium or the production of plutonium, with large volumes of intermediate products and contaminated materials.
Although long-term storage of nuclear waste has been studied for decades, there is more to learn about the medium and long-term viability of materials for storage of spe-ci c radioactive materials. itri cation (embedding the material in glass) to allow for safe storage for thousands of years is one long-term solution being considered.26 ong-term proposals carry certain risks, which have also been studied.27 The science suggests that there is a high level of con dence in the technology for containing the radioactivity of the waste for the time necessary to reduce it to safe levels. Containment of harmful chemicals, however, is less certain for the thousands of years that might be required. This is another example of A C coupled with classical corrosion, and another impetus for a coordinated research program.
• Sites, designs, and licenses, to begin operations of a pilot interim storage facility by 2 21 with an initial focus on accepting used nuclear fuel from reactor sites that have been shut down
• Advances toward the siting and licensing of a larger interim storage facility to be available by 2 25 that will have suf cient capacity to provide exibility in the waste management system and allows for acceptance of enough used nuclear fuel to reduce expected government liabilities and
• Demonstrable progress on the siting and characteri ation of repository sites to facilitate the availability of a geologic repository by 2 48.
While comprehensive and well thought out, the plan depends upon appropriate autho-ri ations from Congress before it can be implemented.2
Understanding the role A C plays in the degradation of storage containers for radioac-tive waste will lead to better reliability in the strategies implemented to deal with the
6. 1 14 . . . .
. 14 15 . . 5 5 5 3
5 . ..
13 . 13 1 15 . .. .
54 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
increasing amounts of nuclear waste produced by all U.S. nuclear activities. Designing nuclear waste containers that are resistant to A C and other types of corrosion is need-ed to ensure safer long term storage and transport of these materials from the sources that generate them to the storage facilities.
The region of the atmosphere from approximately 5 km above the earth s surface to the edges of outer space experiences much more radiation than regions beyond it (see gure below). This volume includes trapped particles within the an Allen belts, which
are regions of intensely charged particles and radiation that collect in the earth s mag-netic elds. Further out, solar winds, consisting of charged and other energetic particles that ow continuously from the sun, contribute to increased radiation (see the gure on page 55). Galactic cosmic rays contribute additional particles and radiation.3 Dr. de Rooi , head of Materials Technolo-gy Section at the uropean Space Agency, notes that materials in space are sub ect to atomic oxygen, ultraviolet (U ) radiation, ioni ing radiation, ultrahigh vac-uum (U ), charged particles, thermal cycles, electromagnetic radiation, micrometeoroids, and man-made orbital debris. 31
Materials sub ected to outer space also must be able to with-stand extreme temperature and pressure uctuations. The impact of these extremes is further ex-acerbated upon exiting and reentering arth s atmosphere, where spacecraft are moving fast enough to generate extreme heat from friction with the atmo-sphere. Due to synergistic or separate interactions in this envi-
3 . 1 15 . . 4 11
. .31. .
31 15 . . . .
55CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
ronment, the spacecraft materials might suffer corrosion, erosion, structure modi cation and surface roughening. 32 These effects can degrade their optical, thermal, electrical and mechanical properties.33
The effects on humans that go into space can also be considered a degradation prob-lem. A human in space for 1 days experiences about the same amount of radiation as human on arth does in 1 years. arious radiation-hardening technologies have been implemented in order to shield both the astronauts and the components of the space-ship from radiation, but none of these completely eliminate the increased dosages hu-mans receive in space.
Whether it is humans or spacecraft components, solutions to retard degradation are needed. umans have been in space for decades and have developed materials, such as polyethylene shielding,34 that work well at protecting astronauts from high-speed neu-trons. Cosmic rays, however, have extremely high energies, and cannot be stopped by any reasonable amount of physical shielding.35 ther shielding materials such as alu-minum sheeting can solve one problem while exacerbating another: the sheeting is in place to de ect primary radiation36 but produces secondary radiation in the process.
3 . .33. .34.
1 14 . . 13 3. .
35. 5 5 15 . . 5 5
.36. 11 11
15 . . 11 11.
Sources of Ioni ing Radiation in Interplanetary Space/Image credit: NASA/ P -Caltech/SwRI
56 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The impact of the irradiative environment on surface materials is particularly important to mitigate degradation to solar cells, which are used to power most systems in space. Photovoltaics (P ) are typically composed of crystalline structures.37 These structures are coated with substances designed to maintain their integrity.38 owever, as the environ-ment degrades this coating, the ef ciency of the solar cell is reduced over time. ther atomic effects on the components also degrade the photovoltaic ef ciency over long periods in space. These effects may become even more important in the future if we move forward with space based solar power systems.3
In space, a material s tolerance of the wide breadth of temperatures and physical forces it will experience must be considered as well as its ability to withstand cosmic rays, solar wind, and radiation belts.4 For example, the surface temperature of the International Space Station (ISS) can increase by up to 5 degrees when passing from the earth s shadow into the sun as it orbits the earth.41 Within spacecraft, heat can accumulate for example, both the humans and equipment within the ISS produce heat. If there is insuf-cient air to serve as a medium for the transport and circulation of heat, temperatures
could rise enough to cause a dangerous environment for the sensitive electronic equip-ment on board.
Another classical corrosion mechanism in space, as mentioned at the beginning of this section is atomic oxygen (AT ). xygen usually occurs as pairs of atoms, which is a highly stable molecule, but AT , an unpaired oxygen atom, is highly reactive and read-ily bonds with a wide range of elements and compounds. Corrosion is most likely to oc-cur to surface coatings of spacecraft at altitudes where AT is concentrated: between 2 and 7 km above the earth.42 Because AT occurs in some of the same regions as the an Allen belts and solar wind, both A C and classical corrosion, and coupled effects between the two types of mechanisms, can and do occur.
aec in microelectronics
We now turn to an area in which A C is expected to become more signi cant in the fu-ture, whether in the harsh environments of nuclear systems and space, or simply in the milder, yet far from radiation free, environment of terrestrial arth. In the
, author Robert Baumann discusses the ef-fects of Terrestrial Radiation on Integrated Circuits. 43 Similarly, -
3 . 11. 15 . . . 11 3. .
3 . 3 13 3 15 . . 13 .
3 . 6 14 1 15 ..
4 . . 1
41. 14 15 . . .
4 . . . .. .
43. . 31.
57CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
teraction in Matter and Detection covers “radiation environments and damage in siliconsemiconductors” and “displacement damage and particle interactions in silicondevices.”44 These and other works have detailed analyses of the effects of radiation on microelectronics. The impact of radioactivity in any environment can lead to errors and also the degradation of semiconductors over time. These references speci cally discuss AEC on older microelectronics with feature sizes in the range of 45-90 nm, 4 to 10 timesas large as the state-of-the-art microchips being developed today.45 In the near future,node sizes are expected to decrease even further to single-digit nm feature sizes. As more sophisticated designs are developed, the issues described in these two works andrelated analyses are likely to become more pressing.
As feature sizes decrease, and consequently component densities on microchips increase, these mechanisms are likelyto become much more important. In this section, we brie ydiscuss the mechanisms by which AEC can affect micro-electronics (see gure page 58). In this section, we merely introduce the mechanisms. The mechanisms are well docu-mented, and the reader interested in a greater level of detail can nd detailed descriptions of some of these mechanismsin appendix 1, a speci c example of an AEC mechanism degrading microelectronics in appendix 2, or for a broader description to any of the available textbooks (such as the twocited in the paragraph above). The issues that remain to bedetermined include the effects of these mechanisms on mi-croelectronics as feature sizes decrease, and whether or not this will bring about new mechanisms.
Single Event Effects
The primary concern with radiation effects on microelectronics currently relates to “singleevent effects” (SEEs). There are several types of SEEs, which include single-event upsets(SEUs), “single event latchups” (SE ), “single event burnouts” (SEB), each of which webrie y explain below.
A SEU occurs when a bit within the microcircuit is changed from its correct value. In a memory chip, this can change the stored data. Multi-bit upsets are also possible, where-in a set of bits are changed, but the term simply describes multiple SEUs. For the mostpart, SEUs are “soft errors,” also known as single event transients (SETs), meaning that the damage is limited to the data error, and that any permanent damage is insigni cant and inconsequential.
It is, however, possible for a SEE to cause a “hard error,” wherein some part of the micro-circuit is permanently damaged. A “single event latchup” (SE ) can, in some instances,
44. Claude Leroy and Pier-Giorgio Rancoita, (Singapore: orld Scien c Pu li ing Co., .
45. Re erence to S i e no .
As feature sizesdecrease, andconsequently
component densities on
degradationmechanisms are likely to
become much more important.
58 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
particular component. Even more detrimental is a “single event burnout” (SEB), whichcan destroy a device due to a high current in a power transistor causing the device tofail permanently.
SEEs are becoming more signi cant as geometries continue to get smaller.46 A change tothe stored bit stream that programs a eld programmable gate array (FPGA: a program-mable microchip) can cause a program error, which can result in a failure to functionupon execution. The bottom line is, whether soft or hard errors, radiation-caused events cause degradation of the microelectronic device that goes beyond simple data errorsto device destruction.
Most of the consequences of single-event effects are due to ionization tracks fromcharged particles that are emitted due to a nuclear event within the chip. External radiation instigates these events. SEEs are typically instigated by an AEC mechanism
46. “Neutron-Induced Single Event Upset (SEU) FAQ,” Microsemi, August 11, Accessed 31 Aug 15, p: .icrose i.co docu ent-portal doc vie 13 6 -neutron-seu- a .
59CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
called linear energy transfer (LET), which is separated into two categories according to how much energy is deposited in a material: “high-LET” or “low-LET.” In either case, energy is transferred during the AEC event to create a shower of ion charges deposited into the microelectronics material, creating “electron-hole pairs.” In this formation, anelectron is ejected from a valence orbital. When this occurs, a positively charged ion, aptly named a “hole,” is left behind. Generally, the electrons are much smaller thanthus more mobile than the holes and thus the electrons can move more freely through the circuit. Both high- and low-LET events cause more or more frequent problems as gate sizes become smaller.
SEEs can also cause “FITs.” The reliability of microelectronics is measured in Failures inTime (FIT). One FIT is equivalent to one error (hard or soft) per billion hours of operation.Soft error rates in microchips can vary from a few hundred to many thousands of FITs.47
At 100,000 FIT, one can expect roughly one error per year of continuous operation. For most consumer applications, this is not a signi cant problem, especially given that most consumers replace their computers, cell phones and other devices every few years. For DoD applications, on the other hand, this could be problematic, both due to their operating environments and the extended life cycles we expect from military systems.Aircraft ying at an altitude of 30,000 feet or higher are subject to neutron densities hun-dreds of times higher than at sea level. One can therefore expect FIT rates to increaseproportionately. For hard errors, greater scaling is possible as multiple events in the same general area within a microchip compound problems, causing degradation that even-tually results in failure.
In most terrestrial, non-nuclear system applications, radiation-induced SEEs may be rela-tively rare, but they can cause upsets and reliability problems, and these can becomemore consequential in newer microelectronics with smaller feature sizes. Terrestrial mi-croelectronics associated with nuclear weapons or power plants can experience higher rates of SEEs due to the higher-radiation environments in which they operate, and poten-tially greater rates of hard errors, including degradation-induced failure.
Other Microelectronics Atomic-Level Degradations
The silicon on which most microelectronics are based is formed in a crystal lattice struc-ture. When manufacturing the chip, various processes are used to create doped silicon48
that produces desirable electrical properties, and the oxides that provide electrical insu-lation. The result of these manufacturing processes is that the forces that hold the crystaltogether are weakened. Near the edges of conducting silicon and insulating oxide, for example, the lattice will naturally be weakened as the crystal changes from one mate-rial to another.
47. Santos u ar, S alu Argar al, and ae Pil ung, “So Error Issue I portance o Lo Alp a Solders or icro-electronics Pac aging,” Rev. Adv. Materials Science 34 (2013): 185-202.
48. “Doping” replaces atoms within the crystal with atoms of another element that either creates extra electrons or extra “holes.” Changing the number of electrons or holes in the material changes the electrical properties of the material,resulting in the designed behaviors of the chip
60 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
microelectronics are small enough that the forces, even in naturally weakened areas such as the silicon/oxide interfaces, hold thecrystal together tightly enough. As wire sizes and gates become smaller, the amount ofedge material, and thus the signi cance of weakening due to doping, both becomegreater. In the same way that molecules of water can drift from the surface of a cup ofwater into the atmosphere by virtue of the molecules’ vibrational energy (i.e., evapora-tion), it is possible for atoms at the edges of crystal lattices to disassociate from the lat-tice. The constraining forces in this case are different because the underpinning energy levels are different, but the general effect is reducing the amount of material that makesup the device. Whether due to manufacturing uctuations or the results of the atomiceffects described, when these paths or gates become narrow enough, they can result in areas of increased resistance and, under suf cient conditions, the microelectronics simply “burn up” (much like a fuse burning out) from the induced heat.
Other effects in microelectronics can involve a combination of atomic and macro effects,and lead to gradual degradation that renders the chip less reliable. One such effect oc-curs in ash memory (which has been used for years in random access memory or “RAM”in computers). As tolerances become tighter with smaller gates in ash memory devices,ash memory “wears out” as cells are repeatedly written and read.49 The mechanisms
involve atomic level changes that occur as charges are moved into and from atomic-sizedevices within the chip. In short, as microelectronics become more sophisticated, effects that were minor in older chip designs can become more prominent.
Microelectronics in Quantum Domains
As gate sizes descend to single nanometer (nm) sizes (for example, Intel is planning toachieve a commercially viable 7 nm feature size in the near future), radiation may cause undesired quantum effects that can lead to degradation and failure of microcircuits.50
Background radiation, cosmic rays, radioactive decay of isotopes, and other environ-mental effects can induce atomic effects that render microelectronic components in-operable, error prone, or cause them to exhibit greater failure rates than were observedin older designs. In the same way that various SEEs cause different kinds of damage,environmental conditions can cause either transient or permanent damage.
Ionization events can happen due to applied electric elds in the normal operationof the microelectronic device. By design, these normally involve just a few volts, andthus the eld density is relatively small. owever, as devices become smaller, the “short channel effects” (referring to the shorter distances charges must travel as microchip
49. C ien, A. and . ara c e , “ oore s La : e First Ending and a Ne eginning,” Computer 46, no.12 ( ec2013): 48-53.
50. ason ic , “I F 2013: Intel S o s Plans or 7n C ips 22n L E Ato s are S ipping,” Daily Tech, 11 Sept 2013,Accessed 20 Aug 2015, p: .dailytec .co I F 2013 Intel S o s Plans For 7 n C ips 22 n L EAto s are S ipping ar cle33354. t .
61CHAPTER 2: THE SCIENCE OF MATERIALS DEGRADATION
feature sizes become smaller) of applied voltage in nanometer feature sizes can cause“hot carrier injection” (HCI) events, meaning electrons or holes carrying charge throughthe semiconductor material become more energetic due to the high electric eld. HCI events are similar to ionizing radiation events.51
When combined, a nuclear event inside a region and a high electric eld can be thecause of an ionic breakdown: AEC causing classical corrosion. These events will be par-ticularly prevalent during short duration maximum electric eld applications common to modern electronics such as power cycles. As carriers move from “source” to “drain” inmultichannel devices, they can develop enough kinetic energy to cause ionization. Astrapped charges accumulate, interfaces within the device can break down and thresh-old voltages can change, affecting the performance of the device.
Degradation caused by external radiation can also be experienced at levels as lowas simple background radiation. The severity of a total ionizing dose (TID) of radiation,something perfectly achievable by normal background levels, will increase signi cant-ly as electronic devices shrink below the 10nm range. This is because the amount of trapped charged material that is needed to short-circuit insulator material is reduced when the total mass of the individual device is reduced. In this realm, small effects thatwould normally accumulate over decades might have impact in months or weeks.
In addition to accumulation of charges (static electricity), microelectronics can be dam-aged by other defects caused by radiation. “Displacement damage” (DD) results in theaccumulation of crystal lattice defects due to high-energy radiation exposure. Proton, neutron and electron impacts can displace silicon atoms from their proper crystal lattice locations.52 Separate from ionizing radiation effects, DD causes changes in the electricalproperties of the components, and can result in circuit failure as the electrical properties of the device are changed. More speci cally, they cause degradation of gain and leak-age current in bipolar transistors. In space, this is particularly important for solar panelsbecause DD reduces the power output of the solar cells. DD can also adversely impact optical detectors and light-emitting diodes (LEDs). Similar devices used in terrestrial ap-plications can also suffer from degradation due to DD. Future technologies are likely to employ miniature optical devices embedded in microelectronics, which will also be subject to degradation due to DD.
51. . entrcia F. e al, . eguella and . Arar, “Ne Approac ased on ANFIS Co puta on to Study t eres old oltage e avior Including rap E ects or Nanoscale G SFE S,” World Congress on Engineering
ol (proceedings, orld Congress on Engineering, London, U. ., uly 3 -5, 2013).52. Leroy, C. and Pier-Geiorgio Rancoita, rinciples o Radia on nterac on in Ma er and Detec on, orld Scien c,
62 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The impact of AEC is increasing as modern technology introduces new realms of mate-rial sustainment. While the physics and underlying causes are complex, there is a lot of science that is well understood relating to degradation of systems due to atomic effects.Nonetheless, to date the main approaches to address AEC involve maintenance,redundancy, and replacement.
While we do not purport to have solutions, we have identi ed severalapplication areas, both existing and future, where these concerns could become paramount. We have focused on microelectron-ics because they are so pervasive in DoD systems, and in society ingeneral. As microelectronics’ sophistication increases, atomic effects are likely to increasingly cause errors and permanent degradation,and these problems are likely to become more severe earlier. We alsohave noted that the harsh environments for stored nuclear weapons,
nuclear waste disposal, nuclear power plants, and outer space give rise to degradationprocesses that include atomic effects corrosion, and sometimes these AEC processescan become the underlying cause for classical corrosion. The next chapter proposesapproaches to address AEC, with the ultimate goal of offering opportunities to improvematerial sustainment in the face of AEC and other corrosion mechanisms, rather thanreact to its effects after the fact.
Modern technologyintroduces new realms of materialsustainment.
CHAPTER : RECOMMENDATIONSWe introduced this book with the argument that in order for DoD to improve material sustainment, a broader de nition than the classical, chemical environment based de ni-tion of “corrosion” was required. We pointed out that there are mech-anisms other than chemical corrosion that cause materials to degrade, and proposed a corrosion spectrum to categorize these mechanisms and their effects. The spectrum includes classical corrosion (molecular level), introduced a new term for macromolecular-level degradation that we called “biological effects corrosion,” and at the atomic level, explored the atomic effects corrosion (AEC) that is the focus of this book. In sum, chapter 1 introduced the topic and addressed the question, “Why should anything change ” in the concept of re en e e m ni r an mana e corrosion and degradation.
With chapter 1 as background, chapter 2 describes the mecha-nisms of corrosion and degradation, including a brief overview of classic corrosion and a more in-depth description of AEC mecha-nisms. In sum, addressing the question, “What are the mechanisms of materials degradation ” en route to recommending a broader approach to dealing with corrosion and degradation that we called material sustainment.
This chapter addresses the “So what do we need to do ” question. That is, it recom-mends what we believe the DoD, and more speci cally the Corrosion Policy and Over-sight Of ce (CPO), should do about corrosion, materials degradation and material sustainment throughout the corrosion spectrum, and why consid-ering all mechanisms of corrosion should be included. In this vein, we make recommendations in the areas of strategy, policy and research. These areas are all related (see The Corrosion Spectrum graphic on the following page). In fact, ur re mmen a i n r
ra e are all a ia e i li essentially, we are rec-ommending a strategic plan for identifying, organizing/prioritizing and implementing policy across the full corrosion spectrum. Therefore, we discuss strategy and policy to-gether, followed by the research recommendations that provide the scienti c under-pinning for both.
“What are the mechanisms of materials
“So what do we need
64 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
dod interests and cpo mission
Before getting into the speci c recommendations, it is important to answer another question, which is “What is the basis for a DoD of ce delving into areas (such as nuclear power plants) that are controlled by other agencies (such as DoE) ” The short answer is because even though DoD does not “own” some of these areas, DoD does have inter-ests in them. The Corrosion Spectrum graphic below provides an overview of how each of these topics is important to the CPO the DoD agent for corrosion prevention and management, even if the systems in these areas are not all controlled by the DoD. At the top is the corrosion spectrum that affects all materials, with the three basic categories that detract from material sustainment. On the left and right sides are DoD Interests and Needlines, respectively, both of which CPO currently manages in the classical corrosion arena. In the area of classical corrosion, the CPO’s mission (which we argue should be across the spectrum) is to develop a comprehensive capability to prevent and mitigate corrosion and its effects on DoD systems and infrastructure.
Corrosion Spectrum Diagram/Alex Taliesen
65CHAPTER 3: RECOMMENDATIONS
In order to carry out its mission, any DoD organization has three levels of involvement: control, in uence and interest. For example, the DoD controls conventional military sys-tems, which are directly acquired, operated and maintained by military Services. At the next level, DoD can in uence areas it does not control for example, Air Force aircraft transport and launch the airborne weapons that comprise the aerial dimension of our nuclear deterrence triad, and Navy ballistic missile submarines transport and launch un-dersea strategic nuclear weapons. In an area where two or more agencies control spe-ci c aspects associated with the application of national capabilities, each is said to have in uence in that area. For example, the Air Force and Navy specify the unique conditions in which the nuclear weapons they transport/launch must operate effective-ly. In some areas, such as space satellites, DoD neither launches nor operates satellites, yet DoD has direct interests in the satellites’ products, such as the imagery needed to produce critical intelligence for our operating forces. So even though DoE controls nu-clear weapons and NASA manages space systems, the DoD has interests in the applica-tion of those weapons and space systems. The point is not that DoD should have more control over more areas, but that it needs to coordinate with other agencies to further our national interests. As we will point out in the recommendations throughout this chap-ter, in the area of corrosion/degradation and material sustainment, there are areas where this coordination needs to expand as technology continues to advance.
Furthermore, and as we’ll illustrate with a speci c example later (see Objective 2, Develop a Broader Coordinated Research Program), we assert that cross-boundary coordination between agencies can result in new and improved systems that are ben-e cial to both, regardless of their particular spans of control. This is a primary motivator for recommending a coordinated re-search program. Though listed as “DoD Needlines” on the right side of the graphic, in reality all agencies with material sustain-ment requirements have the same Needlines. All agencies need to understand the fundamental phenomena that affect their material systems, all need to monitor and mitigate the effects of corrosion/degradation, and, ultimately, all would like to be able to design systems that prevent corrosion or degradation in the rst place. We’ll discuss the strategy and policy implications rst, and then speci cally address the necessity for deeper scienti c understanding in the research recommendations, but the bottom line is this: if we can understand materials and their behaviors (i.e., from AEC through biological effects corrosion), then rather than engineering new systems from empirical data alone we will have the opportunity to know how their fundamental properties translate into both micro- and macro-level performance. Coupling this basic understanding with improved predictive models can result in a national asset that can be applied to material sustainment across the board.
The point is not that DoD should
have more control over
more areas, but that it needs to coordinate with other agencies to further our
66 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
As a simple example of what we mean by “from the bottom up,” let’s return to our caveman, “Og,” of chapter 1. He learned that if he whacked something with a club, the effect was greater (and less painful) than whacking it with his own st. That is empirical evidence: essentially the result of trial and error. Empirical results can be a powerful tool, as anybody without a club would have found out if he engaged in combat with Og. If, on the other hand, Og had possessed the capacity to do the research to develop the science to understand the fundamental properties of materials, then he would have the opportunity to design a club that wouldn’t eventually rot (that is, Og could have ac-complished bottom up ).
To nish the discussion of the Corrosion Spectrum graphic, the “stoplight” colored arrows point out where CPO stands in our proposed three areas of the corrosion/degradation spectrum. The green arrow indicates that there is already a lot of strategy, policy and research in the area of classic corrosion that is being coordinated and managed by the CPO in accordance with the current Title 10 de nition of corrosion. The yellow arrow is the subject of this book, in which we argue for broadening the de nition beyond classi-cal corrosion, and then address one of the broadened areas, AEC. The red arrow simply indicates that biological effects corrosion is currently lacking research and policy recom-mendations (the next book in this series will address this topic).
With the above as context, and the interrelationships between strategy, policy and re-search, we could start with recommendations in any of the three areas. We start with strategy and policy, then address research. The recommendations we address in the remainder of this chapter are summarized below.
1 Develop a comprehensive strategy for the corrosion spectrum.
2 Establish a broader coordinate research program that crosses boundaries in the corrosion spectrum.
3 Identify and make speci c policy changes based on research outcomes.
Research Directions1 Build for Reliability
2 Identify thresholds where AEC matters
strategy and policy
Given an expanded de nition of corrosion as described by the corrosion spectrum (though we prefer the term “degradation” spectrum to distinguish between the classical de nition of corrosion as involving chemical reactions, we will stick with “corrosion” for the sake of consistency), it makes sense that to address the broadened spectrum ef-fectively, the CPO needs a strategy and accompanying strategic plan to organize and prioritize the policy implications.
67CHAPTER 3: RECOMMENDATIONS
There are numerous methods for developing strategy and strategic plans. The military Services use the concept of ends, ways and means. Conceptually, strategy describes the relationship among ends, ways, and means.1 are the objectives and goals sought. Means are the resources available to pursue the objectives. And are how (i.e., methods) one organizes and applies the resources. Each of the components ad-dresses a related question: What do we want to accomplish (ends) With what resources (means) How do we apply resources to achieve ends (ways)
The CPO is the OSD of ce charged with achieving the end of reducing materials deg-radation so that our military material systems sustain their functionality and effective-ness. CPO’s goal is to reach this end via the ways of prevention, detection, prediction and management of materials degradation. The ultimate end for the CPO is to ensure that DoD assets and infrastructures are always in a state of readiness so that Service personnel can complete their mission without unexpected or unmitigated materials degradation reducing their effectiveness. In the current budget arena, with reduced resources, the Services are planning to keep equipment particularly major systems in operation for longer periods, simply because they can-not afford to replace it. The CPO mission becomes even more important in such circumstances.
A key element of the CPO’s strategy for ensuring that DoD assets and infrastructures achieve this End is to promote the philosophy of material sustainment, or ensuring mate-rials are functional throughout their life cycle and degrade on timescales that are pre-dictable. In order to properly do this, a deep understanding of degradation processes is needed. Limiting the development of this understanding to classical corrosion only limits the ways and reduces the ability to assemble the means to achieve this end. It should be clear that the CPO needs to address the full spectrum of corrosion in order to maximize our material sustainment capabilities.
For this reason, we recommend that the CPO needs a strategic plan that addresses the full spectrum of corrosion, and that identi es ways to keep equipment ready and operat-ing for longer periods. It is not unusual for military systems to remain in operation beyond their design limits, and in the current budget environment, we expect that even more systems will have their service lives extended. Certainly, the recommended strategic plan will address classical corrosion along with the other elements of the spectrum, in-cluding AEC and biological effects. ust as certainly, even though the focus of corrosion policy and research has been on classical corrosion, by no means have all the problems in that arena been solved. In short, we are not recommending a change in focus, but an expansion to include the other components of the corrosion spectrum.
With an expanded corrosion spectrum, obviously the CPO will need to seek new ways and means for achieving the ends of material sustainment. Updated policies (ways) ad-dressing the full spectrum of corrosion are needed, and the resources (means) that will
1. Ro ert . or , “A Pri er in Strategy evelop ent,” in U.S. Ar y ar College Guide o Strategy, eds. osep R.Cera i and a es F. olco , r., (Carlisle arrac s Strategic Studies Ins tute, Fe ruary 2001), 11.
Ends are the objectives and goals sought.
Means are the resources available to pursue the
objectives. And ways are how (i.e., methods)
one organizes and applies the resources.
68 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
be available to the CPO are limited. As a result, we suggest that a carefully constructed strategy that addresses issues of both policy and research within the available means (to include leveraging other means see Objective 2, Develop a Broader Coordinated Research Program) is critical. The gure below depicts the complexity of strategy devel-opment, and thus emphasizes the importance of carefully constructing such a strategy.
Note that the military de nition of End includes both goals and objectives. It is often useful to break down the overarching goal into more closely de ned objectives that, together, improve the chances of reaching the desired end goal.
1 Develop a comprehensive strategy for the corrosion spectrum.
2 Develop a broader coordinated research program that crosses the boundaries in the corrosion spectrum, especially in areas where corrosion mechanisms in different parts of the spectrum are coupled.
3 Identify and make speci c policy changes within the comprehensive policy based on research outcomes.
69CHAPTER 3: RECOMMENDATIONS
Clearly, these objectives are all related. The comprehensive policy will identify areas where research is needed, including coordinated research. By the way, when we use the term “coordinated research” we mean research that crosses traditional boundaries between the sciences (e.g., chemistry and physics), or between speci c research areas within those sciences (e.g., between the physics of statistical mechanics and organic chemistry). By extension, coordinated research also includes crossing traditional bound-aries between government agencies such as DoD, DoE and NASA. Let’s describe each objective in turn.
Objective 1: Develop Comprehensive, Full Spectrum Corrosion Strategy
A key element of the CPO strategic plan is developing a comprehensive strategy that expands from classical corrosion by adding the other elements of the corro-sion spectrum: atomic effects corrosion and biological effects corrosion (we re-mind the reader that this book only introduces the idea of biological corrosion, and the next book will address the associated mechanisms in detail). As far as the structure of the comprehensive policy, we believe a model for it already ex-ists in the CPO’s existing policy. For example, DoD Instruction (DoDI) 5000.67, -
addresses Title 10 authority and provides the associated de nitions, policy and responsibilities.2
• Address corrosion prevention and mitigation in trade-off decisions involving cost, useful service life, and effectiveness.
• Implement corrosion prevention and control (CPC) programs and preservation techniques throughout the life cycle of all military equipment and infrastructure.
• Review and evaluate corrosion plans for acquisition category (ACAT) I3
programs, and raise issues to the Defense Acquisition Board.
• Assess military equipment logistics and nancial systems for corrosion-related information to address CPC and related logistics and readiness issues.
• Submit information (each of the Military Departments) on proposed corrosion programs and corrosion-related research, development, test, and evaluation (RDT E) funding to CPO.
To assist in implementing policy, research and solutions in these areas, the CPO-sponsored www.corrdefense.org website provides easy access to a wide range of resources tar-geted to both corrosion professionals and others (such as DoD program managers) in
2. ce o t e Undersecretary o e ense or Advanced ec nology and Logis cs, US (A L), o I 5000.67,Preven on and i ga on o Corrosion on o ilitary E uip ent and In rastructure, Fe 2010.
3. ACA I, or a or e ense Ac uisi on Progra s ( APs), are iden ed y t eir cost and ilestone decisionaut ority ( A) levels. See, or e a ple, p: ac notes.co ac note ac uisi ons ac uisi on-category.
70 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
different disciplines who need corrosion related information. The website is constantly up-dated with new information and resources, and links to other corrosion-related websites.
Currently, CPO policy authority is limited to classical corrosion. Therefore, our rst recom-mendation addresses expansion of this de nition to include atomic and biological ef-fects corrosion. The focus of discussion for this book is on AEC because the research and subsequent recommendations associated with biological effects is our next research task, and the subject of our next book. Regardless of the corrosion mechanism (clas-sical, atomic or biological), these existing policy areas must apply in order to achieve the mission of ghting corrosion and improving material sustainment so that our Service personnel have ready, functional and effective equipment. So the question becomes, “What more should be done to improve material sustainment as corrosion policy ex-pands across the spectrum ”
We recommend there are two additional areas that should be incorporated into the expanded policy: (1) increased coordination and cooperation with other Federal and state government agencies, and (2) a broader investigation and coordination of corro-sion mechanisms in the areas of coupled and multi-mechanism corrosion. Let’s describe what each of these areas entails.
The rst area is increased coordination and cooperation with other Federal and state agencies. We have discussed the need for DoD to prevent, detect, monitor and man-age corrosion and degradation in all systems associated with control, in uence and interests. For example, DoD is interested in the sustainment of not only DoD, but also national, infrastructure. When the Services need to mobilize and deploy for military op-erations in our national interests, they need access to capable state and Federal infra-structure so that military forces can move from garrison locations to sea and air ports to deploy to the objective areas. In a large con ict, before deploying from garrison, the Services need to activate reserves and assemble them at military facilities, and those reserves need functional roads, bridges, railroads and airports to get to their assembly areas. Because many of the infrastructure corrosion mechanisms are indeed classical corrosion, CPO is already addressing the sustainment of national infrastructure, and has reached out to both Federal and state agencies in order to foster collaborative efforts to prevent corrosion and sustain our national infrastructure.
As AEC is further investigated, researched and identi ed, increased coordination and cooperation will be needed in the areas where AEC is likely to be most signi cant. These areas are primarily nuclear weapons, power and waste (DoE) space systems (NASA) and microelectronics (which have proliferated throughout the globe as well as our na-tion). We pointed out in chapter 2 that DoE has and continues to conduct research in a range of AEC mechanisms associated with nuclear systems. Furthermore, NASA has researched mechanisms of AEC in space systems. Both agencies’ research tends to be focused on speci c mechanisms and effects of interest speci cally to them. We recom-mend that because DoD has interests in both these areas, it makes sense for CPO to coordinate more with both agencies to identify AEC mechanisms that have implications for multiple agencies, and also mechanisms that may become more important in broad
71CHAPTER 3: RECOMMENDATIONS
applications such as AEC in microelectronics. Where can DoE research into AEC associ-ated with nuclear systems be applied to space systems, and vice versa Which mecha-nisms DoE or NASA have researched may become important in non-nuclear, terrestrial microelectronics applications We understand that there are highly classi ed speci cs, particularly with nuclear weapons, but the underpinning basic science can be more broadly applicable. We recommend that CPO, with a broad focus on material sustain-ment in general, is ideally positioned to be the agent of increased coordination and co-operation with Federal agencies that specialize in a single area, such as DoE and NASA.
The need to improve coordination in AEC research is particularly acute as microelec-tronics incorporate reduced feature sizes and increased component densities. As in-creasingly sophisticated microchips are produced, we believe that AEC is going to be-come increasingly important. The commercial realm is driving the state-of-the-art in microelectronics, so in this area the task is more complex than direct interaction with other Federal agencies associated with nuclear and space systems. We believe that as microchip technologies improve, and AEC becomes more impactful, there will be more opportunities to address DoD interests in material sustainment of microelectronics. We recommend that CPO can lead this interaction, coordination and cooperation. In short, as CPO has improved classical corrosion mitigation, by applying the same general ap-proach and developing speci c AEC methodologies, CPO is ideally positioned to be the agent of increased coordination and cooperation with both the commercial microelec-tronics community and other DoD microelectronics-speci c organizations such as the Defense Microelectronics Activity (DMEA).
To accomplish both these functions, CPO needs a comprehensive, full-spectrum corro-sion policy along with a strategic plan for coordinating and cooperating with Federal, State and commercial activities. The CPO’s history of coordination and cooperation in the classical corrosion arena provides a model that can be adapted to the broader roles associated with prevent, detect, monitor and manage corrosion in pursuit of mate-rial sustainment across the corrosion spectrum.
In association with a comprehensive policy and strate-gic plan for coordinating, it is reasonable to ask, “What needs to be coordinated ” in the corrosion spectrum. We believe there are two answers to that question. The rst is to expand the types of cooperation among different agencies addressing the same kinds of problems, as CPO already does in the classical corrosion arena. So our rec-ommendation here is to simply broaden the kinds of coor-dination initiatives CPO already promotes. The second is to promote and manage research into what we call coupled or multi-mechanism corrosion that crosses the boundaries of the spectrum. As illustrated in the cancer example in chapter 2, things that happen in one area of the spectrum can cause effects in another for example, an AEC effect can be a cause of classical corrosion. Recall our observations on research: speci cally, there is a lot of excellent
The need to improve coordination in AEC research is
particularly acute as microelectronics
incorporate reduced feature sizes and
increased component densities.
72 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
research that has been completed and that is still underway, but this research tends to focus on a speci c effect, and research projects tend to be of relatively short duration. Such research must continue, but we recommend that CPO’s mission to understand all corrosion mechanisms should include the task of developing and implementing policy for a coordinated research program to address the broader issues of cross-boundary coupled, multi-mechanism corrosion. This research would build on existing and on-going research into speci cs, explore how causes in one area of the spectrum may produce effects in another, take a longer-term view of reviewing speci c research and identifying areas where one agency’s results can apply to another agency’s problems, and also foster cooperative, multi-disciplinary research to address “wicked hard” problems such as tin whiskers (which we’ll discuss more in the research recommendations section).
In sum, the only issue with the current CPO policy is that it is currently limited (by Title 10) to classical corrosion. CPO needs the authority to expand beyond that limitation, into atomic and biological effects corrosion. Of course, that is easier said than done and dependent on obtaining results in the other objective areas of coordinated research and speci c policy updates. On the other hand, it is not necessary to start from scratch in this endeavor. As we described in chapter 2, there is a lot of science already completed on AEC, and we suspect we will nd the same in biological effects corrosion when we research that area in detail. What is needed, and is the topic of the next strategic objec-tive, is better coordination of research in speci c areas, and in determining the coupled and related mechanisms associated with AEC and classical corrosion (and, by exten-sion, biological effects corrosion). So let’s move on to that topic.
Objective 2: Develop a Broader Coordinated Research Program
We have de ned coordinated research as research that crosses traditional boundaries between the sciences, between speci c research areas within those sciences and, by extension, coordination crossing traditional boundaries between government agen-cies. Perhaps a historical example will help explain what we mean before we describe this objective.
Before the rst microchip was developed, it was well known that space is a high-radi-ation environment. When microchips were rst introduced into space systems, radia-tion hardened or “rad hard” microchips were built in small foundries based on custom designs using exotic materials and components to harden the chips from the effects of radiation. In short, rad hard was achieved by custom designs, and rad hard chips were built in small quantities. Because these designs were so speci c and so limited, the cost per chip was much higher than commercial microchips with broad applications that were manufactured in the millions. In the 2000s, scientists at the Defense Advanced Re-search Projects Agency (DARPA) with a commercial manufacturing background won-dered if they could meet the need for radiation hardening by commercial microchip manufacturing along with specialized processing methods such as circuit mitigation and error checking techniques. They found that it was indeed possible, which allowed advanced commercial designs to provide the required radiation hardening without the need for specialized, custom, exotic materials fabrication targeted to single, spe-
73CHAPTER 3: RECOMMENDATIONS
ci c uses. Though this development was not without controversy (particularly from the specialized foundries), the point is that by between specialized microchip foundries and commercial designs hardened by processing, commercially-designed chips (the hardware) plus processing (the software and techniques such as circuit mitigation) could withstand the high radiation environment of space, and could do so more cost effectively.
The above is just one example, but a trend we have noticed in our research for this book especially (and understandably) in the very sensitive and highly-classi ed areas associated with nuclear weapons is that it is very easy for scientists to become pigeon-holed into very speci c areas, and the cross-fertilization between results in one area and their potential application in another is lacking. Why is this important Let’s return to our cancer example from chapter 2: diseases like cancer remind us that when things degrade on the smallest scale, the result can have a serious impact on our daily lives. A cancer that begins in an individual cell degrades the nucleus of that cell, which can spread to other cells, which collectively degrade the tissue or organ, which degrades the human being that is made up of cells, tissues and organs. Fundamentally, the same cascading effect can happen via AEC if, for example, a neutron collision degrades a material lattice, which degrades a transistor, which degrades the chip, which degrades the computer, which degrades the weapon system.
Somewhere between the neutron that degrades the material lattice and the degraded chip, we transition from AEC to classical corrosion. The point is that the excellent but very specialized science being developed for speci c applications is not suf cient. Therefore, we need a that seeks potential cross-bound-ary implications and coordinates the scienti c investigation to determine the causes and effects of observed degradation effects at all scales (atomic/sub-atomic, molecu-lar, macromolecular). It is certainly understandable that scientists involved in specialized investigations are focused on the specialized problem they are trying to understand and resolve. As science has grown more sophisticated, it is natural for increased spe-cialization to occur simply because a single mind cannot comprehend it all at the de-tailed level. However, it is not necessary to understand all the details to identify areas where results can cross boundaries.
For this reason, we recommend that CPO develop a coordinated research program not to investigate the science per se, but to identify problem areas where coordination of different scienti c investigations is needed. That is, CPO’s role is not to do the sci-ence, but to coordinate its investigation and “cross-pollination” between the very specialized elds, communities and organiza-tions. In simple terms, what we are recommending is that CPO should, in concert with a broader de nition that includes the cor-rosion spectrum, seek out areas where the materials degradation problems are or could be crossing boundaries. Obviously, cross-boundary problem identi cation includes coordination with other government agencies such as DoE and NASA. Equally obviously,
The point is that the
excellent but very specialized
science being developed for speci c
applications is not suf cient.
74 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
there will be some areas where the investigation and implications of research in speci c areas such as nuclear weapons sustainment will be so sensitive that they are classi ed and compartmentalized. But we believe that at the basic science level, those will be relatively few, and the potential gains from coordinating research on common problems are tremendous. In sum, the recommended coordinated research program includes both identi cation of cross-boundary research and also cross-agency coordination.
One additional, much-simpli ed example (addressed in more detail in the research sec-tion) supporting coordinated research is the tin whiskers that occur when lead-free sol-der is used (by the way, “tin” is not the only metal that can result in “whiskers,” just the most commonly observed “metal ” whiskers are possible, and have been observed, in multiple lead-free solder applications). Tin whiskers, because they are metal, are electri-cally conductive structures that grow from surfaces where tin is used they can occur in both terrestrial and space applications. If they grow in the wrong places, they can short out electronic circuits, and as the node sizes of microelectronics decrease, their effects are likely to become more pronounced. Tin whiskers were rst observed in the vacuum tube era in the 1940s and 1950s.4 et to date, there is no single accepted explanation of the mechanisms that cause tin whiskers. Generally, they are recognized as being initiat-ed by atomic effects (they grow atom by atom), but they have effects (e.g., circuit shorting) commonly attributed to classical corrosion. With the multiple physical phenom-ena potentially underlying the cause of tin whiskers, it seems logical that coordinated research addressing the problem from multiple perspectives might have a better chance of succeeding where individual research efforts to date have not succeeded.
One nal recommendation on a coordinated research program: a focus on longer-term problems and complex mechanisms that combine multiple individual causes and their effects is needed. As science has specialized, it is only natural that scienti c investiga-tions would specialize, too. The results of our investigation of degradation mechanisms have resulted in identi cation of a trend toward investigating speci c, specialized cause
and effect mechanisms in short-term projects. Doing this science is without doubt a good thing and has ad-vanced our scienti c knowledge, but we need a com-ponent of the coordinated research program that also looks at broader, longer-term effects and the scienti c investigations that need to be conducted to connect individual mechanisms. Again, our cancer analogy applies: we need to identify those areas in which one cause results in an effect, and that effect becomes the cause of another effect, and so on. As our scientists
rightly pursue the speci cs, we need to identify the longer-term chains of mechanisms that start at AEC, move “up” to classical corrosion, and ultimately result in biological degradation effects.
4. NASA asic In o FAQ: p: nepp.nasa.gov is er ac ground inde . t .
...we need a component of the coordinated research program that also looks at broader, longer-term effects and the scienti c investigations that need to be conducted to connect individual mechanisms.
75CHAPTER 3: RECOMMENDATIONS
Objective 3: Enact Specific Policy Changes Based on Research Results
A comprehensive policy is a starting point that provides context to the investigation and resolution of problems within the corrosion spectrum, including both single mechanisms and the impact of cross-boundary mechanisms. Because we address research mecha-nisms in more detail in the following section on research including both general re-search directions and speci c examples, and because the impacts of speci c research remain to be determined, we do not yet know what those speci c policy changes will be. We do know, however, that speci c changes will be needed as we uncover more degradation mechanisms and related connections. The gure below shows a researcher in a laboratory as she achieves research results, the policy implications need to be ex-amined, too.
Therefore, we recommend recognition that as science develops, its policy implications also develop. This is true in a broad range of arenas for example, Einstein’s research leading to the theory of relativity, and the subsequent development of atomic weapons and their use in World War II, certainly led to policy and strategy changes in both the mili-tary and political arenas. Though we expect few implications so impactful as Einstein’s discovery, we also recognize that as science develops, so also must policy. And as policy develops, strategic plans need to adjust to policy changes.
76 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The point is that as research continues, including coordinated research, there will be spe-ci c policy implications, and therefore the need to develop (and thus change) policy, will undoubtedly occur. As a result, we recommend that as research results emerge, the CPO should be prepared to alter speci c policies that implement the results of that research. CPO has certainly done so in the past in the area of classical corrosion, so to them this is not a new idea. We simply point out that scienti c progress also results in policy changes. Therefore, corrosion (degradation) policy will evolve as the science to prevent, detect, predict and manage materials degradation evolves to improve mate-rial sustainment. Now let’s move on to the area of research.
We have already touched on research in association with discussions of strategy and policy: the three areas are closely intertwined and it is impossible to discuss any one area effectively without reference to the others. Strategic plans propose policy changes that result in new research requirements. Policies direct research that results in changes to strategy. New research can lead to policy changes that update strategies. In this section, we recommend general research directions, and also provide some speci c research examples, in order to illustrate the importance of research through-out the corrosion spectrum in providing the foundational science for good corrosion strategy and policy.
The goal of this section is to “prime the pump” for research in support of potential speci c strategy and policy changes. The rst topic is what we call “build for reliability.” What we mean by this term is conducting research that enables understanding of physical phenomena and interaction mechanisms throughout the spectrum of corrosion. The in-tent of this research is to identify opportunities to change how we design systems from the “bottom up.” That is, rather than engineering from empirical data, study material properties and interactions at the fundamental level, identify how those properties and mechanisms translate into both micro- and macro-level properties, and then design sys-tems founded on the basic science of materials. For example, a paper on nuclear reactor materials argues:5
In this paper, the authors argue that the investigation of atomic-scale degradation which we call AEC can allow understanding of how atomic interactions affect the macro behaviors of materials used in nuclear reactors. What this means is that they recognize that AEC mechanisms, once understood, are critical to selecting materials for designing improved nuclear reactors. By extension, improved designs to prevent or mitigate degradation are possible if we can understand the underlying mechanisms that produce them. As we discussed earlier, Og the caveman selected a club based
5. ar uis, E anuelle A. et al. “Nuclear reactor aterials at t e ato ic scale.” Materialstoday 12, no. 11 (2009): 30-37. p: .sciencedirect.co science ar cle pii S1369702109702962.
77CHAPTER 3: RECOMMENDATIONS
on empirical evidence that he could whack things harder when he used that club. But Og had no scienti c evidence of what causes the degradation mechanism (rot) that eventually resulted in that club becoming useless. Even with our advanced science, we still design systems today based on empirical results: we have observed over time that material A works better or lasts longer than material B, so we use material A to build our system. When the science of those materials and how they degrade is better under-stood, we have the opportunity to select or design better materials and apply them to improved designs a priori rather than after extensive experience in short, this level of understanding allows us to pro-actively “get ahead of the game” rather than reacting based on experience.
The second topic is what we call “identify thresholds.” What we mean by this is deter-mining when AEC matters in terms of both numbers of events and time. Chapter 2 has already pointed out multiple AEC mechanisms, and for some of them the numbers of events are suf ciently low that at least in current systems, they don’t have a noticeable impact during their design life cycles. We anticipate that as the nodes decrease in size and component densities increase, AEC in microelectronics will become more impor-tant, and we recommend research to identify the thresholds and service life expectan-cies for which AEC will matter in the future.
Let’s look now at each of these areas in turn, along with a few illustrative examples, in order to understand how research is fundamental to improving material sustainment. Inevitably, one can argue that an example included in Identify Thresholds can affect Build for Reliability, or conversely, and the argument is valid. So the organization of our examples is somewhat arbitrary. We include the examples where we do simply to indi-cate how speci c research can contribute to general research directions.
Examples: Build for Reliability
The basic tenet of build for reliability is contained in its name: the desire to build systems that are as reliable as possible throughout their life cycles. Supporting this desire is the need to understand the basic science associated with materials and material degrada-tion so that component of a system contributes maximally to the sys-tem’s reliability. As we explained in the introduction to this section, developing the sci-ence to understand the fundamental properties and degradation mechanisms of materials at all levels enables a “bottom up” design that is based on sound science, not the trial and error of empirically based engineering. The goal is to understand mate-rials behave as they do, not just recognize that material A works better than material B based on experience.
The rst research example is The gure on page 78 shows the growth of tin whiskers on a circuit board. This phe-nomenon, which is the growth of electrically conductive tin structures on surfaces, can cause havoc in electronic circuits by posing a signi cant reliability risk in electronic assemblies where tin solder is used. Considered by many the best alterna-
The basic tenet of build for reliability is contained in its
name: the desire to build systems that
are as reliable as possible throughout
their life cycles.
78 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
tive to environmentally caustic lead-based solder, tin solder is becoming more prevalent in electronics. NASA has a website6 devoted to tin (and other types of metal) whiskers that notes that tin whiskers can cause both long-term and transient short circuits, metal vapor arcs, and contamination in electronic circuits. Tin whiskers are a signi cant prob-lem in building reliable electronic assemblies, whether for use in the harsh environment of space or in terrestrial applications tin whiskers have been observed in both.
Tin whiskers were rst observed in the vacuum tube era of the 1940s and 1950s, yet to date NASA’s website notes in large red text for emphasis that “A single accepted explanation of the mechanisms has NOT been established.”7 The website points out that existing theories of tin whisker formation hypothesize that they occur by one of two mechanisms: (a) they grow in response to a mechanism of stress relief, or (b) they result from recrystallization and abnormal grain growth processes affecting the tin structures. In short, tin whiskers have been around for roughly seven decades, yet we still do not know what causes them.
We hypothesize that perhaps a build for reliability approach that investigates multiple mechanisms, or combinations of mechanisms, might produce more positive results in in-vestigating the causes of tin whiskers. It could be that each of the two theories has merit, and maybe tin whiskers are the result of multiple AEC mechanisms (no one seems to seriously dispute that tin whiskers are initiated by atomic effects, even if they eventually cause other effects). Therefore, we recommend that a broad spectrum, cross-boundary,
6. “ in is er (and t er etal is er) o epage,” ASA.gov, 8 ay 2012, Accessed 25 Sept 2015, p:nepp.nasa.gov is er inde . t l.
7. “ asic In or a on Regarding in is ers,” ASA.gov, 8 ay 2012, Accessed 25 Sept 2015, p: nepp.nasa.gov is er ac ground inde . t .
SilSililvvvvvevererrvve SSuSuSuSuuuull dl ddl dl ddl ddde We We We We WWWWhishihisisishishishhishish kekerk s gs rowrowowingng ouououoouutt ot ot of ssf sf uurfurfur acacecee-mo-mmomountntun reeresisistororssffrofrofrofrof ofr mmmm am MoMoogg DS2S22DSDS22000000000000000 seseservorvodridridrive.ve.veve / o/ oo/ onananattnan honhoononReiReiR nhanhahnh rt
79CHAPTER 3: RECOMMENDATIONS
multidisciplinary approach may yield better results than adherents of the two basic theo-ries working separately. Could it be that stress relief mechanisms result in recrystallization and abnormal grain growth We don’t know, but we recommend that the topic of tin whiskers is important in research investigating AEC.
Tin whiskers cause problems in electronic circuits and microchips, but they are not the only AEC mechanism that needs further research. We have already pointed out, in the section describing the development of a broader coordinated research program, an example where cross-boundary investigation led to a more cost-effective approach to developing radiation tolerant, “rad hard” microchips. In this approach commercial foundry methods plus processing techniques resulted in rad hard chips without having to resort to small, boutique foundries using exotic materials to source these chips. The result was microchips with equivalent rad hard performance at lower cost. It was accom-plished by a cross-boundary approach: commercial foundries employed manufacturing techniques developed for other types of chips plus processing techniques to a special-ized, space application. The commercial methods crossed the boundary between high-volume consumer microchip development into what had previously been the highly specialized eld of designing microchips speci cally for operation in the harsh environ-ment of space.
While the rad hard example demonstrates commercial techniques crossing the bound-ary into space techniques, we believe it could be useful to cross that boundary in the op-posite direction. Commercial microchip manufacturers are concerned about reliability, even in the lower-radiation terrestrial environment. Developers of space systems require chips that must last for years in the higher-radiation environment of space, and in which you cannot simply replace a chip that goes bad to repair a system. Getting space sys-tem designers together to discuss lessons with the commercial reliability community is almost certain to result in identifying techniques from space systems that can be applied to terrestrial applications. CPO, with the mission of improving reliability for all DoD systems and infrastructure, could help coordinate these useful interactions. The image below and the diagram on page 80 depict areas where CPO can help coordinate interactions across boundaries.
Nuclear power plant/www.pixabay.com
80 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Similarly, scientists investigating failure mechanisms and reliability in the nuclear weap-ons, power and waste areas have a problem similar to one space system designers have: both communities’ systems must work in a high-radiation environment for long periods of time. Many of the details of nuclear systems, particularly nuclear weapons, are highly classi ed. The basic science discoveries associated with investigating and over-coming failure mechanisms should for the most part not be classi ed. If they are, then government-to-government information exchanges can be conducted at the classi ed level. Scientists in the nuclear power arena are already working on better understanding of the fundamental mechanisms associated with designing nuclear reactors for reliabil-ity: their goal is to develop bottom-up designs based on rigorously-developed science rather than continuing to rely on empirical data derived from experience (which can be a harsh teacher: as the old aphorism says, “experience is what you get when you survive your mistakes” source unknown).
Combining what we learn from continued research with better predictive modeling (an-other goal of the nuclear weapons community in an age where the U.S. no longer tests nuclear warheads) might result in cross-boundary applications developed from the ex-change of information between the nuclear and space communities. Some results can probably also be applied to improving commercial microchip reliability, especially as the feature sizes in microchips decrease. Because the commercial foundries are driving
81CHAPTER 3: RECOMMENDATIONS
smaller feature sizes, all these communities could bene t from appropriate exchanges of information about basic science and predictive modeling.
We have already said that as science continues to develop, the scientists at the leading edge are growing more specialized. The body of knowledge has grown large enough that specialization is necessary no one scientist can possibly “know it all.” The CPO can monitor developments and broker interchanges in the AEC arena that promote build for reliability in the same way that the CPO already does this in the arena of classical corro-sion. All that would be needed is for CPO to expand an already-working approach for classical corrosion into AEC.
Examples: Identify Thresholds
The other general research direction we have recommended is “Identify Thresholds.” As designs become increasingly sophisticated, AEC mechanisms that are not causing prob-lems today may well do so in the future. At the macro level, we do not worry much about the effects of cosmic radiation on construction equipment, for example. The total doses are so low that other corrosion and wearout mechanisms result in the failure of these ma-chines long before ionizing radiation results in any observable problems. The same is true of older-model microchips with relatively large feature sizes. AEC was certainly observed in these chips, but they were designed such that the radiation effects would be unlikely to cause a problem during the design life of the chip.
As feature sizes decrease and component densities increase in modern microchips, that may no longer be the case. The intent of Identify Thresholds is to promote research to determine when AEC is likely to become a problem, and develop methods to overcome it. Current design techniques, such as redundancy, are used to ensure that if AEC dam-ages one critical part of the circuit, there are (usually multiple) backups for that function. Of course, having to include multiple backups for critical components obviates some of the advantages of increased component densities. If research could identify other tech-niques to overcome AEC in microchips, it would be possible to regain the advantages of advanced designs. To date, however, there are no known mechanisms by which high-energy radiation can be completely shielded, and for this reason we recommend coordinated research into Identify Thresholds, both in terms of understanding how AEC is caused and to develop ways to detect, predict, and manage it. In short, we need to know when AEC mechanisms are going to cause signi cant damage as microchips with smaller feature sizes are developed.
High-level descriptions of AEC mechanisms affecting microchips are described in chap-ter 2, and more scienti c detail is available in appendix one. Examples of microchip AEC mechanisms include single event upsets, single event latchups, single event burnouts, hot-carrier injection, total ionizing dose, lattice displacement damage, electro-migration and dielectric breakdown. The effects of these mechanisms can be transient, such as changing the value of stored data, or can cause permanent damage. Currently, most of these effects are mitigated by empirically derived design features: redundancies, moving critical nodes further apart, and error correction processing techniques such
82 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
as parity checks. All of these introduce a penalty in microchip designs. As feature sizesbecome smaller and component densities increase, many of these effects may cause signi cant degradation to the microchips’ function, requiring more redundancies or other features, and thus incurring an additional penalty that reduces the advantage ofincreased component density. As more modern microchips are developed, research is needed to Identify Thresholds at which AEC becomes signi cant.
The macro effect of corrosion from any mechanism on microchips is seen in microchipreliability and wearout. The graphic below illustrates experience in microchip life cycles. Early in a “new” microchip design, the primary concern is early life failures (ELF). Micro-chip foundries devote a lot of resources to mitigating ELF because they do not want todeliver defective microchips to their customers. Once the initial ELF issues are resolved,a given microchip design moves into the bottom of the “bathtub” depicted in the chart below. Once the initial “bugs” are resolved during ELF testing, a microchip becomesrelatively stable and that style of chip is put into production. At that stage, a manufac-turer is suf ciently con dent in offering that particular model microchip for sale. Failurescertainly occur, but they do so at much lower levels.
Later in their design lifetimes, wearout mechanisms increase the failure rates in micro-chips, if for no other reason than entropy (the label scientists have assigned to the natural tendency toward more disorder). Nothing lasts forever, and all systems, including micro-chips, eventually wear out. Recognition of this fact is a major contributor to establishingthe expected design life for any system. If, however, AEC is having signi cant effects,
Experience in microchip life cycles/Alex Taliesen
83CHAPTER 3: RECOMMENDATIONS
microchips may experience premature wearout due to corrosion. Research is needed to identify the points, the causes and the timeframes at which AEC becomes signi cant in modern microchip designs to ensure that chips are not failing early due to corrosion instead of normal wearout mechanisms.
Microchips are not the only designs where AEC may occur. As Micro-electro-mechanical systems (MEMS) continue to develop, these orders-of-magnitude smaller machines may be damaged signi cantly by AEC. Nanotechnologies (“nanotech”) manipulate matter at atomic and molecular levels in order to fabricate macro-scale products. Nanotech-nologies are designed at the scale where quantum mechanical effects are important. Unlike a macro machine that will fail from classical corrosion or component wear long before radiation damage becomes signi cant, MEMS and nanotech may be damaged by much smaller doses of radiation. Research is needed to identify thresholds applicable to areas in which the radiation environment causes signi cant AEC in all areas where MEMS or nanotech are applied: space, nuclear and terrestrial applications may all be affected by AEC.
The CPO manages DoD’s interests in all these arenas, and therefore can become the coordinating agent for research into the effects of AEC as microchips, MEMS and nanotech continue to develop. One purpose of coordinating research is so that as signi cant AEC thresholds are identi ed, the results can be shared with other communities. It may be that signi -cant effects in one area are not so signi cant in another, but CPO can coordinate the research and make scientists and engineers in all arenas aware of signi cant results as CPO does for classical corrosion today.
summary: corrosion at the atomic scale represents one area on a spectrum of corrosion effects that spans from the nanoscale to macroscale
The goal of the Of ce of Corrosion Policy and Oversight (CPO) is to help ensure that DoD assets and infrastructures remain in a state of readiness so that Service personnel employing them can successfully complete their missions. To do so, DoD assets and ma-terials need to be reliable, technologically superior, and affordable. Part of the CPO’s strategy for ensuring that DoD assets and infrastructures are secure is to promote the philosophy of material sustainment, which is intended to ensure materials are functional throughout their life cycles and degrade on timescales that are predictable. In order to properly do this, DoD needs scienti c understanding of degradation processes. Tradition-ally, this understanding of degradation has focused on “classical corrosion,” referring to speci c material structures degrading due to bulk chemical effects caused by envi-ronmental forces that evidence themselves in macro structures such as bridges, aircraft and military vehicles. Corrosion in the classical sense deals with degradation events that
Nanotechnologies are designed
at the scale where quantum
mehanical effects are important.
84 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
metals rusting. There was no other broadly applied con-sideration of the way that materials could degrade. The results of this study shown inThe Corrosion Spectrum graphic above indicate that this is an incomplete vision of the corrosion problem.
We have recommended that the corrosion spectrum, including AEC, classical corrosionand biological effects corrosion, requires studying degradation mechanisms and effectsat all relevant scales. Matter has different properties at different scales, and the eventsthat cause matter to degrade occur through different mechanisms and phenomena at different scales. For example, an aircraft is made up of many different parts, the partsinclude many different types of materials, materials incorporate different componentsthat perform various functions, and “size matters” for many of those components to con-tinue to function throughout their design life cycles. This is particularly true for DoD systemsthat are often retained in service beyond their original design life cycles. The metal thatmakes up the aircraft wing needs to have a certain type of composition, be a certain
Corrosion Spectrum Diagram/lex Taliesen
85CHAPTER 3: RECOMMENDATIONS
thickness, and exhibit speci c properties in order for the wing to perform as needed inthe conditions in which the aircraft will be own. The materials that make up a transistor that is part of a microchip that runs the internal computer system also need to be of acertain composition, be a certain thickness, and exhibit speci c properties in order toperform as needed in the conditions in which the aircraft will be own. The importantdistinction here is that the degradation mechanism that leads to the failure of the wingis different than the degradation that leads to failure of a transistor. The environmentthat the wing needs to be designed to endure is different then the environment that thetransistor is designed to endure. This is because the wing and the transistor have different purposes and different designs, and are constructed at different scales, all contributingto the continued function of the aircraft.
Thus, considering a material sustainment strategy for an aircraft requires identifying the role that each component part plays in ensuring the overall function of the airplane. Thismeans identifying the operating environment to which each part will be exposed, and identifying the different types of phenomena in each environment that can lead to thedegradation. Because the parts of an airplane range in scale from nanometers to me-ters, the sources and mechanisms of degradation will be different for the different parts. ust as humans cannot “step on” bacteria to kill them, the mechanisms that degrade
some materials may not affect others because they act at different scales.
This atomic effects corrosion (AEC) study revealed that a spectrum of corrosion effectsexists. Attempting to categorize degradation events in the nucleus of an atom in chemi-cal terms only, such as the energy required to disrupt a molecular bond, is incorrect.Therefore, limiting corrosion to the classical effects that occur at the scale of chemical interactions between molecules is insuf cient. Recognizing this fact is not a new idea,but characterizing corrosion as the degradation effects at multiple scales throughoutthe corrosion spectrum offers increased opportunities to prevent, detect, predict andmanage corrosion. It is important to note that the corrosion spectrum concept needs to be studied further and better de ned. Our description here provides a starting point for AEC, and in the next phase of our study we will address biological effects corrosion.
What matters most in material sustainment is being able to understand the ways thatmaterials can degrade. We contend that as materials become more complex, there aregoing to be more ways in which materials can degrade. The goal of material sustain-ment is to identify as many of the degradation pathways as possible for all materials,then develop strategies for detecting and preventing degradation, and nally to de-velop solutions for material degradation. Researching how degradation pathways work together to create failures in materials through processes that are not yet thoroughly understood offers opportunities to develop new solutions. Materials degrade through combinations of spontaneous degradation, high-energy, low-energy, and eld effects.Focusing on single mechanisms of effects is important, and we applaud the body of re-
86 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
search that has been amassed to date, but we assert that understanding how combina-tions of effects cause degradation is also important. Studying the full spectrum of degra-dation pathways and developing solutions to them such as “bottom up design” can increase the con dence our Service personnel have that the systems and infrastructure they depend on are reliable and functional.
The point of this book has been to make the case to decision-makers and stake-holders in the design, acquisition and sustainment of material systems that materi-als degradation should be considered as a spectrum of degradation pathwaysdependent on several factors:
• The nature of materials
• The types and sources of degradation events
• The thresholds of degradation events that compromisea material’s function or reliability.
The classical de nition of corrosion worked well in the industrial age, but is insuf cient in the modern age. For this reason, we proposed the corrosion spectrum that includes atomic level (AEC), molecular level (classical corrosion), and macromolecular level(biological) effects. To ensure that DoD systems and infrastructure are ready when our Service personnel need them, corrosion mechanisms and effects across this spectrumneed to be determined so the CPO can cor-
rosion in all forms, and thereby promote material sustain-ment. Investigating the corrosion spectrum requires newresearch to identify new mechanisms and combinations of mechanisms resulting in materials degradation, thereby enabling science-based policy changes, managed with a strategic plan for developing and coordinating solutions that increase system and infrastructure reliability, and re-duce sustainment costs.
What matters most inmaterial sustainmentis being able to understand theways that materialscan degrade.
APPENDIX science of materials
This appendix discusses the science of materials. We also discuss the importance of un-derstanding how a material’s composition and structure are interconnected, and how these interconnections lead to the properties that give materials their capabilities. To demonstrate this point, we collect and overview science related to atomic effects cor-rosion (AEC). This appendix is not intended as a “textbook” there are many textbooks and other resources available that delve deeply into various topics synopsized here, and several of these resources are referenced. Rather, its purpose is to provide the scienti c rationale for thinking about materials at all scales, considering all structures, and relating this information to their properties. Thus, this appendix brie y describes the foundational scienti c concepts required to understand AEC mechanisms. This discussion is intended to demonstrate that AEC is a largely ignored area of degradation in corrosion preven-tion and control (CPC) strategies, and to illustrate how understanding AEC mechanisms can enable a more thorough investigation of materials degradation in order to prevent, detect, predict and manage corrosion across the spectrum.
the scientific principles of aec
A material is de ned as “the elements, constituents, or substances of which something is composed or can be made.”1 The eld of materials science and engineering attempts to understand the intricate details of the forms of matter (materials) we use to build technologies and structures.2 Until the invention of instruments like the scanning probe microscope (such as the example in the gure on page 88), a “top-down” science ap-proach has been used to study the properties of materials.3 Materials have mostly been studied with little information available about the precise arrangement of atoms. This new ability to study the underpinning science, and apply it to engineer materials at the nanoscale is revolutionizing our understanding of materials and their capabilities.4 In the very near future we will see materials with new properties that outperform older materi-als. In addition, these materials will provide economic and environmental ef ciencies as processes such as additive manufacturing mature.5 These new materials offer the potential for new capabilities that can be applied to improve society and better protect the United States of America.
1. “ aterial,” Meriam We ster, Accessed 09 Sept 2015, p: . erria - e ster.co dic onary aterial.2. “ aterials Science,” Wi ipedia, odi ed 20 Sept 2015, ps: en. i ipedia.org i i aterials science.3. “Scanning pro e lit ograp y,” Wi ipedia, odi ed 13 uly 2015, Accessed 25 Sept 2015, ps: en. i ipedia.
org i i Scanning pro e lit ograp y.4. ar uis, E anuelle A. et al. “Nuclear reactor aterials at t e ato ic scale.” Materialstoday 12, no. 11 (2009):
30-37.5. “Co pany to E plore Nanocar on as or ing aterial,” ano er e s, 07 ct 2013, Accessed 25 Sept 2015,
p: .nano er .co ne s2 ne sid 32643.p p.
88 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The emergence of new technologies requires an increased understanding of their sci-enti c foundation so as to identify and mitigate mechanisms of degradation. Planning for a material’s life cycle requires approaching material structures from the “bottom up.” A bottom-up approach means understanding how the atomic structures of materi-als at the nanometer scale lead to the properties we observe at the microscopic and macroscopic scales. If we do not understand how a material is put together, how can we plan to mitigate the ways it may fall apart For certain materials, the uses do not require a precise understanding of a materials underlying atomic structure because the engineered macrostructures serve their purpose without this knowledge. For ex-ample, steel beams have been around for decades, and we can con dently say it is not necessary for every atom to be placed perfectly because we have experience in the application of steel beams. But as nanoscale devices such as microelectron-ics and micro-electromechanical systems (MEMS) continue to advance, to maintain technological superiority, the DoD will need to consider new materials with optimized atomic structures to create macroscopic properties that support the development of new technology-enabled capabilities.
The periodic table categorizes the known elements, which are generally segmented into metals and non-metals. Materials are typically classi ed into four categories known as metals, ceramics, polymers, and composites.6 Metals include all the metallic elements, such as iron (Fe), aluminum (Al), copper (Cu), and titanium (Ti), and these are always found in orderly atomic arrangements. Ceramics are typically ionic (sometimes cova-lent) compounds composed of non-metals and metals. These include metal oxides,
6. “General aterial Classi ca ons,” DT Resource Center, Accessed 08 Sept 2015, ps: .nde-ed.org Educa-onResources Co unityCollege aterials Introduc on classi ca ons. t .
Overview of the main types of Scannig Probe Microscope types/Kristian Molhave/ Opensource Handbook of Nanoscience and Nanotechnology
nitrides, and carbides.7 Silica is an example of a ceramic that is composed of a mol-ecule containing a metal silicon (Si) atom bound with two non-metal oxygen (O) atoms. Polymers are typically associated with organic molecules (i.e., containing carbon (C), hydrogen (H), oxygen (O) and other non-metals). Plastic and rubber materials are poly-mers. Polymers are distinct from metals and ceramics in that they have large molecular structures that contain a backbone of covalently bounded C atoms.8 Composites are hybrid materials that contain elements of metals, non-metals, and polymers. Table 1 summarizes the characteristics of metals, ceramics, polymers and composites.
Table 1: Comparison of material classi cations.
BONDING TYPE PROPERTIES
Metals MetalsMetallic and Covalent (occasionally)
Strong, High electrical and thermal conductivity, malleable, ductile, sensitive to corrosion.
Brittle, insulating, resistant to heat and corrosion,
Polymers Non-metals Covalent
Properties range widely from hard to soft, brittle to elastic, usually insulating, and resistant to corrosion
Longevity of Non-metals Metalsharsh Environments
Metallic, Ionic, Covalent
Combinations of the previous three material types. Properties range widely based on ma-terials combined.
Each of these material types is classi ed according to certain chemical and physical properties. Those properties are dependent on their atomic and molecular structures. The relationships between the atomic structures of materials and the properties they exhibit are what materials scientists and engineers study. To develop new technologies or systems, material scientists and engineers need to understand the intended capabili-ties, and the associated underpinning chemistry and physics that provide the desired properties to achieve those capabilities. This requires understanding the fundamentals of the elements and the forces that control their behaviors and structures. ust as a painter’s ability to create beautiful works of art depends on his/her knowledge of paints, a material scientist or engineer is limited to the kinds of materials he/she can create by the knowledge of atoms and molecules in essence, a material scientist’s or engineer’s paints are the elements on the periodic table.
7. “Cera ic,” Wi ipedia, odi ed 13 Aug 2015, Accessed 23 Sept 2015, ps: en. i ipedia.org i i Cera ic.8. “Poly er,” Wi ipedia, odi ed 24 Sept 2015, ps: en. i ipedia.org i i Poly er.
90 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
With the complete understanding of the chemistry and structures that give materials their capabilities, the properties of materials can be ne-tuned to meet speci c require-ments. The eld of materials science and engineering breaks down material properties into six categories: mechanical, electrical, thermal, magnetic, optical, and deteriorative.9 A material’s capabilities depend on the types of elements that make it up and the ordered arrangement (i.e., structure) of these elements (as atoms, ions, or molecules). From a material sustainment standpoint, it is important to understand exactly how the fundamental properties of materials come into existence and why. The answer to “why” allows the material scientist or engineer to design a material for a speci c function and understand how that same arrangement could degrade. It is important to recognize all the possible characteristics of a material rather than those required for a particular capability: this knowledge makes it possible to predict and understand how a material might degrade in different environments or when used in manners different than origi-nally designed.
thermodynamics of materials
Thermodynamics is the study of energy ow between a system and its corresponding surroundings. The mathematics that explain thermodynamics are available in numerous textbooks here, we provide a generalized description of the principles that matter fol-low.10 In order to understand the basic driving forces that explain why materials conform to certain con gurations and take on speci c properties, it is important to understand the forces that affect the behavior of those materials.
There are four laws of thermodynamics, as depicted in the gures on page 91, that de-scribe the behaviors of matter and energy.11 They also de ne the fundamental physical quantities known as temperature, energy, and entropy that characterize all thermody-namic systems. The “zeroth” law of thermodynamics states that any two systems that are in thermal equilibrium with a third system are also in thermal equilibrium. This law is critical to a proper understanding and derivation of the concept of temperature. The rst law states when energy passes into or out of a system, either as work, heat or mat-
ter, the internal energy of the system must change in accordance with the law of con-servation of energy. This means it is impossible to invent a machine that runs without added fuel (energy): perpetual motion machines of the rst kind are not possible. The second law of thermodynamics states that it is impossible for a system to undergo a cyclical process where its sole effect is the ow of energy into the system from a heat reservoir and the performance of an equivalent amount of work by the system on the surroundings.12 Another way to say this is that any exchange of energy between a system and its surroundings must result in an increase in disorder of the universe. This concept is known as entropy, which is one of the fundamental laws that applies to the science of degradation. Materials represent ordered arrangements of matter, and the second law
9. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
10. For a ore detailed descrip on see: o as Engel and P ilip Ried, P ysical C e istry (Pearson Educa on, Inc: 2006).
11. id.12. o as Engel and P ilip Ried, P ysical C e istry (Pearson Educa on, Inc: 2006).
of thermodynamics essentially says that even the most stable arrangements of matter are temporary in the grand scheme of things all things degrade and return to a more disordered state. The third law of thermodynamics states that the entropy (i.e., level of disorder) of a system is well de ned when it holds the minimum amount of energy it can. This minimum energy state is then de ned as an absolute zero temperature a system does not “move” at absolute zero. The third law is not directly relevant to the discus-sion of materials degradation, beyond establishing a temperature scale and giving that scale a oor.
In order for any system to change spontaneously, the system must enter a more stable state.13 What this means is that the potential of a system to change is a re ection of the stability of the energy distribution of a system.14 If there is a more stable way to distribute
13. id.14. Note: ere energy o a syste enco passes t e energy o eat, or , and a er.
0. Three atomic systems in thermal equilibrium with each other demonstrating the zeroth law.
1. Energy (E1) is added to a system with an internal energy (E2) to give a new system with an energy that is the sum of E1 and E2
demonstrating the 1st law of thermodynamics.
2. A system de ned by an ordered lattice structure becoming more disordered as time increases
demonstrating the second law of thermodynamics.
3. An atomic system that demonstrates the3rd law of thermodynamics by showing that as the temperature approaches 0Kthe atoms in the system stop vibrating.
Four Laws of Thermodynamics./Alex Taliesen
92 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
the energy in the system, then the system will do so until it reaches a state known as equilibrium.15 At equilibrium, the net exchange of energy between the system and its surroundings is zero. The spontaneous transition of a system from one state to another results in the release of energy from the system to the surroundings. This phenomenon is mathematically expressed in thermodynamics as Gibbs free energy, shown in its simplest form below:
For any potential process involving matter and energy change/ ow, the change in Gibbs free energy ( G) can be approximated using this equation (or more complex variations of it16) with various known constants and measurements. The change in Gibbs free energy is the difference between the change in a term known as enthalpy ( H), which describes the change in internal energy of a system, and a term that describes the change in the entropy ( S) of the system at a particular temperature (T). In order for a system to change spontaneously this difference has to result in a nega-tive Gibbs free energy. If a system does not change, then it does not contain enough energy to overcome either an enthalpic and/or entropic energy barrier. If a system does change it is because a more stable future state became possible, or because energy has been added to the system (e.g., by heating) such that the system can overcome imposing energetic barri-ers. The degradation of a material at any scale can therefore be viewed as the result of a thermodynamic pro-cess, and the laws of thermodynamics state at least two things: materials will degrade naturally over time due to the driving force of entropy, and materials can degrade when phenomena cause energetic changes to that system (or the surroundings act on the system).
15. o as Engel and P ilip Ried, P ysical C e istry (Pearson Educa on, Inc: 2006).16. id.
All atoms can spontaneously degrade over time, though for many it is highly unlikely. For those that do (e.g., 234U or 214Pb),17 this phenomenon can create a problem when the decaying atoms are a part of or near certain types of materials. The decay of an atom results in the spontaneous release of energy, which can cause changes to the atomic properties of neighboring atoms. Such changes could, for example, help facilitate the diffusion of atoms within crystal lattice structures of a material. A change in the lattice structure could be all that is needed to ensure a loss of desirable capabilities of that material. ust as a tower of blocks can fail if one block is removed, materials can fail because a single atom moves. Atomic effects corrosion (AEC) happens when material failure begins at the atom. Understanding the phenomena that cause degradation to the atomic and molecular structures of materials is at the core of what is important when it comes to AEC.18
properties of materials
We introduced the six commonly referred to materials properties in the eld of materials science: mechanical, electrical, thermal, magnetic, optical, and deteriorative. In this section, we discuss each property as it relates to atomics effect corrosion. Deteriorative properties are referred to throughout this discussion.
Mechanical properties refer to a material’s ability to remain in a particular atomic, micro, and/or macro con guration when a particular load or force is applied to that material for a speci ed amount of time, in a particular environment, and in a particular way. For mechanical properties, there are standardized measures used to communicate relative magnitudes of effects when discussing them. The American Society for Testing and Ma-terials (ASTM) is one of the more active organizations in cataloguing the results of many standardized tests made to materials to determine their mechanical properties.19
There are many mechanical properties that are considered in selecting materials for an intended design, and we do not propose to explore each in depth here. Brie y, the most im-portant mechanical properties refer to a materials strength, stiffness, hardness, ductility, plasticity, and toughness.20 These are measured in several standard ways, including fracture toughness, tensile strength and Poisson’s ratio. The fracture toughness measures how much energy a material can absorb
17. “Radioac ve ecay,” Wi ipedia, odi ed 24 Sept 2015, Accessed 09 Sept 2015, ps: en. i ipedia.org i iRadioac ve decay.
18. E anuelle A. ar uis, “Nuclear reactor aterials at t e ato ic scale,” Materialstoday 12, no. 11 (2009): 30- 37.19. “A out AS Interna onal,” ASTM nterna onal, Accessed 28 Sept 2015, p: .ast .org.20. For a ore detailed descrip on o t ese proper es see: illia . Callister r. and avid G. Ret isc , unda
mentals o Materials Science and Engineering An ntegrated Approach ( o o en, N : o n iley Sons, Inc,2012).
The most commonly used
material properties are mechanical,
electrical, thermal, magnetic, optical and deteriorative.
94 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
per unit area before it fractures tensile strength measures how much stretching stress a material can withstand before it fails Poisson’s ratio is simply the ratio of lateral to axial strain. These properties re ect the resiliency of material to change when different types of stresses are applied.
For example, if you wanted to test the mechanical properties of steel beam you could try to crush the beam (compression test), you could apply a load in the middle of the beam to see how much weight it can support, or you could try to elongate the beam. Materials engineers conduct various tests based on the intended usage of the material. The goal in determining a material’s mechanical properties is to simulate the environ-ment in which it will be used in order to learn how those mechanical properties might hold up or degrade over time.
What is important from the perspective of AEC is understanding how these mechani-cal properties emerge from the atomic structures of materials. For example, for plastic deformation, which is the permanent deformation of a material after release of an ap-plied load, we know that bonds of the atomic structure are broken between neigh-boring atoms and then reformed with new neighbors.21 This means atoms have been displaced from their original position to occupy a new position within the material. These new atomic arrangements can result in the loss of the original mechanical properties and the establishment of a new set of mechanical properties the new properties may not be suitable for the needs of that material.
From a design perspective, it should be obvious that not all atom displacements are equal, and that altering the location of atoms in a large crystal lattice will have different impacts depending on the criticality of those atoms to the overall desired mechanical properties of the material. This is why it is important to study mechanical properties at the atomic scale.22 For example, mechanical properties are often observed to degrade through “wear and tear.” Discovering that a single atomic displacement could be the catalytic event to total system collapse of a particular mechanical property could be
a major advance in designing materials that withstand wear and tear for much longer. Current research is ex-ploring how certain nanomaterials such as graphene can reduce the wear on materials23 and how understanding nuclear reactor materials at the atomic scale could lead to stronger, more reliable nuclear infrastructures.24 If me-chanical properties are understood from the bottom up, then the predictive models for failure and additional deg-
21. id.22. iadong an, et al. “In situ ato ic scale ec anical icroscopy discovering t e ato is c ec anis s o plas c-
ity in nano-single crystals and grain rota on in polycrystalline etals,” ltramicroscopy 151 (April 2015): 94-100.23. Evan Lerner, “Nanotec ear and ear, Ato y Ato ,” niversity o ennsylvania, 4 Fe 2013, p: .
uturity.org nanotec - ear-and-tear-ato - y-ato .24. E anuelle A. ar uis, “Nuclear reactor aterials at t e ato ic scale,” Materialstoday 12, no. 11 (2009): 30-37.
What is important from the perspective of AEC is understanding how mechanical properties emerge from the atomic structures of materials.
radation pathways (such as traditional corrosion) can be made more accurate. These models can then be used to create better, longer lasting materials, and reduce the incidence of unexpected failures.25
Technologies such as microelectromechanical systems (MEMS)26 and nanoelectrome-chanical systems (NEMS)27 systems paired with visualization technologies such as the scanning probe microscope28 allow materials scientists to study the atomic properties of materials more precisely. Materials scientists and engineers thus learn how the atomic properties of materials translate into the micro- and macroproperties of materials.29 This kind of bottom up understanding can also improve our ability to predict failures.30 As technology evolves the need for smaller materials on the nano- and microscales is going to increase. MEMS and NEMS will have materials that act as sensors, actuators, electron-ics, and as structural elements to create the capabilities needed for new technologies. The environmental forces that act on materials at these scales are different, and thus the properties of such materials will be different than the properties observed at the macro scale. The decay, diffusion, or displacement of an atom through some force or process can result in serious consequences to the mechanical properties of materials at much smaller scales. With better bottom-up understanding applied in the design approach, such atomic effects can be predicted and prevented to ensure materials perform reli-ably and effectively.
The electrical properties of materials depend on their composition and structure.31 As with other properties, standardized measures are used to describe electrical properties, such as electrical conductivity or resistance.32 Electrical properties are characteristic of how the material’s atoms respond to an applied electric eld. An important property for many solid materials is its ability to transfer an electrical current over some distance. This property is described by Ohm’s Law, which states that the product of the current (I in Coulombs/second) through a material and the resistance of that material through which the current is passing (R in Ohms) is equal to the applied voltage ( in oules/Coulomb) causing the current.
V = IR
From this relationship, it is possible to determine the electrical resistivity and electrical conductivity of a material, both of which depend on the con guration of the underly-
25. id.26. “ at is E S ec nology ” MEMS anotechnology E change, Accessed 30 Aug 2015, ps: . e s-
e c ange.org E S at-is. t l.27. “Nanoelectro ec anical Syste s,” Wi ipedia, odi ed 1 Sept 2015, Accessed 08 Sept 2015, ps:
en. i ipedia.org i i Nanoelectro ec anical syste s.28. Sergei . alinin, Sergei, et al, “Nanoscale Electro ec anics o Ferroelectric and iological Syste s: A Ne
i ension in Scanning Pro e icroscopy” Annual Revie o Materials Research 37 (August 2007): 189-238.29. Andreas le en , et al, “Ato ic Scale ec anis s o Fric on Reduc on and ear Protec on y Grap en,”
anole ers 14, no. 12 (2014): 7145-7152.30. ar ite and osep . ernstein, “ icroelectronics Relia ility: P ysics-o -Failure ased odeling and
Li e e Evalua on,” et ropulsion a oratory (Fe 2008), ps: nepp.nasa.gov les 16365 08 102 4 20PL ite.pd
31. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
96 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
ing atomic structures of the material.33 As materials move from the nanoscale to the macroscale, like other properties, their electrical properties change because size cre-ates new emergent properties.34 A simple example is the electrical resistance of a wire: though the same materials are used, a wire with a smaller diameter will have more re-sistance than a larger wire made of the same material (e.g., copper and other alloyed metals). The electrical parameters of a material like silicon at the macroscale do not predict the electrical properties of a silicon transistor that exists at the nanoscale. In order to properly gauge the electrical properties of a material it is necessary to study these properties on the scales that apply to their speci c designs.
Materials are able to conduct electricity because their atomic arrangements allow for the delocalization of electrons.35 Depending on the type of material, different types of bonding structures hold the material in its particular atomic and electronic geometries. These geometries orient themselves such that the valence electron orbitals are in the most stable con guration according to thermodynamic predictions. Forcing atoms into dense spaces, for example, can lead to the creation of unique orbital con gurations that allow for the delocalization of electrons (see gure below).36
Forcing atoms into dense spaces can lead to the creation of unique orbital con-gurations that allow for the delocalization of electrons/Alex Taliesen
In metals, the atomic bonding scheme is metallic, which means that there are minimal restrictions to the number and positions of neighboring atoms.37 Consequently, there are many different packing schemes for metallic crystal structures and each has its own unique properties as a result. Additionally, different metals with the same basic lattice-
33. id.34. “ at s So Special a out t e Nanoscale,” ano.gov, Accessed 07 Aug 2015, p: .nano.gov nano-
tec -101 special.35. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Ap
proach ( o n iley Sons, Inc, 2012).36. . . Gra a Solo ons and Craig . Fry le, rganic Chemistry Eighth Edi on ( o n iley Sons, Inc.,2004).37. E. Cat erine ousecro and G. Alan S arpe, norganic Chemistry (Pearson Educa on Li ited, 2001).
packing scheme (e.g., face-centered cubic) will have distinct electrical properties due to different atomic properties such as electronegativity. Because the electrical proper-ties of metals depend on the precise arrangement of the crystal structures of the materi-al, any impurities, vacancies, self-interstitial atoms, dislocations, or other types of defects in the lattice structure of a material will alter that material’s electrical properties.38 The smaller the material, the more one of these defects will impact the electrical properties of that material. These defects, for example, change energy band gaps, which are the energy gaps between where an electron is currently occupied in an orbital and the energy it would need to participate in a conduction process.39
For materials whose capabilities heavily rely on their ability to conduct, insulate, or par-tially conduct electricity, ensuring the integrity of the atomic structures is important. For example, microelectronics rely on materials with speci c electrical properties that must be stable over time to function effectively. The materials in modern microelectronics are nanomaterials such as transistors or interconnecting wires, which means that even a sin-gle-atom change in the atomic structures of these materials can alter their electrical properties, and thus result in loss of designed capability. The gate is a critical component of modern day MOSFET transistors current gate sizes are less than 22 nm in size.40 At this scale, the behavior of materials is governed more by quantum mechanical than bulk mechanisms certain materials, such as the quantum tunneling diode,41 rely on incredibly ne-tuned band gaps to operate precisely. As technology becomes more dependent
on nano- and micromaterials with speci c electrical properties, it is becoming impera-tive to develop new solutions to ensure their integrity in operation. The inner workings of a personal computer are always in a relatively “safe” environment. However, computa-tional technologies are being employed in weapons in much harsher battle eld environ-ments weapon-control computers are therefore exposed to very different types of stresses than personal laptops.42
The basic science underpinning materials’ electrical properties is well understood from the atomic scale up. As materials engineers design new materials with unique electrical properties, and these proliferate in technolo-gies with advanced microelectronics, we need to ensure they can function throughout their design life cycles. This will require developing better understanding of how AEC degradation that acts on individual atoms can be miti-gated or prevented.
38. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
39. “ and Gap,” Wi ipedia, odi ed 29 Aug 2015, Accessed 14 Sept 2015, ps: en. i ipedia.org i i and gap.40. “22 Nano eter,” Wi ipedia, odi ed 10 Sept 2015, Accessed 14 Sept 2015, ps: en. i ipedia.org i i 22
nano eter.41. “ unnel iode,” Wi ipedia, odi ed 19 Sept 2015, Accessed 15 Sept 2015, ps: en. i ipedia.org i i un-
nel diode.42. C. odd Lope , “ 25 Counter e lade arget Engage ent Syste ay Lose y Ne t August,” SA Army, 9
Aug 2013, p: .ar y. il ar cle 109049 25 Counter e lade arget Engage ent syste aylose y ne t August .
As technology becomes more dependent on
nano- and micromaterials with speci c electrical
properties, it is becoming imperative
to develop new solutions to ensure their
integrity in operation.
98 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Thermal properties refer to how a material responds when heat is applied.43 These properties are typically described with measures such as heat capacity, coef cient of thermal expansion, thermal stress, and thermal conductivity. Heat is a thermodynamic expression for energy transfer through non-directional mechanisms. Heat’s counterpart, work, is the transfer of energy with a vector component, meaning it is typically the ow of energy against or in the direction of an applied eld. As materials absorb heat, the overall temperature of the material rises. The energy added to the material can be ab-sorbed to excite vibrational, translational, and electronic energy levels characteristic of the atoms in the material and their bonding scheme. The amount of heat that a material can absorb before the material’s temperature rises by a particular unit of temperature is known as the material’s heat capacity and is typically expressed in units of /mol- K. The heat capacity of a material refers to the tolerance of that material to added heat. High heat capacities (e.g., silica molar heat capacity 42.2 /mol- K)44 mean the mate-rial can absorb a lot of heat before the temperature of the material begins to rise the opposite is true for low heat capacity materials.
One of the reasons the temperature rises in heated materials is because the added heat causes the atoms within the material’s crystal lattice to vibrate more. The science that describes this phenomenon is quantum mechanics.45 All atoms in any lattice structure regardless of composition are vibrating at high frequencies with low amplitudes. This is the reason instruments such as infrared (IR)-spectrometers can identify various func-tional groups within molecules.46 This instrument detects these vibrational, rotational, and translational frequencies, and a trained chemist can discern the various functional groups based on the spectra produced from the spectrometer. The vibration of atoms in a material causes them to radiate heat. If something is room temperature, it means that the atoms have reached thermal equilibrium with the room, and are vibrating such that heat they give off is equal to the heat they are absorbing. Added heat causes the vibrations to increase, or occur faster, leading to more heat being given off and the temperature of the material rising. It is important to realize that these are not random, but coordinated, vibrations in a material such that the lattice vibration is almost wave-like (i.e., as phonons see gure on page 99). As the vibrations become more intense, the material begins to experience more stress to its underlying lattice structure. When the added heat becomes to great, the lattice can begin to slip or fall apart.47
43. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
44. “ eat Capacity,” Wi ipedia, odi ed 17 Sept 2015, Accessed 20 Sept 2015, ps: en. i ipedia.org i ieat capacity.
45. o as Engel and P ilip Ried, hysical Chemistry (Pearson Educa on, Inc. 2006).46. id.47. ragica asiles a, aterina Raleva, and Step en . Goodnic ,” ea ng E ects in anoscale Devices, p: cdn.
intec open.co pd s- 10114.pd
ibrations of atoms/Alex Taliesen
The ability of a material to maintain its structure upon the addition of heat is depen-dent on the composition and atomic structure of that material. These two factors are responsible for the micro and macro properties observed as materials are scaled up from the atomic level. In addition to potentially melting, most materials expand upon the addition of heat because the spacing between atoms in the lattice structures gets larger.48 This occurs because the added heat increases the vibrational energies of those atoms. For each type of material, the greater atomic bonding energy associated with its atomic structure will give rise to an increase in interatomic separation for a particular rise in temperature. The continued heating and cooling of a material can, therefore, result in mechanical stresses being applied to the material. These stresses can create the same types of defects normally associated with mechanical stress. The continued thermal expansion and contraction of a material can cause that material to warp, fracture, or elongate.
The response of a material to applied heat can also be similar to what is observed when an electric eld is applied to a material. Materials can transfer heat through bond vi-brations or through the transfer of electrons. The size of the material affects the impact
48. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
100 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
that single atomic changes (for example, transfer of an electron) will have. Scientists and engineers use knowledge of how the atomic underpinnings of a material lead to its thermal properties to design materials with improved capabilities. Knowing how environ-mental heat cycles can accelerate mechanisms such as decay, diffusion, displacement or other atomic changes will become increasingly important as we design smaller-scale technologies such as nanomaterials.
Magnetic properties refer to the response of material when subjected to an applied magnetic eld. Certain materials exhibit magnetic properties regardless of whether or not a magnetic eld is applied. These properties are described and measured in terms such as magnetization, magnetic ux density, and permeability. Magnetic proper-ties are a consequence of the composition of the atom.49 Magnetic elds arise when charged particles move through space, so in an atom an electron can generate two potential magnetic elds, as shown in the gure, page 101. Because the electron is charged and orbiting the nucleus (note that the descriptions in this paragraph are sim-pli cations the actual behavior is more complex at the quantum mechanical level)50 it can be thought of as a small current loop that creates a very small magnetic eld in which the magnetic moment is oriented along its axis of rotation. Additionally, each electron spins around its own axis, so this magnetic moment is directed along the cor-responding spin axis. An easy comparison is to imagine the earth is an electron and the sun the nucleus. The earth revolves (spins) around the sun creating a magnetic moment, and the earth also rotates (spins) on its own axis creating another, different magnetic moment. Every electron in an atom acts like a small magnet: each electron has both a permanent orbital and spin magnetic moments.51
Magnetic moments from electrons in an atom tend to cancel: every spin “up” that is paired with a spin “down” electron cancels the pair’s net magnetic moment. The same is true for orbital moments. An atom’s net magnetic moment is the sum of the orbital and spin magnetic moments of all its electrons pair cancellations reduce the overall net mo-ment. Thus, different magnetic properties will manifest depending on the electron con-gurations of atoms. Furthermore, as atoms form molecules or become parts of larger
aggregate structures, such as in a crystal lattice, new magnetic properties characterize those structures.52 This gives rise to the phenomena of diamagnetism, paramagnetism, ferromagnetism, antiferromagnetism, and ferrimagnetism.53
49. o as Engel and P ilip Ried, hysical Chemistry (Pearson Educa on, Inc. 2006).50. “ o r-van Leeu en eore ,” Wi ipedia, odi ed 3 an 2015, Accessed 18 Sept 2015, ps: en. i ipedia.org
i i o r van Leeu en t eore .51. “Spin agne c o ent,” hysics orums, 2 ct 2014, ps: .p ysics oru s.co t reads spin- agne c-
o ent.773970 .52. Ro in F.C. Farro , et al. Magne sm and Structure in Systems o Reduced Dimension, (Plenu Press, N : 1993).53. “ agne s ,” Wi ipedia, odi ed 10 Sept 2015, Accessed 28 Sept 2015, ps: en. i ipedia.org i i agne-
At the micro scale, structures known as magnetic domains exist. Regardless of whether or not the material has a permanent magnetic dipole, the various domains of the mi-crostructure can be aligned differently, and this alters the magnetic properties of the material.54 An applied eld can align the domains. How strong the eld needs to be in order to achieve alignment is a function of the magnetic properties of the particular ma-terial. This property is important in the function of devices such as soft magnets because the applied eld might reorient the domains with little heat loss. Hard magnets, on the other hand, require much stronger elds and when their domains are reoriented there is greater heat loss. For these reasons, materials with either soft or hard magnetic properties are selected for speci c purposes.
Magnetic properties are utilized in microelectronics for information storage.55 In hard disk drives or magnetic tapes, information is stored by creating unique patterns of magne-tized grains in materials such as cobalt-chromium alloy. Storage typically requires a com-mon magnetization of about 100 grains.56 This encompasses many atoms, but technolo-gy advances are making it possible to store information on structures that are smaller.57
54. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
55. “ agne c Storage,” Wi ipedia, odi ed 12 Sept 2015, Accessed 24 Sept 2015, ps: en. i ipedia.org i iagne c storage.
56. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
57. ua uan and avide E. Laug lin, “Grain Si e Reduc on or Perpendicular agne c Recording edia Using anAr-ion Etc ed Ru Seedlayer,” Applied hysics e ers 93 (2008).
Magnetic moments from orbital movement and spin/Alex Taliesen
102 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The smaller these structures get, the more sensitive they will become to changes in the underlying atomic structures of the materials that make up the storage medium. The magnetic properties of materials thus play an important part in the electronics domain, as well as other domains where electronic information needs to be safely and perma-nently stored.
Understanding the impact changes in the atomic structures and composition might have on these properties is critical in ensuring the reliability of designs using magnetic mate-
rials. Ferrimagnetic materials typically rely on unique con-gurations of atoms to ensure a net magnetic moment and
lower cancellations. The degradation of materials through atomic effects can change such con gurations, and po-tentially result in the failure of that material. Materials exist today for which magnetic properties at the nanoscale are important the use of such materials is going to increase in the future. Understanding the degradation that can occur through AEC will be key in ensuring these existing materials are reliable.58
Optical properties of materials are those that cause a material’s property to change due to interaction with electromagnetic radiation, or cause electromagnetic radiation to change upon interaction with the material in the “light” regions of the electromagnetic spectrum (infrared, visible, ultraviolet). If a material has optical properties it means it can alter, be altered, or do both upon interacting with electromagnetic radiation. The ability of a material to re ect, refract, absorb, transmit, or change via interaction with electro-magnetic radiation depends on the composition and atomic crystal lattice structure of a material. The particular nature of the lattice and the atoms, ions or molecules con-tained within it will determine the various quantized energy levels for the matter’s ability to interact with light.59 When absorption occurs, it is because an electron has absorbed the energy of a photon that is equal the energy difference between its ground state and a quantized excited state. When light passes through a material it is because it did not contain the right energy needed to match the ground to excited state energy band gap. The type of atom and its atomic con guration determines these quantized energy levels for the optical properties of materials.
Metals are for essentially opaque to all electromagnetic radiation on the low end of the electromagnetic spectrum and transparent to high frequency radiation such as gam-ma. Metals are able to absorb most photons in the regions of the electromagnetic spec-trum called “light” because of the wide range of excitable electron energy states they
58. Pui- a a, C. . oo, and S.L. udarev, “Spin-La ce yna ics Si ula ons o Ferro agne c Iron,” hysics Revie 85, No.18 (1 ay 2012).
59. o as Engel and P ilip Ried, hysical Chemistry (Pearson Educa on, Inc. 2006).
Understanding the impact changes in the atomic structures and composition might have is is critical in ensuring the reliability of designs using magnetic materials.
have available. Changes to the atomic structures of metals that alter the energy band gaps for absorption change their optical properties. Most metals are highly re ective their ability to re ect light with nearly the same frequency and number of photons as the incident light is an important property for systems designed to transmit light. Non-metals tend to be more transparent to light due to the nature of their energy band distributions. Thus, materials containing non-metals absorb, re ect and transmit light differently.
Optical phenomena are important to materials scientists and engineers looking to cre-ate new technologies.60 The concept of photoconductivity combines knowledge of the atomic properties of materials such as semiconductors with the knowledge of how electromagnetic radiation can change those properties to create technologies like the solar cells.61 Understanding the electroluminescence properties of materials allows for the development and use of light emitting diodes.
The rubies we use in lasers are a ceramic composed of sapphire (Al2O3) and around 0.05 Cr3+ ions. Doping sapphire with chromium +3 ions provides speci c electron states to the ruby lattice that are critical to its ability to act as a laser (see Figure 7).62 Once the ruby laser has been appropriately processed, the excitation of electrons within the ruby lattice is achieved via a xenon ash lamp. At that point, two things happen: Some Cr3+ electrons get excited and decay back directly to their ground state, and some Cr3+
electrons decay to a metastable state that exists for approximately 3 ms. The result is that many electrons in the ruby occupy this metastable state simultaneously.63 This meta-stable state eventually avalanches, and due to the design of the apparatus containing the ruby rod crystal, results in the emission of a high-intensity, coherent laser light beam. There are many other types of materials used for lasers, and the same principles apply. Such technologies rely heavily on the precise nature of the atomic lattice structures of materials to provide useful optic properties.
60. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
61. arco . Furc i, et al., “ ec anis s o P otoconduc vity in Ato ically in oS2,” ano e ers 14, no. 11 (2014): 6165-6170.
62. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
104 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Changes to the atomic lattice structures of materials used for their optical properties can be impacted by AEC. Optical properties are a consequence of quantum mechanical phenomena that depend on the atoms and their atomic con gurations that make up a material. Many optical properties that require absorption depend on speci c energy band gaps that exist between ground state electrons and unoccupied atomic/molecu-lar orbitals within the material. AEC can directly impair such energy band gaps through disruption of the crystal lattice. AEC can also accelerate the degradation of optical properties by acting as a catalyst for the loss of order within a structure (e.g., help cata-lyze diffusion).
Basics of Metals
Metals make up the majority of the elements on the periodic table (see gure page 105).64 The alkali earth metals are found in columns IA and IIA on the table. The electron con guration for these elements puts the valence electrons in an s-orbital at one energy level higher than the last full valence shell. The chemical properties of these elements re ect this situation, and they often ionize to take on noble gas electron con gurations. This allows them to form stable salts with non-metals in columns IA and IIA.
The transistion metals and the metals/metalloids in columns IIIA and I A are also impor-tant materials. The transistion metals’ electron con gurations put their valence electrons into a d-orbital, and the chemical properties of the transistion metals re ect this valence structure. Transistion metals are good conductors because the valence d-electrons are loosely bound, making it easier for the electrons to delocalize. For the same reason these metals have low ionization energies in general, allowing them to take on multiple oxida-tion states relatively easily.65 They are generally electropositive, meaning willing to give up electrons. This ability allows them to form a range of ionic or partially ionic com-pounds. Most of the transistion metals mix well because they all have similar atomic sizes (although relatively large) making it easier to replace one another in a crystal lattice.
When pure metals are mixed with another metal or non-metal they are called alloys, and experience different properties than pure metals the periodic table shows some of the properties of metals and non-metals. Brass is a mixture of copper (Cu) and zinc ( n) for example. Metals typically pack into high densities, are malleable, and ductile. They exhibit different levels of strength, hardness, and other mechanical properties. The transistion metals experience a range of magnetic properties due to the nature of their available valence structures. Most metals are optically re ective. Certain metals
64. Steven S. u da l and Susan A. u da l, Chemistry i h Edi on ( oug ton ill n Co pany, 2000).65. id.
exhibit totally different properties simply because the particular temperature and pres-sure favors one crystal structure over another. Gray and white tin are an example of this phenomenon. A major problem with the transistion metals from a material sustainment standpoint is that they easily oxidize, or corrode. Thus, if metals are needed in their pure form or in a particular oxidation state that is not their highest oxidation state, materials engineers have to take precautions to achieve the desired form or state.
The electron con guration of the metals and metalloids of columns IIIA and I A have their valence electrons in a p-orbital. Due to the nature of these valence structures, these metals tend to display intermediate properties between metals and non-metals, depending on the speci c con gurations of their valence electron structure. In general, though, they exhibit many of the same properties as transition metals. Table 2, page 106 contrasts metal and non-metal properties.
Periodic Table of Elements
106 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Metals are crystalline materials, meaning that they are solid and exhibit order over a wide range of atoms.66 Consequently, solid metals are arranged in repetitive three-di-mensional patterns in which each atom is bonded to its nearest neighbors. Any material that does not form such regular order can be either non-crystalline or amorphous: in these materials, without the ordered arrangement of atoms, there is no underlying atom-ic structure to create a solid material. Some pure metals actually arrange themselves into more than one ordered arrangement depending on temperature and pressure these are known as allotropes. The particular arrangement of atoms in a metal crystal lattice gives the material speci c properties that can vary dramatically with scale.67
The crystal lattice structures of most metals are described using an atomic hard-sphere model where atoms (or ions) are considered to be spheres that touch their nearest neigh-bor atom.68 Within any lattice structure there is a repeating unit of symmetry known as the unit cell. For most crystal structures, parallelepipeds are used to describe the unit cell. The properties of a unit cell help explain why other properties of a material manifest.69
For example, closed-packed crystal structures are able to form denser materials than body-centered cubic structures. Understanding the relationship between a material’s lattice structure and its properties can help explain why impurities that distort the lattice structure lead to changes in the material’s properties. To determine the impact of AEC, then, it is necessary to understand the connection between the crystal lattice structure of a material and the properties it displays.
66. E. Cat erine ousecro , and G. Alan S arpe, norganic Chemistry (Pearson Educa on Li ited, 2001).67. id.68. id.69. id.
Table 2: Metal and non-metal properties.
PROPERTY METALS NONMETALS
Appearance Shiny Dull
DensityHigh (metals feel heavy for their size)
Low (metals feel heavy for their size)
Strength Strong Weak
Pliability Pliable Brittle
Ductility Ductile Not ductile
Electrical conductivity Good Poor
Heat conductivity Good Poor“Metals v non-metals,” BBC, 2014, Accessed 30 Oct 2015.
Metals such as gold, lead, aluminum, copper and silver all tend to be found in face-cen-tered cubic geometries with atoms located at the corners of the lattice and the centers of each face on the cube, as shown in the gure to the right. This type of lattice has a coordination number of 12 (one atom sees 12 other atoms) and an atomic packing fac-tor of 0.74. The atomic packing factor is the ratio of the volume of atoms in a unit cell to the total unit cell volume.70 This represents the maximum packing possible for spheres of the same diam-eter in a particular lattice con guration. These dense packing patterns make it easier for metals to facilitate the delocalization of electrons that gives these metals their excellent conductive properties and also provides shielding for their nuclei.
Chromium, iron, tungsten, and molybdenum tend to pack in what is known as body-centered cubic crystal structure. For this type of packing, there are atoms at each of the eight corners of the cubic structure and a single atom in the center. This gives a coordination number of 8 and an atomic packing factor of 0.68, less than the face-centered cubic crystal structure.71. This type of packing tends to be the favored packing style for metals at high temperatures, even when the cooler temperature style is close-packed. This packing style tends to lead to harder mi-crostructures and macrostructures, that are less malleable than close-packed metals.
The last common type of unit cell packing is the hexagonal close-packed, shown in the gure. Metals such as cobalt, tita-nium, zinc, and cadmium tend to pack this way. This packing, although not cubic, gives the same coordination number (12) and atomic packing factor (0.74) as the face-centered cubic structure.72
These lattice structures repsresent the atomic arrangements of pure metals and are good approximations of the actual pack-ing patterns. Their packing structures are key determinants of many mechanical, electrical, thermal, magnetic, optical, and deteriorative properties observed in metals. Mechanical engi-neers understand the importance of these lattice structures and their relationships to micro and macro material properties. By manipulating these structures through the introduction of impu-rities, material properties can be ne tuned for speci c needs. In the same way, a material’s property, especially at the na-noscale, can be fundamentally altered by atomic effects. An
70. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
71. id.72. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Ap
proach ( o n iley Sons, Inc, 2012).
Examples of crystal lattice structures.
Image Credit: Alex Taliesen
108 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
atomic interaction that fundamentally alters the state, composition, or position of a sin-gle atom in lattice can have signi cantly greater impact73 than a single or small-number event in bulk materials.
Packing structures also give rise to single crystal or polycrystalline micro- and macrostruc-tures. Single crystals are critical to modern technologies such as microelectronics, where single crystals of silicon and other semiconductors are utilized. In a single crystal, all the unit cells are interlocked so as to be in the same orientation, and thus the arrangement of atoms is repeated throughout the crystal. Current bottom-up approaches to building some nanomaterials are designed to build perfect single crystals to support the develop-ment of advanced technologies.74
Although single crystals can be found in nature, most crystals are termed polycrystalline, meaning they are the combination of two or more small crystals that joined during solidi-cation. The consequence is that the material becomes made up of speci c domains
called grains, and these grains are separated by a grain boundary.75 Within each grain it appears as though the atoms are arranged in a single crystal, but at the grain boundary, this order is lost. These grain boundaries are important factors in determining the proper-ties of a material and the potential ways it might degrade76 In a sense, these boundaries are “chinks” in the material’s “armor.” Certain atomic effects that lead to this displace-ment of atoms at the grain boundary may facilitate or catalyze unique phenomena like the initiation of tin whiskers in microelectronics (according to the electrostatic theory for tin whiskers).77 We need better understanding of the atomic structure at these grain boundaries, and how atomic effects change the atomic structure at grain boundaries, to develop better designs and corrosion preventative measures for metals.
Specific Metals and Their Properties
Metals exhibit a wide range of properties and have many different uses. A thorough discussion of every metal of interest is well beyond the purpose of this work that level of comprehensive treatment is contained in material science textbooks. In this section, we use an exemplar to explain the scienti c rationale for the importance of AEC. To il-lustrate the point, we have chosen steels: metals that are essentially ubiquitous in society and familiar to virtually everyone. Classi cations of steel alloys are depicted in Figure 11. The point we will demonstrate is that materials are impacted by AEC, AEC affects the material properties of their underlying atomic structures, and at smaller scales a few AEC events can have an observable deleterious impact.
73. E anuelle A. ar uis, et al., “Nuclear reactor aterials at t e ato ic scale,” Materialstoday 12, No.11 (2009): 30-37.
74. . arc adou, undamentals o Micro a rica on and anotechnology olume Manu acturing Techni ues or Micro a rica on and anotechnology. rd Edi on (CRC Press, 2011).
75. Pavel Le ec , rain oundary Segrega on in Metals (Springer, 2010).76. . Ger ig, et al., “Ato ic-Scale Quan ca on o Grain oundary Segrega on in Nanocrystalline aterial,” hysi
cal e ers Revie 112, No.12 (2014).77. ictor arpov, “Electrosta c eory o etal is ers,” hysics Revie Applied 1, No.4 (2014).
Classi cations of steel alloys.
Ferrous Alloy Steels
An alloy is a combination of two or more metals some alloys are comprised of a metal with a non-metal impurity. The ferrous alloys, which are alloys in which the primary com-ponent is iron, are the most manufactured type of alloy today.78 Iron is abundant in the earth’s crust, is easy to work with, and is versatile depending on the alloy, designers can achieve a wide range of mechanical and physical properties. A major problem with ferrous alloys, though, is the that the iron atoms undergo oxidation easily in the presence of a strong oxidizing agent such as oxygen. Everyone is familiar with the result, which we call rust.
Steels are a mixture of iron with different concentrations of carbon.79 There are low, me-dium, and high-carbon steels, each of which displays unique properties. In addition to carbon, in certain alloy steels, impurities (such as low concentrations of manganese) are added purposefully to create unique properties. In current steel manufacturing pro-cesses, getting the right combination of ingredients combines both art and science. The techniques rely on an empirical approach to engineer these alloys, and then reproduce those that have been proven to work.80 To date, it has not been possible to obtain the exact same atomic con gurations of iron and its impurities in the production of steel. If we can determine how to manufacture materials atom-by-atom, that may change.
78. “Ferrous etals and Iron Alloys In or a on,” S Engineering, Accessed 21 Sept, 2015, p: .glo alspec.co learn ore aterials c e icals ad esives etals alloys errous etals iron alloy.
79. “Steel,” Wi ipedia, odi ed 22 Sept 2015, Accessed 24 Sept 2015, ps: en. i ipedia.org i i Steel.80. Step en . Cra er, ed., ASM and oo olume C Corrosion Environments and ndustries (AS Interna onal,
110 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Low-carbon steels generally contain around 0.25 (by weight) of carbon the microstruc-tures of these steels typically consist of ferrite and pearlite. Ferrite has a body-centered cubic crystal structure, while pearlite is a mixture between cementite (a face-centered cubic crystal structure) and ferrite.81 Low-carbon steels are the most highly produced steels despite being relatively weak and soft, they are extremely ductile, tough, mal-leable, and inexpensive to produce. These types of steels are found in numerous ap-plications such as automobiles, structural beams (i.e., I-beams), pipelines, buildings and bridges. These steels can be made into what are called “high-strength, low-alloy” steels through the addition of copper, vanadium, nickel, and molybdenum to add strength.82
Medium-carbon steels contain between 0.25 and 0.6 (by weight) of carbon. These steels have microstructures of tempered martensite, in which the iron atoms pack into a close-packed structure. The mechanical and thermal properties of these steels can be adjusted through the additions of alloying agents such as chromium, nickel, and molyb-denum. As a result of their increased strength, these steels are less ductile but are very tough. Typical uses of medium-carbon steels involve crankshafts, railway car wheels, and other applications requiring materials with high strength and wear resistance.
High-carbon steels contain between 0.6 and 1.4 (by weight) of carbon and have microstructures that are entirely pearlite,83 thus giving their atomic structures a face-centered cubic crystal lattice. These are the hardest and strongest types of steels, which means they are also the least ductile. The increased strength and hardness results in improved thermal and mechanical properties: they are more heat resistant than other carbon steels and less susceptible to wear. For example, high-carbon steel knives can hold a sharp edge longer than medium- or low-carbon knives. High-carbon steels can also be made harder and more wear resistant by adding chromium, vanadium, tung-sten, and molybdenum into the mixture. These kinds of steels are used for tools, blades, springs, and high-strength wire.
The different carbon steels are all susceptible to classical corrosion, but there is a fourth class of carbon steel that is much more resistant to these effects: stainless steel. Stainless steels are low-carbon steels with a high concentration of chromium added (at least 11 by weight), along with other elements such as nickel and molybdenum. The spe-ci c mixes depend on the desired application. Stainless steels can be manufactured to have predominately three different microstructures: martensite, ferrite, or austenite. Their different microstructures give the stainless steels the different thermal and me-chanical properties needed for different applications.84 Of all stainless steels, the aus-tenite is the most corrosion resistant, but austenite steels lack the magnetic properties that the ferrite and martensite derivatives have. Stainless steels have a wide array of applications, including gas turbines, aircraft, missiles, nuclear power-generating units, and heat-treating furnaces.
81. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
82. “ ig -Strengt Lo -Alloy Steel,” Wi ipedia, odi ed 25 ay 2015, Accessed 24 Sept 2015, ps: en. i ipedia.org i i ig -strengt lo -alloy steel.
83. “ ig -Car on Steels: Full Pearli c icrostructures and Applica ons,” ASM nterna onal (2005): 281- 295.84. ei S a, and anli Guo, Maraging steels Modeling o microstructure proper es and applica ons ( ood ead
Pu lis ing, 26 ct 2009).
Microscopic structure of steel/Webcorr
Steels are not single crystals they are characterized by polycrystalline microstructures. As a result, all steels consist of various grains and corresponding grain boundaries (see gure above). The grain boundaries re ect areas with lattice defects, and such defects
include vacancies (an iron atom is missing from a lattice point) and dislocations (linear defects in the lattice). The atoms in metal lattice structures have a tendency to diffuse, and the vacancies act as a diffusion facilitator because they represent areas of “low concentration.”85 AEC can facilitate the displacement of atoms at any point in a par-ticular microstructure of steel, but those that occur at grain boundaries are the most sig-ni cant. Because AEC can create vacancies within a lattice, AEC can initiate diffusion that might not have taken place in the absence of the atomic effect. When such steels are used on the micro- or nanoscale, these effects can have much greater impacts on the rate of degradation of the steel material through other, more classical mechanisms of corrosion. Recent insights into the impact of AEC on materials such as steel in environ-ments such as nuclear power plants have revealed the importance of understanding how AEC mechanisms accelerate the degradation of macroscopic properties.86
In polycrystalline metallic materials, the smaller the grain size, the smaller the grain boundary, and therefore the more strength and toughness the metal will have. This phenomenon illustrates the importance of creating small grains when producing steels. Even so, the nature of typical high-energy AEC processes can have important impacts: by causing corrosion at grain boundaries, AEC may create the rst crack in a lattice, thereby creating a grain boundary where was none. Limited study of atomic effects on materials such as steels has been completed because steel use typically occurs at
85. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
86. E anuelle A. ar uis, et al., “Nuclear reactor aterials at t e ato ic scale,” Materialstoday 12, No.11 (2009): 30-37.
112 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
the macroscale, so many AEC events would have to occur before noticeable impacts arise. If, on the other hand, we better understood AEC effects, it might be possible to improve lifetimes and reliabilities by designing ways to reduce their negative impacts87. As technology development reaches into smaller scales, fewer AEC events are needed to cause an observable impact.
Basics of Ceramics
Ceramics are compounds of metals and inorganic non-metals. Unlike metals, which develop their atomic, micro, and macro properties through the various structures and chemistries possible as a result of metallic bonding, ceramics develop their properties through a range of bonding schemes88. Ceramics form their structures and develop their properties through a combination of ionic, covalent, and secondary bonding (e.g., dipole interactions) mechanisms. The phenomena that must occur in order to create the fundamental properties of ceramics were poorly understood for most of humanity’s experience with them. Ceramics got their name from the Greek word , which roughly translates into “burnt stuff.” This name was associated with the fact that ceramics were made from heating substances such as clay to very high temperatures (i.e., ring). The solidi cation process that occurs after heating ceramics to such high temperatures allows the ceramic molecules and ions to crystallize into the atomic con gurations that give them their unique properties.89 Ceramic crystal structures are held together by ionic and/or covalent bonds and are less prone to deformation: generally, fracture occurs before deformation.90 In part, the reason ceramics are so brittle compared to a metal is because unlike metallic bonds, ionic and covalent bonds don’t “bend.”
The metals in ceramics are described in the previous section. The non-metals are located in columns I A, A, IA, and IIA of the periodic table (refer to the Periodic Table on page 105 for speci c elements in these columns). Non-metals tend to have electronega-tive atoms, and they tend to participate in chemical and physical phenomena that in-crease the density of electrons surrounding their nuclei. This contrasts to most metals that are more electropositive, and therefore less “needy” when it comes to particular elec-tron density requirements. The electronegativity property of non-metals is related to the fact their valence electron orbitals are at a point where it is more energetically favorable to acquire electrons to ll their valance shells, rather than give them up, as many metals do. Thus, these atoms tend to involve themselves in bonding schemes that give them the desired “octet” in the s and p orbitals of their highest valence shell.91 For example, nitro-
87. id.88. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Ap
proach ( o n iley Sons, Inc, 2012).89. “Scien c Principles,” niversity o llinois, Accessed 14 Sept 2015, p: atse1. atse.illinois.edu cera ics
prin. t l.90. ntroduc on to Materials Science, C apter 13, Structure and Proper es o Cera ics, p: e .ut .edu prac
se201 C apter 2013 20Structures 20and 20Proper es 20o 20Cera ics.pd .91. E. Cat erine ousecro and G. Alan S arpe, norganic Chemistry (Pearson Educa on Li ited, 2001).
gen tends to orient itself into geometries that favor three covalent bonds, oxygen tends to favor two, and the halogens only desire a single covalent bond. Complex electronic geometries are possible with non-metals. Halogens only need one bond because they only need a single electron to complete their octet. The other 3 electron pairs (i.e., lone pairs) occupy unique electronic geometries that allow them to take on various geospa-tial shapes. For the second energy level, for example, these typically consist of tetrahe-dral geometries. At the third energy level, the unoccupied d orbitals become important, and atoms can in certain circumstances surround themselves with more than eight va-lence electrons. The alence Shell Electron Pair Repulsion ( SEPR) theory describes the types of possible electronic geometries possible with the non-metals that participate in covalent bonds.92 The gure on page 114 shows the various electronic bond geometries that are possible.
The unique atomic properties of the types of atoms that make up the class of materials called ceramics explain why the structures of ceramics are more complex than those of metals. With structures dependent on bonds dedicated to strict sharing (i.e., no delocal-ization) of electrons, ceramics tend to make excellent insulators. Certain ceramics are able to take on a mixed property of electric conductivity known as semi-conductivity. These ceramic-based semiconductors are critical to the microelectronics industry.93
Recent advancements in understanding the science behind the atomic con gurations of ceramics, and how these con gurations give them their unique properties, has led to new understanding of the kinds of materials that can be made from ceramics.94
Modern day ceramics can be made more fracture resistant, and have found wider uses than the “traditional ceramics” used for bricks, china, porcelain, and glass. Today, ceramics are used in varied applications, from cookware to computers. The relatively recent breakthrough is at least partly attributable to the ability to understand ceramics at the atomic level. This understanding spurred new ceramics to take advantage of the properties induced by changes or deformities in their atomic structures. Some deformities are therefore useful, but unintended deformities are not likely to be so. Ceramics in environments where phenomena can cause changes in the properties or locations of individual atoms will be subject to AEC. Unlike chemical oxidation-reduction reactions, which require speci c types of atoms,
92. id.93. E. Cat erine ousecro and G. Alan S arpe, norganic Chemistry (Pearson Educa on Li ited, 2001).94. April Goc a, “Ne Ato ic-scale serva ons Could Lead to Engineering o uc le yet Strong Cera ics,” The
American Ceramic Society, 12 April, 2015, p: cera ics.org cera ic-tec -today ne -ato ic-scale-o serva-ons-could-lead-to-engineering-o -duc le-yet-strong-cera ics.
The unique atomic properties of
ceramics explain why the structures
of ceramics are more complex than
those of metals.
114 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
ions and molecules in order to occur, high-energy collisions from gamma radiation or high-speed neutrons that cause AEC do not discriminate when it comes to what types of materials can be degraded.
Bond geometries associated with valence-shell electron-pair repulsion theory ( SEPR). (CC B -SA 3.0)
Basic ceramic structures come in two types, depending on the bond structures: those that are strictly ionic, and those that are a mix between ionic and covalent.95 The differ-ence in the bonding types determines the atomic structures of different ceramics.
Ionic bonds are the strongest chemical bonds because they occur between two atoms separated by at least one complete charge.96 All other bonds occur because of charge separation, but only ionic bonds occur because of the attractive force stimulated by total charge separation. For ceramics, the cations (positive ions) are metals and the anions (negative ions) are non-metals. The crystal structures of ceramics are a function of the magnitude of the electrical charge on each ion and their relative ionic radii. In order for a ceramic solid to form, the charges within the unit cell of the crystal lattice must bal-
95. “Scien c Principles,” niversity o llinois, Accessed 14 Sept 2015, p: atse1. atse.illinois.edu cera icsprin. t l.
96. E. Cat erine ousecro and G. Alan S arpe, norganic Chemistry (Pearson Educa on Li ited, 2001).
ance, so the net charge on that cell is neutral. This requirement has a large impact on the nature of the atomic orientations observed within the unit cell. Because cation nuclei have a greater pull on their remaining valence electrons, their atomic radii tend to be smaller than those of the corresponding anions. This geometry creates a fundamental difference between ceramic and metal crystal lattice structures. In metals, the atomic radii are similar in ceramics the unit cell consists of different sized ions, and thus different structures are possible. The most stable ceramic structures are those where all cations and anions are “in contact” within one another “in contact” means there is overlap between bonding orbitals (see the gure below).97
Critical Radius Ratio/Matthew Rollings
The coordination numbers of ionic compounds are also different than those of met-als. Coordination number is typically greater for ions with larger ionic radii, and less with smaller radii. The coordination number has the same effect, though: the larger the coordination number, the more tightly packed the unit cell is.98 Because ionic crystal lat-tice structures must balance, there are several variations that commonly exist amongst ceramics.99 The lattice designations are typically denoted Am p, where A is the cation,
is the anion and the subscripts m and p denote the ratio of each in the unit cell. For a 1:1 ratio, m and p are 1 and these types of lattice structures are denoted A -type crystal structures.
Lattice structures for ionic compounds are typically determined by the anion packing style. For A structures, the anions typically pack in face-centered cubic or simple cubic arrangements. The compounds sodium chloride (NaCl), cesium chloride (CsCl), and zinc sul de ( nS) have coordination numbers of 6, 8, and 4, respectively. Even though the ra-tios in the unit cell are equal, the different coordination numbers arise from the different charge magnitudes and relative sizes of the ions. Other ceramic ionic compounds have
97. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
98. id.99. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Ap
proach ( o n iley Sons, Inc, 2012).
116 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
ratios different from 1:1, such as CaF2, and these lead to different properties. One of the more interesting ionic structures is composed of two different cations, typically referred to as AmBn p. BaTiO3 is a ceramic ionic compound in this category, and this ceramic takes on what is known as a crystal structure. This atomic structure gives rise to some unique electromagnetic properties, such as colossal magnetoresistance and superconductivity.100
Ceramics are capable of forming close packed structures. These ceramic structures con-sist of closely packed planes of ions. The packing of the planes leads to interstitial sites that can take on particular geometries such as tetrahedral and octahedral. The factors that in uence these geometries are the close-packed anion layers and the manner in which cations occupy the interstitial sites. Whether a particular ceramic lattice structure tends to surround the cations with four or six anions depends on which orientation pro-vides the structure with the most thermodynamically stable con guration. For example, in the crystal structure of sodium chloride (i.e., table salt) the most stable con guration is to occupy sodium atoms in an octahedral con guration, such that each sodium cation is “touching” six other chloride ions.
While many ceramics take on these stacking behaviors, some do not. The perovskite crystal structure, for example, has unique properties associated with it. There is a spinel structure associated with the AmBn p lattice structure (see “Spinel structure” gure, page 117). MgAl2O4 for example (a ceramic used in structural, chemical, optical and electrical industries)101 has the O2- anions packed in a face-centered cubic arrangement.102 This arrangement creates both tetrahedral and octahedral interstitial sites. For this particular material, the Mg2+ occupy the tetrahedral sites and the Al3+ occupy the octahedral sites. Many magnetic ceramics take on variations of such spinel lattice structures, and their magnetic properties are determined by the nature of the cations that occupy the tetra-hedral and octahedral sites.103
100. “Ferroelectric Proper es o a a i 3,” Materials Design, nc., 2009, Accessed 29 Sept 2015, . aterialsdesign.co syste les appnotes a i 3 1.pd .
101. Li Rooi Ping, A dul- a eed A ad, and eng an ung, “ agnesiu alu inate ( gAl2 4) spinel produced via sel - eat-sustained (S S) tec ni ue,” Material Research ulle n 36 (2001): 1417-1430.
102. A.R. olla, C.R. esavulu, R.P.S. C a rad ar, A. ara der, S. . o anty, .L. Rao, . ar a ara, and S. . is as, “ icrostructure, ec anical, t er al, EPR, and op cal proper es o gAl2)4:Cr3+ spinel glass-cera ic nanoco -posites,” ournal o Alloys and Compunds 583 (15 an 2014): 498-509. 509.
103. Raul alen uela, Magne c Ceramics Chemistry o Solid State Materials , (Ca ridge University Press, 2005).
Silicates are another important category of ceramics.104 Silicates consist of silicon and oxygen. Given that these are two of the most abundant elements in the earth’s crust, silicates tend to be major components of soils, rocks, clays and sand. Silicate ceramics can have either crystalline or amorphous structures (see the two gures at the top of page 118). For structures that are amorphous, AEC is less relevant because the major impact of atomic effects is the introduction of disorder into ordered atomic structures. Therefore, our discussion of silicate ceramics will focus on the structure of the more or-dered varieties.
The various silicate geometries arise from the covalent character of the Si-O bonds. Sili-con has 4 valence occupancies and a tetrahedral electronic geometry.105 This means that each silicon atom in a silicate exists in an oxidation state of +4, and each oxygen atom exists in an oxidation state of -2. The SiO4
-2 tetrahedron makes up the basic structure in which silicates exist. The different 1, 2 and 3-dimensional structures it forms determine the type of silicate and its properties. The Si-O bonds within silicates are covalent, and the different structures that silicates manifest are consequences of secondary bonding schemes such as van der Waals forces.
Silica, SiO2, is the simplest silicate. It is comprised of an arrangement of SiO4-2 tetrahedrons,
but the crystal structure that forms has an overall ratio of 2 oxygen atoms for every silicon
104. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
105. E. Cat erine ousecro and G. Alan S arpe, norganic Chemistry (Pearson Educa on Li ited, 2001).
118 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
atom. uartz is a well-known silicate important for several applications, such as oscilla-tors for frequency and timing. In addition, despite the fact that silicates have relatively open atomic structures, and are less densely packed than metals and other ceramics, they can withstand high temperatures. This makes silicates useful in the construction of space ship hulls and engine components.106
Silicates can form complex atomic arrangements due to the fact that one, two, or three of the O atoms in the SiO4
-2 tetrahedrons can be part of another tetrahedron. Silicate structures can also incorporate other ions such as Ca2+, Mg2+, and Al3+ in order to achieve crystal neutrality, and these ions further strengthen the structure by bonding ionically to the tetrahedra. For example, akermanite (Ca2MgSi2O7) is a silicate mineral that has po-tential biomaterial applications (one application is as a biodegradable coating used in biomedicine) it has a complex structure dependent on the Ca2+ and Mg2+ ions.107
Layered silicates have meta-atomic structures that occur when three oxygen ions in the silicate tetrahedra are shared. For example, kaolinite clay is a layered silicate with the formula Al2(Si2O5)(OH)4. The U.S. Naval Medical Research Institute used a kaolinite-derived aluminosilicate nanoparticle to infuse gauze and develop uickClot Combat Gauze that facilitates the rapid clotting of wounds.108 Kaolinite’s silica layer is made neu-tral by a layer of Al2(OH)4
2+. This two-layered sheet is held together through strong ionic-covalent bonds, and adjacent sheets are held together through secondary bonds (e.g., van der Waals).
Although the structures of various ceramics are more complex and less ordered than the structures of metals, ceramic structures arise through strong bonds that are both ionic
106. Ulric Sc u ert, ed., Silicon Chemistry (Austria: Springer- erlag ien, 1999).107. “ er anite,” Wi ipedia, odi ed 3 arc 2013, Accessed 12 Sept 2015, ps: en. i ipedia.org i i er-
anite.108. Gegel, et al. “An evidence- ased revie o t e use o a co at gau e (Quic Clot) or e orr age control,”
American Associa on o urse Anesthe sts ournal 81, No. 6 (2013): 453-458.
Chemical structure of uartz/Wimmel
The amorphous structure of glassy Silica (SiO2) in two-dimensions/Wimmel
and covalent in nature. Defects in the structures of ceramics (see gure below) therefore tend to result in atomic con gurations that promote diffusion, which ultimately results in lattice deformations and degradation of the ceramic’s material properties. Because ceramics are typically comprised of ionic substances, they need to retain their electro-neutrality to ensure their structures. As with metals, the atomic structures of ceramics can experience both vacancies and interstitials. A major difference between metals and ceramics is that in ceramics, the atomic point defects can occur with two different types of ions rather than just a single type metal atom. The nature of a vacancy or interstitial defect will differ, depending on whether a cation or anion is at the center of the defect.
Crystal Lattice Point Defects
Crystal Lattice Point Defects/Alex Taliesen
120 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Atomic effects can displace atoms from their lattice structures, and can thereby lead to defects in the atomic structure of ceramics. Frenkel defects occur in ceramics when a cation migrates from its normal lattice position to an interstitial site within the lattice, causing deformities.109 This migration can also cause a change in the lattice polarity, potentially creating a charge gradient that facilitates further ion migration within the ceramic. In metals, such events may lead to problems such as tin whiskers. In ceramics, these events can also result in adverse effects such as fracturing. In A type ceramics, for example, Schottky defects occur when both a cation and anion vacate their interior lattice positions. In instances where a defect causes a change in the charge stoichiom-etry, substitutions can be made as long as the replacement ion is of similar relative size and charge.110 Still, such replacements will distort lattice structures. Non-stoichiometric degradation events can occur through other mechanisms, such as when one of the ions within the lattice structure is capable of taking on multiple oxidation states. Iron oxide is such a material, and if an iron ion (Fe2+) undergoes a further oxidation event, a charge of +1 will arise within the lattice. The most likely correction of this imbalance is creation of an Fe2+ vacancy to retain the thermodynamically stable electroneutral structure. These moves result in changes to the ceramic’s properties. The likelihood of a Frenkel or Schott-ky defect is a function of the energy required to form the defect, the number of lattice sites, and temperature.111
Impurities in ceramics lead to different material properties. In a sense, impurities can be a two-way street for defects in ceramic lattice structures. They can be the root cause of lattice defects, or they can be the solution to lattice defects (see gure page 120). The introduction of impurities tends to be facilitated by the need to maintain electri-cal neutrality in the ceramic lattice structure. When vacancies arise in ceramics they create opportunities for diffusion. Diffusion is the natural tendency of atoms, ions, and molecules to move to areas where their concentrations are lower. If a material depends
on its atomic structure, diffusion represents a mechanism that re-quires an initiating event, such as a vacancy. The displacement of an atom from a lattice will create not only a temporal concen-tration gradient, but also a temporal charge gradient. There are many natural mechanisms that can create such displacements and trigger the onset of diffusion-induced degradation. Atomic effects can also be the culprit. These diffusion defects are not always immediately apparent, and thus the root cause of a del-eterious effect may be overlooked. Damage to atomic lattice
structures leads to the eventual breakdown of microstructures, which changes macro material properties. Understanding the role that atomic effects play in creating vacan-cies will become more important as ceramic structures are increasingly applied in mi-cro- and nanomaterial designs.
109. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
110. id.111. id.
Ceramic structures arise through strong bonds that are both ionic and covalent.
Ceramics are used for different purposes in various systems, components and technolo-gies. Ceramics are typically more brittle than metals, but are also often stronger, harder, and more heat resistant. They are typically poor conductors because their atomic struc-tures depend on bonding schemes that do not favor delocalization. Ceramics are there-fore good insulators, and have been used as such for many years. Ceramics can take on magnetic properties (e.g., Fe3O4), and those properties depend on speci c lattice con gurations.112
Traditional ceramics are typically made from processed silica and clay. These create glass and cement-like ceramics. Newer ceramics are designed differently and manifest a wider range of properties, such as more ductility. Although not strictly ceramics, the properties of silicon and carbon are normally discussed in the context of ceramics. These two substances play important roles in microelectronics and nanotechnologies.
Ceramics such as those used for piping and high-temperature conditions are likely less sensitive to a few individual AEC events than other types. Due to the nature of their bonding schemes, their lattice structures are stronger, and a single displacement defect on the lattice will have less of an immediate impact on their macroproperties. Other properties though, such as their electrical and magnetic properties, can be affected by AEC, especially in materials used for microelectronics and nanotechnologies. AEC cer-tainly play a role in initiating events that in turn can lead to the degradation of ceramic microstructures, and the concomitant loss of macroscale properties, through classical corrosion mechanisms. As with metals, AEC can couple with classical corrosion to de-grade ceramics.
traditional ceramics/ SciELO.org
112. Gallo ay, “ iote pla ng arrays o nano agnets using t e io ineralisa on protein s6,” P t esis,niversity o eeds (2012).
122 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Traditional ceramics (see gure 121) make good insulators (both heat and electricity) and thus are frequently used to insulate other materials. Although the properties of com-mon insulators depend on their crystal lattice con gurations, AEC is seldom a “direct” problem because it has to affect the connectivity of hundreds of thousands of atoms to be noticeable. These are the cases where AEC may act to accelerate other forms of corrosion. Traditional ceramics are strong, hard, heat-resistant and brittle. They are utilized by DoD and society for structural purposes.
The important properties of traditional ceramics used in cement, piping, and other struc-tural applications are not likely to be signi cantly degraded due to AEC at the mac-roscale. This is not to say that AEC does not matter at the macroscale: as mentioned before, AEC caused by ionization or displacement can lead to atomic point defects that create lattice defects, which can ultimately result in microfracturing. In structural ceramic applications, microfracturing can lead to structural failure.
Advancements in material science have enabled scientists and engineers to under-stand the relationships between the atomic makeups of ceramic materials and how they manifest into the material properties that make ceramics useful in modern society. With the invention of new manufacturing and processing technologies, ceramics have found new applications that take advantage of the underlying phenomena that give them their structures and properties.
MEMS are small, “smart” technological systems that integrate micron sized mechanical systems with electrical elements mounted on a silicon substrate (see gure 123).113 These systems incorporate precisely engineered microstructures that act as sensors and actua-tors. The sensor materials have speci c atoms, ions, or molecules in speci c crystal lattice structures that collectively demonstrate predictable behaviors in response to mechani-cal, thermal, chemical, optical and/or magnetic stimuli. For example, an increase in a microsensor’s temperature might cause a change in the packing within the lattice unit cell that change is detected by an adjacent microsystem connected through a path-way that allows for allosteric communication. Thus, changes in the material properties of the microsensors can be processed by microelectronic components of the MEMS, which in turn generate another atomic change to signal to activate a microactuator. In this sense, MEMS can form an environmental signal/response system, where the atomic substructures of their microsystems respond to various stimuli, these stimuli are processed through materials capable of mathematical operations and information processing (e.g., transistors) and then a desired response from the MEMS actuator is produced. These responses can perform functions such as moving, ltering, pumping, regulating, or positioning. Thus, MEMS can be micron-sized versions of machines such as gears or motors, or other structures such as membranes.
113. “ icroelectro ec anical syste s,” Wi ipedia, odi ed 28 Sept 2015, Accessed 12 Sept 2015, ps:en. i ipedia.org i i icroelectro ec anical syste s.
MEMS are produced with the same processes used to create silicon-based integrated circuits. These include photolithographic, ion implantation, etching, and deposition technologies, as well as other micromachining techniques. There are limitations with rely-ing heavily on silicon for MEMS, due to silicon’s low fracture toughness, its low softening temperature, and its reactivity in the presence of water and oxygen. For these reasons, materials such as silicon carbonitrides (silicon carbide-silicon nitride alloys) are being considered for use in MEMS.114 There are already uses for MEMS today, and likely to be more applications of MEMS in the future. For example, MEMS may be used as chemical detectors for hazardous materials,115 microsystems for DNA ampli cation,116 and data storage.117 The working parts of MEMS are microstructures that depend on the integrity of the underlying atomic structures to work. ust as classical corrosion can lead to deg-radation of modern day macromechanical equipment, AEC can be a key player in the degradation of MEMS.
Nanoelectromechanical systems (NEMS), which are the nano equivalent of MEMS, are the next scale step in this technological evolution: from macro, to micro, to nano.118 Cur-
114. ictor . rig t, Ris i Ra , ar n L. unn, and o n . aily, n ecta le Ceramic Microcast Silicon Car on itride SiC , Micro Electro Mechanical Systems MEMS or E treme Temperature Environments ith E tension Micro ac ages or ano Devices (Ne or , N : anuary 2004).
115. Sara S. edair and Gar . Fedder, “C S E S scillator or Gas C e ical etec on,” Department o Electrical and Computer Engineering, Carnegie Mellon niversity (Pi s urg , PA), 2004.
116. ang C, u , a , and eng , “PCR icro uidic devices or NA a pli ca on,” iotechnological Advances 3 (2 ec 2005): 243-284.
117. o ong, Feng ang, Sco A. randt, arrell .E. Long, and o as .E. Sc ar , “Using E S- ased Storage in Co puter Syste s- E S Stoarge Arc itectures,” ACM Transac ons o Storage 2, No.1 (Fe 2006): 1-21.
118. .L. Rou es, “Nanoelectro ec anical Syste s,” Condensed Ma er hysics (Cali ornia Ins tute o ec nology, CA: 2000), p: ar iv.org pd cond- at 0008187.pd .
MEMS microcantilever resonating in an SEM./Pc et01
124 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
rently, NEMS materials rely heavily on the science of various allotropes of carbon, such as diamond and graphene. These allotropes contain the necessary mechanical properties needed for NEMS to function, and the metalloid characteristics of carbon allow for the desired metallic and semiconductor electric behavior required in NEMS. NEMS will be highly susceptible to AEC as their nanometer scaled structures will be sensitive to a few atomic changes. At this scale, their material properties depend on the correct con gu-ration of atoms, and the disruption of a few atoms may cause NEMS to fail.
Piezoelectric ceramics have been used for some time for both commercial and military applications, and their use continues in modern day technologies due to their elec-tromechanical behavior. The piezoelectric property (see gure page 125) arises in ce-ramics with crystal lattice structures that contain a low-degree of symmetry.119 The word piezoelectricity basically translates to “pressure electricity.” When a mechanical stress is applied to the crystal structure of a piezoelectric ceramic, a voltage is induced be-tween the parts of the crystal lattice that are stressed. Conversely, if a voltage is placed across a piezoelectric ceramic crystal lattice, a mechanical stress will result. Ceramics that demonstrate this property include Pb rO3, NH4H2PO4, BaTiO3 and quartz (SiO2). Piezo-electrics rst made a “practical” name for themselves in submarine sonars.120 The British navy developed a sonar that used two piezeoelectric materials, one for emitting a sig-nal and one for receiving a return signal. The piezoelectric emitter would have a volt-age applied to it and subsequently emit a high-frequency121 mechanical vibration that would travel through seawater. When the vibration wave hit an underwater object, the return signal would strike the piezoelectric receiver, which would interpret the vibrational energy signature into an electrical signal that could be analyzed to reveal the approxi-mate location of that object. Aside from sonar, piezoelectric ceramics have found their way into many different technologies and systems. For example, they can be found in automotive wheel balancers,122 air bag sensors,123 as microactuators in hard disk and notebook computer transformers,124 smoke detectors,125 and ultra-sound equipment for medical diagnosis.126
119. E. Cat erine ousecro and G. Alan S arpe, norganic Chemistry (Pearson Educa on Li ited, 2001).120. S aul at ir, “ o ne pie oelectricity Rut er ord and Langevin on su arine detec on and t e inven on o
sonar,” otes Records o the Royal Society 66, No. 2 ( une 2012): 141-157.121. oyle IR 23 Nove er 1916: Produc on and recep on o ig - re uency sound aves y t e et od o t e
ro n grid agnetop one ( IR 14243 16), U NA A 293 5.122. “Pie o-cera ic sensors and sensor applica ons,” Ceramtec, Accessed 30 Sept 2015, ps: .cera tec.co
applica ons pie o-applica ons sensor-tec nology .123. “Pie oelectric Cera ic evices Auto o ile Innova on,” Morgan Advanced Materials, 13 uly 2010, Accessed
29 Sept 2015, p: . organtec nicalcera ics.co do nloads tec nical-ar cles pie oelectric-cera ic-drives-auto o ile-innova on.
124. ang ing, Luo ian in, enyan ang, and Guo ian u, “Fa rica on o pie oelectric cera ic icro-actuator and its relia ility or ard dis drives,” EEE Trans ltrason erroelectr re Control 5, no.11 (2004): 1470-1476.
125. “S o e etector,” Wi ipedia, odi ed 22 Sep 2015, Accessed 18 Sept 2015, ps: en. i ipedia.org i iS o e detector.
126. “Genera on o an Ultrasound ave,” SRA, 2008, Accessed 29 Sept 2015, p: .usra.ca genera ono -ave.p p.
The effect of applied voltage on piezoelectric materials/Creepin475
Piezoelectric ceramic materials provide the ability to transduce mechanical energy into electrical energy. The trend, as in other areas, is using smaller structures in future applica-tions. The piezoelectric property depends on the complex nature of the crystal lattice in piezoelectric ceramics. As a result, only a very small number of atomic changes to the crystal lattice have to occur before the material’s properties begin to degrade. As future applications trend toward smaller structures, the displacement of a single atom due to interaction with a high-energy gamma ray or fast neutron may be all that is needed to degrade the piezoelectric property of that material to a level that no longer meets the material design requirements.
Silica is nding a new use as an optical ber in the communications sector.127 “Ultrapure silica” is virtually free from any impurity or defect that may cause absorption, scatter, or attenuation of light. Processors are being developed that use silica bers that are approximately the diameter of the human hair to transmit information with improved information density, reduced error rate and increased transmission distance. Given the importance of communications within the DoD and the reliance on technologies that increase information density, beroptics will seek to create smaller silica cores that can be packaged to transmit more information faster. As with any submicron structure, the impact of AEC will be more destructive if its mechanisms and the resultant effects on these structures are not well understood.
Although not “true” ceramics, carbon allotropes and silicon currently play (and will play in the foreseeable future) a large role in the capabilities of modern day microelectronics. These elements are a mix between metals and non-metals (i.e., metalloids) and thus tend to experience properties of both within a single material. One such property displayed in both graphene and silicon is the property of semi-conducting. Silicon has become ubiquitous in microelectronics. The silicon transistor played a major role in bringing about
127. “ ard-clad silica op cal er,” Wi ipedia, odi ed 20 arc 2013, Accessed 28 Sept 2015, ps: en. i ipedia.org i i ard-clad silica op cal er.
126 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
the digital revolution.128 Transistors are nanometer crystals of silicon doped with elements such as phosphorus or boron to create polarized regions within the material that provide the desired functionality. A typical MOSFET transistor is shown in the gure below.
Silicon crystals are comprised of a large lattice of tetrahedral silicon atoms, and these atoms are covalently bonded.129 The electrical properties of a pure silicon crystal can be altered dramatically by the introduction of a few dopant atoms. For example, the addition of phosphorus brings an added electron that can be delocalized in the 3 d-orbitals of silicon and phosphorus.130 The network of orbitals in which electrons can be delocalized within the silicon lattice is typically referred to as the “conduction band.” The energy difference between the conduction band and the valence orbital an electron normally resides in is known as the energy gap. By using different semi-conducting ma-terials or precise doping of silicon substrates, the energy gap can be modi ed to meet speci c needs. For example, the quantum tunneling diode works by creating an energy band gap that promotes the phenomenon of quantum tunneling. This is accomplished by precisely doping the silicon lattice at the p-n junction (an area 10 nm or less wide) to create a conduction band gap in which the n-side conduction band states are es-sentially equal to the p-side valence hole states.131 These properties only exist within these materials at the atomic scale. Many argue that no other material is more important to technological superiority in the digital age than the materials used to transmit, pro-
128. “ ransistor,” Wi ipedia, odi ed 26 Septe er 2015, Accessed 28 Sept 2015, ps: en. i ipedia.org i iransistor.
129. “Silicon,” Wi ipedia, odi ed 29 Sept 2015, Accessed 1 ct 2015, ps: en. i ipedia.org i i Silicon.130. Pr. Ali avey, “Integrated Circuit evices,” Semiconductor undamentals ecture (University o Cali ornia, er ley,
28 Aug 2007), p: -inst.eecs. er eley.edu ee130 a07 lectures Se iconductor unda entals lec1.pd .131. o as Engel and P ilip Ried, hysical Chemistry (Pearson Educa on, Inc. 2006).
Basic structure of an n-channel MOSFETs in cross-section (planar)/Hennig
cess, and analyze information signals. And as these materials become smaller in scale in micro- and nanoelectronic technologies, they also become more susceptible to the impacts of AEC.
One of the mechanisms used to create n-type silicon is called neutron transmutation doping this process literally uses atomic effects to create a desired property. The ab-sorption of a high-speed neutron by 30Si converts the silicon to 31P through the nuclear reaction:
One way in which this can be accomplished is by placing a pure silicon crystal near a nuclear reactor to absorb neutrons.132 Although not as widely used as diffusion or ion implantation, neutron transmutation doping has the added characteristic of creating uniform dopant distribution. The neutron transmutation doping procedure takes advan-tage of an environment that produces the phenomena (e.g., neutrons) capable of pro-ducing atomic effects. This leads to changes in the atoms within the lattice structures of a material, and fundamentally alters the materials properties in a way that is clearly distinguishable (i.e., changing from insulator to conductor). Both DoD and the world in general are becoming more reliant on devices like the transistor, and new materials are being designed that utilize different electrical, magnetic, and/ quantum properties to create new capabilities.
The use of doping to create new material properties is a form of AEC that is bene cial, but other AEC mechanisms are not. Developing science makes it clear that we need to understand the phenomena that degrade the lattice structures of materials as well as those that lead to desirable design features. Otherwise, we may realize, after the fact, the impact and costs of AEC are signi cant. This recognition occurred in the classical corrosion arena in 2002: a report by NACE133 informed DoD of the true cost of classical corrosion, which was considerably higher than expected.
Carbon nanotubes are another pseudo-ceramic nanostructure that offers the potential to revolutionize the nanotechnology world in ways that may parallel what silicon has done for microelectronics.134 Carbon nanotubes obtain their unique mechanical and electrical properties due to the very precise lattice orientations that form upon their cre-ation. Carbon nanotubes are essentially a single plane of graphite (i.e., graphene) rolled onto itself and capped with a C60 fullerene. This gives the nanotubes a roughly 100-nm di-
132. “Neutron rans uta on oping o Silicon at Researc Reactors,” nterna onal Atomic Energy Agency ( ienna,Austria: 2012), p: -pu .iaea.org C Pu lica ons P F E 1681 e .pd .
133. Ger ardus . oc , ic iel P. . rongers, and Neil G. o pson, “Corrosion Costs and Preven ve Strategies int e United States,” ACE nterna onal, 2002, p: .nace.org uploadedFiles Pu lica ons ccsupp.pd .
134. “Car on Nanotu e,” Wi ipedia, odi ed 30 Sept 2015, Accessed 1 ct 2015, ps: en. i ipedia.org i iCar on nanotu e.
128 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
ameter. Nanotubes are covalently bonded, making them an extremely large molecule: essentially a cross between a ceramic, a metal, and polymer. This phenomenon allows the nanotubes to be extremely strong (it is the strongest known material) and stiff while also being fairly ductile.
By changing the connectivity of the lattice that holds the nanotube together, different properties result, such as the ability to change from a conducting material to semicon-ducting material (see Nanotubes gure below). The orientation of the hexagonal sub-units of the graphene motif relative to the tube axis determines the electrical conduc-tance properties of the material. The impact these types of materials are going to have in the near future with regards to materials and technologies could be huge. Given their size and reliance on the integrity of their lattice structures for their unique properties, it is important to comprehend the impacts AEC could have on such materials.
Nanotubes: armchair or zigzag/W2raphael
Basics of Polymers
Polymers are another class of materials used to engineer systems with desirable proper-ties and behaviors.135 The gure below shows the different classi cations of polymers. Compared to metals and ceramics, polymers differ in their material properties due to the nature of the molecular structures that hold them together. Polymers may be natural or synthetic. All polymers are de ned by the fact their connectivity consists of a series of linked subunits, normally termed “repeating units,” bound by covalent bonds. Most poly-mers are hydrocarbon based, meaning that the repeating unit of the polymer is made up of covalently linked carbon atoms that are bound to at least one hydrogen atom.
Different types and classi cation of polymers.
Polymers can comprise several linked repeating units (as in hydrocarbon fuels), or mil-lions of repeating units (as in DNA). Useful natural polymers include cotton, wool, and silk. From an engineering standpoint, synthetic polymers are of greater interest because these polymers can be chemically altered or synthesized in controlled ways to have desirable properties.136 Polymers can form crystalline structures, and also exist in liquid, amorphous, or a cross between amorphous and crystalline phases. By controlling the chemical nature and number of repeating unit(s), the properties of a polymer can be changed. Thus, the underlying molecular structures determine polymer properties.
135. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
136. . illia , Callister, G. avid Ret isc , undamentals o Materials Science and Engineering An ntegrated Approach ( o n iley Sons, Inc, 2012).
130 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Polymers tend to exist in more disordered forms than either metals or crystalline-state ceramics. The covalent nature of polymers gives their molecules great exibility. Many of the macroscopic uses of polymers are the result of emergent properties that form as polymer molecules attempt to maximize bonding interactions, such as van der Waals forces (e.g., the hydrophobic effect). For materials at this scale, AEC is only signi cant when those materials nd themselves in highly irradiative environments such as a nuclear reactor. Some special polymers, like graphene, have important properties that change depending on their actual molecular con guration. These polymers, like with any other material whose properties depend on the integrity of their atomic/molecular structures, are susceptible to only a few instances of AEC.
Tetrahedral bond geometry for the most simple hydrocarbon methane/Alex Taliesen
Common polymers are typically composed of hydrocarbon backbones, though there are other types of polymers with different backbones. DNA, for example, utilizes a phos-phodiester backbone in order to achieve its polymerization of the component deoxyri-bonucleic acids. Organic polymers (with hydrocarbon backbones) occur naturally, but some of the more useful polymers are synthesized. For organic polymers, knowledge of the chemistry that describes their structures makes synthesis possible and controllable.
Hydrocarbons are molecules composed of carbon and hydrogen that have a string of connected carbons (i.e., carbon backbone) linked through covalent bonds. Carbon is located in the p-block within column I A of the periodic table, and has 4 valence electrons. Carbon is small and relatively electronegative compared to most other metals and non-metals. The four valence electrons of carbon assume a tetrahedral geometry where the bond angle is 109.5 , as shown in the gure above. When carbon forms cova-lent bonds with hydrogen or other non-metals in this geometry, the 2-s and 2-p atomic orbitals hybridize into four sp3 orbitals that position the valence electrons in the tetrahe-dral geometry, as this is the most thermodynamically stable con guration. Rotation can occur around any of the four sp3 orbitals. This rotational exibility allows long chains of hydrocarbons to have many bends and twists. The bending and twisting of long chain hydrocarbons can result in a random “folding” of hydrocarbons where sections of the chain are held together through a collective force derived from secondary bonds (e.g., van der Waals interactions). The degree of folding or aggregation in a hydrocarbon is a delicate balance between obtaining energetic gains (i.e., enthalpy) and the entropy of the polymer’s structure. The major factors that in uence this structure are the polymer chain length, the connectivity of the repeating unit(s), and the chemical makeup of the repeating unit.
To better understand the chemical nature of polymers, let’s start by looking at how simple hydrocarbons are put together. The compound ethane consists of two carbons covalently linked, and each of these carbons are bound by three hydrogens (see gure “Ethane three dimensional bonding structure,” below). The bonding occurs between the hydrogen 1-s orbital and the carbons four sp3 orbitals. In this con guration the carbon can rotate freely around the C-C or a C-H bond, and will assume the conformation that minimizes steric hindrance between neighboring C-H bonds (see gure “Differing ethane rotational orientations,” below). In ethane, this conformation is staggered. If a few other CH2 groups are added to ethane, hexane can be made. Hexane has more degrees
of rotational freedom and thus can assume more conformations. However, it is unable to form enough secondary bonds to formulate any type of amorphous or crystalline structure at normal temperatures.
The hydrocarbon backbones are not restricted to bonding schemes that force them into tetrahedral geometries with sp3 hybridized orbitals. The repeating units of hydrocarbons can also include carbons linked through double or triple bonds. Here the single bonds are formed with sp2 or sp hybridized orbitals, and the double and triple bonds are made through unhybridized p-orbitals. The introduction of double and triple bonds into poly-mers does two things: it creates more rigidity in the hydrocarbon backbone, and it pro-vides a mechanism for delocalization of electrons (i.e., resonance), which is important for the electrical conductivity properties a polymeric material exhibits.
Ethane three dimensional bonding structure/Alex Taliesen
132 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The introduction of double and triple bonds to a polymeric backbone creates order within the molecular structure. Such bonds can establish “kinks” in the backbone that allow the polymer to retain a speci c molecular orientation. The placement, frequency, and nature of the kinks thus can in uence the material properties of a polymer. Ad-ditionally, carbons do not have to bond exclusively to other carbons and hydrogens. Part of any polymer or repeating unit within a polymer can consist of functional groups de ned by covalent bonds with carbon and other non-metals such as nitrogen, oxygen, or the halogens. Because these functional groups contain non-metals, this formation creates polarization in the molecular structures. This polarization in uences the material properties and chemical reactivity of the polymers. Different repeating subunits can be utilized in the construction of a polymer, and such polymers are typically referred to as copolymers because they are combinations of either different repeating units or smaller polymers of various lengths and composition (see gure below).
Random co-polymer: monomer units arranged randomly.
Block co-polymer: blocks of homopolymer units.
Graft co-polymer: homopolymer chains joined.
Alternating co-polymer: monomer units alternate.
Different linkages of copolymers/Alex Taliesen
Considering their different structures and material compositions, polymers can take on a wide spectrum of properties. Many of the properties attributed to synthetic polymers depend on the unique mix of disorder and order within their molecular structures. Unlike other materials like metals and ceramics, science has not yet determined how to cre-ate polymers with speci c molecular con gurations rather, properties are engineered through empirical processing techniques founded in chemical theory. Bulk properties of polymers can be fairly nely tuned, but getting a polymer to aggregate into a precise three-dimensional orientation every time is a very dif cult and complicated task. To date, science can barely explain how an enzyme manages to fold into the same orientation during its synthesis, and enzymes are polymers whose end structure is precisely known.137
137. en A. ill, S. anu an, . Sco S ell, and o as R. ei l, “ e Protein Folding Pro le ,” Annual Revie o iophysics 37 (2008): 289-316.
There is still a lot of science to be developed in the eld of understanding the precise nature and mechanisms of how large polymers obtain stable orientations.
For more ordered polymers though, (i.e., those that have more crystalline structures) a great deal is known about how the atomic properties of the substances translate into the observed atomic structures. In general, the more “links” in a polymers chain, the more likely it will be that it can take on a solid-state structure. The principles behind this phenomenon explain why certain fats are liquid (e.g., oils) or solid (e.g., lard) at room temperature: the longer the hydrocarbon chain, the more secondary bonding interac-tions can take place that allow the different polymeric chains to stack into ordered structures. These are typically termed hydrophobic interactions. When hydrocarbons contain functional groups with electronegative non-metals, stronger dipole interactions between adjacent polymers can help create more rigidity within the material. Polymers can also have their chains covalently linked together in a process known as cross-linking. Order can also be established when polymers form networks utilizing a repeating unit with three active covalent bonds. It is important to remember, though, that unlike a metal the order established in polymeric networks and systems is somewhat random in nature. The same types of bonding patterns and structures form when polyvinyl chloride (P C) is made, but each sample of P C is unique in its precise network of atomic/mo-lecular connectivity.
The atomic structures of metals and ceramics are made from atoms and ions, while polymeric molecular structures are made from molecules. This makes the nature of those polymers that do crystallize much more complex than other materials. The polymeric chains pack in unique ways to create vast atomic arrays, and some of these have use-ful emergent properties at the micro- and macroscales. Typical polymer crystals consist of regions that contain both amorphous and crystalline regions (see gure below). The amorphous regions of polymeric chains are twisted, coiled or kinked and the crystalline regions are more ordered structures held in place through various bonding patterns. The
Polymer with both amorphous and crystalline structures/Alex Taliesen
134 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
more complex the chemical properties of the repeating unit in the polymer, the less likely it will crystallize. Cross-linked polymers are also less likely to obtain crystalline structures because the covalent linkages prevent the necessary rearrangements needed for crys-talline formation. The differences between crystalline and non-crystalline polymers are similar to those of ceramics. A crystalline polymer is typically stronger, less ductile, and a better conductor of heat and/or electricity.
The impact of AEC on polymers such as plastics is distinctly different than what occurs in other materials. Polymers are generally used for to their macroscopic properties, and those properties tend to depend on the length of the polymeric chains that make them up. Atomic effects on polymers can result because interactions with, for example, high-energy gamma photons can break the covalent bonds in the polymer’s backbone. This in turn reduces the average molecular weight of the polymeric chains and allows the polymeric system to take on more disorder. Plastics in radioactive environments are known to degrade this way, essentially being “cut” into smaller polymeric pieces by high-energy particles.138 Additionally, polymers are nding new uses in more high-tech applications such as organic semiconductor materials. As with metals and ceramics, when a material’s property (e.g., information storage/processing) depends on the spe-ci c orientation of its underlying atomic/molecular structure, AEC is a serious concern.
The majority of synthetic polymers have properties characteristic of plastics and rubber. Generally, synthetic polymers are not very strong or stiff, are ductile, are easily formed into complex shapes, are relatively inert chemically, and are resistant to traditional electrochemical corrosion. These polymers nd applications from structural materials, to coatings, to lms. Normally the structures of polymers lack the necessary arrangements needed for delocalization electrons to conduct electricity. However, recent advance-ments in polymer science have enabled the study of polymer properties at the atomic scale making it possible to synthesize polymers that have more desirable properties such as semi-conductivity. This bottom-up science approach is likely to lead to expanding the use of polymer materials, and also to a new reliance on properties that are more char-acteristic of the individual polymer chains than their macroscale properties.
138. “ e E ect o Nuclear Radia on E posure to R duroid P FE- ased Co posites,” Rogers Corpora on, 2015, ps: .rogerscorp.co docu ents 753 acs e-E ect-o -E posure-o -R -duroid-P FE- ased-Co posites-
to-Nuclear-Radia on.pd .
Plastics and Other Polymers
Structures of different types of monomers for plastics/Alex Taliesen
Plastics (see gure above) such as polyvinyl chloride (familiarly known as P C), polysty-rene, polyesters and epoxies all exhibit a range of material properties. These properties manifest from the degree of crystallinity these materials form at various scales. Linear, branched, cross-linked, and networked assortments of polymeric chains will exhibit dif-ferent properties because their molecular arrangements determine the ways in whichthese chains can pack and crystallize. Ordered structure is necessary for electrical conductivity and strength, but this degree of order is not important to a material’s abil-ity to be molded into any shape. Plastics such as polystyrene are used in applicationsthat require a material with optical transparency this property is actually dependent on the amorphous nature of these structures. Amorphous or uid-like materials have adisordered microstructure and are less susceptible to the impacts of a few occurrencesof AEC because the phenomena that tend to cause atomic effects create disorder in an ordered system. What matters in these materials is the frequency at which theyexperience AEC: there is a threshold at which enough AEC can accumulate to make adiscernible difference in a polymer’s behavior. If that threshold is not reached during a material’s design life-cycle, then what matters is the extent AEC aids other degradation phenomena (i.e., classical corrosion).
Elastomers are polymers that give us materials such as rubber. The elastic properties ofthese materials depend on the molecular structures formed during processing proce-dures such as vulcanization.139 Arguably one of the most important elastomers is styrene-
139. “ ulcani a on,” Wikipedia, odi ed 15 Sept 2015, Accessed 28 Sept 2015, ps: en. i ipedia.org i i ulca-ni a on.
136 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
improved with the addition of carbon black to have increased tensile strength, wear and tear resistance, and stiffness.140 Silicone elastomers possess a high degree of exibilityand are resistant to the damage induced by wear and tear, making them potentially useful materials in things such as automobile engine components. All elastomers are bynature cross-linked, and their elastic properties depend upon the degree to which theycan form ordered molecular structures. Elastomers, just as steels used in nuclear reactors,can be better designed to withstand both the direct and indirect effects of AEC.
The other important polymer category is polymeric bers. These bers are used mainlyin textiles, which means they have important roles in the material properties of DoDsystems such as tents and clothing. The use of polymers as fabrics requires that they posses properties that allow for deformation, elasticity, high-tensile strength, and limitedchemical reactivity. These properties are determined by the chemical nature of thepolymer chains and the degree of crystallinity in the polymer structure. The propertiesof bers will deteriorate in the presence of phenomena that cause AEC, just as will any other polymer.
Polymers are used as coatings, adhesives, lms, and foams, among other things. Themany different uses of polymers re ect the degrees of crystallinity that can form with polymeric chains of varying sizes and chemical compositions. For the different types of materials derived from polymeric hydrocarbon chains, the mechanical properties are the manifestation of their molecular structures. Changes to their structures will have varying degrees of impact on the materials’ capabilities. If science can achieve the ability to understand how material properties manifest from the “bottom-up,” then we can custom design new polymers and polymeric materials. Learning how the propertiesof polymers emerge from their molecular underpinnings will also reveal how AEC can cause the degradation of these materials. By investigating the mechanisms of AEC inpolymers from the bottom up, new information about the causes of failures can be iden-ti ed and incorporated into predictive models. These models can then be used to moreaccurately determine a material’s reliability.
As polymers are understood in greater detail at the atomic scale, new techniques are being invented to control the assembly of various polymeric molecular architectures, and thus create advanced polymers that have desirable properties. For example, ultra-high-molecular-weight polyethylene (see Figure 31) has molecular weights on the order of 4x106 g/mol.141 This material is currently being utilized as a component of bulletproof
140. “Styrene-butadiene,” Wikipedia, odi ed 5 Sept 2015, Accessed 12 Sept 2015, ps: en. i ipedia.org i iStyrene-butadiene.
141. “Ultra- ig - olecular- eig t polyet ylene,” Wikipedia, odi ed 7 Aug 2015, Accessed 2 Sept 2015, ps:en. i ipedia.org i i Ultra- ig - olecular- eig t polyet ylene.
vests and military helmets. It is also used in valve gaskets, golf-ball cores and other tech-nologies. This form of polyethylene is versatile, but due to its high molecular weight it is sensitive to phenomena that can cause covalent breakage of its long polymeric chains. Such phenomena can include heat or radiation (i.e., AEC).
Schematic of an organic eld effect transistor/Materialscientist
Recently, polymers have been explored for their use as organic semiconductors.142 In silicon, the crystal lattice structures are virtually perfect, and it is relatively easy to ma-nipulate the physical environment around silicon crystals to move electrical charges.Therefore, silicon based semiconductors are currently the backbone of microelectronics. The problem is that silicon semiconductor manufacturing requires complex, multi-layer processes, and developing ef cient manufacturing processes is becoming increasinglydif cult as feature sizes decrease. Organic semiconductors offer the advantage of real-izing complex electronic circuits with a single semiconducting layer, deposited by simplecoating techniques. The problem is that organic polymers’ crystal lattice structures are far from perfect, and constructing polymeric materials that have semiconducting prop-erties ef ciently has been a huge challenge. If this challenge can be overcome, poly-mers that are much simpler to manufacture can be used in microelectronics and other advanced technologies.143
The problem with polymers is that in order to have a useable semiconducting property,the conjugated pi-electron orbital systems of organic polymeric molecules must exist in a state that can mimic the delocalization network of traditional inorganic semicon-ducting materials like silicon. The rates of current transfer through conjugated pi-electronsystems currently lag the rates possible with silicon-based semiconductors. However, manufacturing organic electronic materials is much simpler and less costly than tradi-tional silicon/metallic materials. Furthermore, organic materials can be used to create what is known as “ exible electronics,” which have many potential uses.144 For example,
142. Giorgio ell Erba, Alessandro Lu io, ario Natali, u an i , ongyoon i , ong- u i , ong- ong No ,and ario Caironi, “ rganic intergrated circuits or in o ra on storage based on a bipolar poly ers and c argein ec on engineering,” Applied hysics e ers 104, No.15 (16 April 2014).
143. I.G. ill, . illron, . Sc art , and A. a n, “ rganic se iconductor inter aces: electronic structure and trans-port proper es,” Applied Sur ace Science 166 (2000): 354-362.
144. Alan S. ro n, “Fle ible electronics could trans or t e ay e a e and use electronic devices,” ennsylvania State niversity, April 8, 2013, p: ne s.psu.edu story 272086 2013 04 08 researc e ible-electronics-could-trans or - ay- e- a e-and-use-electronic.
138 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
organic electronicscould make them signi cantly more affordable. For organic electronics that are likely to be low processing (e.g., display electronics) and inexpensive, their degradation dueto AEC mechanisms will be less of an issue in terms of material sustainment – at least in environments where they can be easily replaced.
If major breakthroughs occur in the science of organic semiconducting materials, theresult could be organic transistors that perform as well as their inorganic counterparts.We already know that the electrical properties of organic semiconductors degrade dueto the effects of gamma radiation, but it is not clear why that is so.145 One “educatedguess” is that these atomic effects create disorder that disrupts the ability to establish the needed conjugated pi-electron system in these materials. But if newer, high-speedorganic electronics are developed, and these remain susceptible to AEC, then it will beimportant to understand the degradation mechanisms induced by AEC146. The pointis that as organic semiconductors are developed, it is also necessary to explore the degradation mechanisms that may affect their performance and longevity. Given the potential versatility and cost-effectiveness associated with organic microelectronics,there could be a successful future for these technologies in critical DoD systems. Thus, itis in DoD’s interest to further research such materials, and to consider the impacts AECcan have on the reliability of such materials.
Composites are unique hybrids of materials that contain elements of metals, non-met-als, and polymers. Composites can degrade as other materials do, and the impacts ofsmall changes in the molecular structures of these materials could contribute to their eventual macroscopic failure. If and when these materials are used at the micro andnano scales, atomic effects may result in degradation of a composite’s desired prop-erties to a level that is unacceptable for the particular needs of that material. So wecannot rule out signi cant AEC in composites. Given the complex atomic structures and variety of chemical structures contained within composites, however, the investigationand discussion of degradation in composite materials is deferred to the next book ad-dressing biological effects corrosion.
145. L.G. Kaake, P.F. Barbara, and X.Y. Zhu, “Intrinsic Charge Trapping in Organic and Polymeric Semiconductors: A Physical Chemistry Perspec ve,” The ournal o hysical Chemistry e ers 1, No. 3 (2010): 628-635.
146. alaver An um, Rachild Sougrat, Kui Zhao, and Aram Amassian, “Inves ga on o radia on e ects on the proper-es o organic semiconductors using lo -dose TE analysis,” Microscopy and Microanalysis 18, No. 2 (May
AEC In DoD Military Infrastructures and Systems Containing Microelectronics
This appendix provides examples of atomic effects corrosion (AEC) degrading system functionality. The appendix is organized into two parts: the rst part discusses AEC in microelectronics; the second part discusses AEC in the nuclear reactors on Navy sub-marines. The purpose of the appendix is to provide illustrative examples for which AEC matters to the sustained operation of DoD systems and infrastructure.
In 1958 the Department of Defense, in collaboration with the Department of Energy, conducted a nuclear test series under the designation Operation HARDTACK in the Pa-ci c Ocean and Nevada. This series of 35 tests occurred in three parts.1 The rst part was an examination of the basic effects on ground motion, structures, and materials follow-ing a nuclear blast from megaton devices. The second part was aimed at studying the effects of nuclear blasts underwater. The third part was aimed at understanding nuclear weapons in air and ballistic missile defense.
Project 6.3 in Operation HARDTACK was af liated with the rst part of the series. This proj-ect had three objectives, stated as follows:
These tests were analyzing the effects of radiation following neutron uxes of 1012 neu-trons/cm2 s and 10,000 Roentgen (which is approximately 93 Sievert; Sv) of gamma ra-diation. The results of this test series led to the conclusion that the reliability of electronic systems operating in the vicinity of a nuclear blast will likely be compromised.3 Although the precise mechanisms for radiation-induced failures in electronic systems were un-known, by 1961 the DoD knew that electronic systems could degrade due to the effects of radiation.
1. e ense Nuclear Agency, “Opera ng AR TACK I,” Department o De ense (1958), h p: .d c.mil d c trullte t u2 a136819.pd .
2. E.E. Conrad, B. . obriansky, A. Simon, R. . Tucker and F.N. imenit , “OPERATION AR TACK, E ects o Nuclear Radia on on Electronic Fu e Components and Materials,” De ense Technical n orma on Center (April Oct 1958), h p: .d c.mil docs cita ons A A995242.
3. e ense Nuclear Agency, “Opera ng AR TACK I,” Department o De ense (1958), h p: .d c.mil d c trullte t u2 a136819.pd .
140 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The B-52, Navy A4D, and Navy F54 aircraft were also tested to determine the radiation effects on their structural components. No measurements regarding the impacts on the micro- or nanostructures within these aircraft materials were recorded because the nec-essary technologies to do so did not exist. Despite this limitation, it was clear that mate-rial properties could degrade due to exposure to high-energy radiation environments, such as those that exist following a nuclear blast.
In sum, AEC is not a new phenomenon, we now do have the means to measure impact on micro- and nanolevel structures, and we propose that it is time to recognize AEC’s importance in the corrosion spectrum in order to combat the total impact of corrosion on DoD equipment, infrastructures and systems. AEC can directly destroy nanomaterial capabilities, and can indirectly act as a catalyst or nucleating event that leads to accel-erated microscopic and macroscopic material failures, in both cases resulting in a loss of
capabilities. The purpose of this appendix is to examine these two degradation pathways in detail within the context of the equipment, infrastructures, and systems that are important to our military forces. To do so, we have chosen two illustrative examples: we discuss direct damage effects to microelec-tronic systems, and indirect damage effects to Navy nuclear powered submarines.
direct aec damage: loss of capability in microelectronic material properties
This section will provide a more in depth analysis of how materials degradation in micro-electronics due to AEC can adversely affect military equipment, and to emphasize the importance of creating an appropriate material sustainment strategy to combat these impacts. This section is divided into four parts that together provide a complete “story” of AEC in speci c DoD assets that contain microelectronics.
First, we present a historical context regarding the relationship between DoD capabili-ties and microelectronics, to provide background that demonstrates the importance of reliable, trusted microelectronics in DoD assets. Second, we describe the fundamental components of microelectronics systems in order to establish the scienti c underpinnings for explaining how these component parts can be destroyed by phenomena associat-ed with AEC, and how these phenomena can lead to failures in critical DoD equipment.
Third, we provide examples of two types of AEC degradation that can degrade the core components of any state-of-the-art microelectronic component; the point is to demon-strate the importance of a material sustainment strategy that incorporates the impacts of AEC. Due to the almost ubiquitous nature of microelectronics in many DoD assets and the continued application of even more advanced microelectronics, we do not discuss the microelectronics in a speci c system, but rather the mechanisms that can lead to the destruction of virtually any microelectronics component. A complete description of how AEC can lead to the failure of each of the microelectronic systems within a complex
AEC is not a new phenomenon, but it is time to recognize its importance in the corrosion spectrum.
system such as the F-35 ( oint Strike Fighter), for example, would warrant an entire book in and of itself.
Fourth, the nal part of this section focuses on preparing a material sustainment strategy for AEC. In this we discuss current approaches to predicting failures due to AEC and how these can be incorporated into the CPO’s corrosion prevention and control strategies to create a more complete material sustainment strategy that combats materials degra-dation mechanisms throughout the corrosion spectrum.
History of Microelectronics in Military use
Many would argue that no technology advance of the twentieth century transformed the capabilities of the United States military as much as microelectronics. In less than a generation, microelectronics have enabled massive advances in the communications technologies, radar detection systems, and computing capabilities, to name a few examples, compared to what we had during WWII and the Korean War. The electronic systems of the past were limited in their performance by factors such as the size re-strictions of electronic circuit components (e.g., capacitors, vacuum tubes, individual transistors, and so forth). The need for higher performance electronics led the DoD to invest heavily in miniaturizing the components of electronic systems.4 Without these in-vestments by the DoD, it is quite likely the microelectronics industry would be decades behind where it is today.
A primary goal in microelectronics has always been miniaturization. The smaller you can make components for an electronic circuit, the more components you can put into a given volume (e.g., on a single chip) and the more complex con gurations can be designed. The ability to increase the density of components and complexity of design features led to many new capabilities of microelectronics that were not possible in 1904 when the rst diode was invented by ohn Ambrose Flemming.5 In fact, it was the inven-tion of the rst bipolar transistor in 1948 at Bell Telephone Laboratories6 that made the eld of microelectronics possible. Until that time, transistors, the switches in electronic
circuits, were bulky and required the use of vacuum tubes. The bipolar transistor created the ability to move electrons in a controlled manner through a solid state rather than a vacuum tube system. This was the crucial rst step needed for miniaturization.
The original bipolar transistors were about the size of dice (ridiculously large by today’s standards, but orders of magnitude smaller than vacuum tubes); over time, advances in transistor design enabled size reductions to the point that they were eventually the size of a spec of dirt. As transistors began to approach the size at which they could not be seen with the naked eye, a new problem began to emerge. The components on an electri-cal circuit are connected through pieces of metal known as interconnecting wires (or simply interconnects). These interconnects are the roads by which electrical current can
4. ohn . Mote , “The Role o o s Investment in Electronics on the ecline o the Consumer Electronics Indus-try,” ndustrial Cellege o the Armed orces ( ashington C: Aug 1995- Aug 1996), h p: oai.d c.mil oai oai verb getRecord metadataPre html iden er A A314887.
5. o MEA Microelectronics Trusted Source,” ephyr hotonics, 2015, Accessed 28 Sept 2015, h ps:en. ikipedia.org iki ohn Ambrose Fleming.
6. Peter Ashburn, Si e etero unc on ipolar Transistors (England: ohn iley Sons Ltd., 2003), 1, 2.
142 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
travel, and the complex orchestration of the ow of electricity through the circuit gives it the ability to do things such as compute and store information. As components became smaller, more components could be placed onto chips, but this led to a problem of numbers of interconnects. At the time, chips were assembled by hand and the military requirements for chips were becoming sensitive enough that consistency in interconnect length and thickness (and thus electrical resistance) began to matter. What this meant was that a new method of chip manufacture was needed that didn’t require circuits be built by hand.
In 1959, ack Kilby of Texas Instruments helped solve this problem with the invention of the integrated circuit (IC).7 This pursuit was driven largely by the needs of the space race and demands associated with the Cold War. In the 1960s, the DoD’s Minuteman program, a nuclear-armed ballistic missile program, required approximately 4000 ICs per month.89 This program was needed to ensure military superiority during the cold war by deterring other nations from engaging in open con ict with the United States for fear we could overmatch them in a nuclear exchange.10 At the same time, the DoD was also investing heavily in the development of satellites for multiple purposes, from communications to surveillance to remote sensing. Combined, these programs meant that the DoD required not just more, but better, miniaturized electronic components. Increased funding into microelectronics R D resulted in the development of new transistors and ICs that cre-ated breakthroughs in new applications such as phased array radar and smaller-scale computer technologies; improved ICs enabled the higher processing speeds required to make these new systems viable.
By the 1970s, following the DoD’s support of the very high-speed integrated-circuit ( HSIC) program, major weapons systems began to incorporate increasing numbers of electronic components, leading to improved capabilities. ICs were included in nu-merous advanced systems, such as the F-16 ghter, Trident ballistic missile submarine, and also smaller systems such as Stinger, Maverick and TOW guided missiles.11 As DoD systems incorporated ICs, commercial IC applications were also becoming a viable market for industry. As commercial IC applications expanded, industry began regarding commercial applications as a lucrative marketplace. As a result, DoD eventually lost the leadership role in the microelectronics market. With commercial applications driving advances in microelectronics, DoD struggled to ensure the defense systems that relied on microelectronic components incorporated the latest state-of-the-art microelectron-ics. Furthermore, as commercial markets continued to develop, “disposable” electronics became more common: why would a consumer try to maintain the 100 electronic calculator when he could replace it with a better model for 20. Such economies were not available, however, for sophisticated weapons systems. Thus, the DoD was faced
7. “The istory o the Integrated Circuit,” o elpri e.org, May 5 2003, Accessed Sept 29, 2015, h p: .nobel-pri e.org educa onal physics integrated circuit history .
8. ohn . Mote , “The Role o o s Investment in Electronics on the elcine o the Consumer Electronics Indus-try,” ndustrial College o the Armed orces ( ashington, C: Na onal e ense University, 1996).
9. “Minuteman Missile istory,” Strategic Air Command, Accessed 29 Sept 2015, h p: .strategic-air-com-mand.com missiles Minuteman Minuteman Missile istory.htm.
10. “Air Force istories Released through Archive La suit Sho Cau ous Presidents Overruling Air Force Plans or Early Use o Nuclear eapons,” The a onal Security Archive (George ashington University, 30 April 2008), h p: nsarchive.g u.edu nukevault ebb249 .
with the need to maintain sophisticated systems for long life-cycles in a microelectron-ics market that was simply throwing out old devices and replacing them with newer, better, less expensive models. et even with regard to microelectronics components, DoD could not simply insert newer commercial ICs because they were not compatible with other existing system components. In sum, the DoD faced a dilemma: it was costly to custom build their own state-of-the-art microelectronic components, but they could not simply swap out the more affordable state-of-the-art microelectronics designed for commercial applications.
This problem still exists within the DoD today. High-volume microelectronics are designed almost exclusively for commercial applications, and new generations of microelectron-ics emerge every few years. On the other hand, the DoD has to integrate electronic components into sophisticated systems, such as the like the F-35, that take years to de-velop. As a result, the microelectronics in many new systems are out of date compared to commercial designs before the new systems are even elded. In order to manage the costs associated with elding and maintaining sophisticated systems, microelectronic components must last much more than the few years common to commercial micro-electronic systems.12 Thus, understanding all the ways in which microelectronic compo-nents can degrade, to include considering the harsher environments in which DoD sys-tems must operate, is extremely important. This means the DoD must understand the impacts of AEC on systems containing microelectronics components, and develop ma-terial sustainment strategies to prevent their premature failure, thus ensuring they func-tion reliably when the military needs them.
Microelectronics, as the name suggests, are made of the same basic components as tra-ditional electronics – e.g., transistors, resistors, capacitors, inductors, and diodes – except their individual component dimensions are many times smaller than can be seen by the naked eye. In recent years, components have reached sizes of less than 10 nm, which is well within the range where single atom defects can adversely affect a component’s performance. This section will brie y review the various types of basic components used in microelectronics, how they function, and some of their common uses. Understanding how a system’s components work helps to understand how the components can fail, and the con-sequences their failures can have on the overall system.
Electronics are so named because they make use of the ow of electrons in materials: for example, making calculations and storing information by moving electrons around and placing them in speci c locations. Individual components interact with each other, and external users interact with the electronics system as a whole; electric potential dif-ferences, also known as voltages, make the movements of electrons and interactions of electronic components possible. In the next few paragraphs, we brie y overview elec-tronic component functions.
12. epartment o e ense, “ epartment o e ense Assured Microelectronics Policy,” ce o the nder Secretary o De ense or Ac uisi on, Technology, and ogis cs, uly 2014.
DoD has to integrate
electronic components into
sophisticated systems that take years to develop.
144 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Resistors resist the ow of electric current, and in doing so generate a measurable volt-age drop as electric currents move through resistive components.13 All objects have a natural resistance to electric current; the amount of resistance depends on the speci c material, as well as the size and shape of the object. When used in electronics, resistors must have a speci c, known resistance so that designers can predict what voltages need to be applied to achieve desired results. In normal electronics, the type of material is the main factor in determining the value of an individual resistor, but as microelectron-ics become smaller and smaller, the size and shape of a resistor takes over as the domi-nant factor determining the value of a resistor. The dimensions become so small, in fact, that even the electrical resistance of components not used as resistors must be carefully taken into account. Therefore, considering the electrical resistance of all microelectron-ics components in uences the design and physical layout of the entire system. Since the typical distance between two atoms in a microelectronics component is roughly half a nanometer, when entire component sizes are only 10 nanometers or less, a change in the properties of one atom in that component can change the dimensions of that component signi cantly, and in turn alter its resistance.
The purpose of capacitors in electronics is to store charges (electrons and positively charged ions). They are composed of two pieces of electrically conductive material, the electrodes, which are separated from each other by an electrically insulating mate-rial, the dielectric. These individual electrodes are then connected to the circuit. Applied voltages cause electrons to accumulate on one electrode, which causes an excess amount of electrical charge and attracts positive ions in the other electrode towards it. The insulating material between the electrodes, however, prevents the electrons from travelling directly between the electrodes. It is only when the electrodes are connected to the circuit, and a full path through conductive material opens up, that the electrons can ow from the electrode where they have been stored to the other electrode, and balance the electric elds. In order for a capacitor to function correctly, electrons must not be able to pass directly between the two electrodes, thus the dielectric is a critical part of the capacitor. On the macroscopic scale, many materials are suf ciently insulat-ing that passing an electric current through them is extremely unlikely. However, when capacitor dimensions are reduced to only a few nanometers thick, there are very few materials capable of preventing at least a few electrons from passing through them. Fur-thermore, some dielectrics can increase the amount of charge a capacitor can store, not through stronger insulation, but instead through the ability to polarize, meaning that even smaller degradations in their performance can allow them to pass current and cause the capacitor to fail. Capacitors designed for today’s microelectronics have ex-tremely exacting properties, and even slight deviations can cause signi cant changes.
Inductors are coils of wire and they function to resist changes in electrical current; that is, inductors are used to smooth out uctuations in current. Inductors are used almost exclusively in analog circuits. In the current digital age, analog circuits are becoming
13. Because o Ohm s la , hich states that the si e o the voltage in an ob ect is propor onal to the si e o the cur-rent o ing through that ob ect, mul plied by the resistance o that ob ect: IR.
increasingly rare, but there are still specialized applications, such as communications and signal recording, in which inductors are used. Faraday’s law states that any change in an electric eld (or current) generates a magnetic eld, therefore an inductor gen-erates magnetic elds when operating. These magnetic elds extend into the region surrounding the inductor. Magnetic elds, especially changing ones, are often danger-ous to electronics. Engineers attempt to take magnetic eld generation into account when designing microchips that use inductors; however, engineering models are neither completely accurate, nor do they always account for the elds produced by a mis ring or improperly operating inductor. Inductors thus present not only the risk of degrading themselves, but in the process of degrading also induce the added risk of their magnetic elds causing the degradation of surrounding materials. As inductor dimensions become
smaller to meet the demands of modern state-of-the-art microelectronics, the integrity of their underlying lattice structures increases.
Diodes function as one-way gates. Today’s diodes are almost exclusively solid-state, made from semiconductors. The way that unidirectional current ow is achieved is by sandwiching two pieces of the same material together. One piece, however, has been doped with atoms that add extra electrons to the material (called n-doped), while the other piece has been doped with atoms that add extra holes (called p-doped). When the two pieces are placed in contact with each other, the extra electrons and holes in the region surrounding the contact point can move across the contact boundary and cancel each other out. The region around the boundary where this charge cancellation happens is called the “space-charge region.” The movement of electrons and holes across the boundary is mainly possible because the n- and p-type pieces are made of the same material, which minimizes other differences that would restrict such electron movement.
In the resulting setup, illustrated in the gure below, one side of the diode has excess holes to carry electrical current, and the other side of the diode has excess electrons to carry current, but the center of the diode has a region with no particles available to
Diagram of the diffusion across a pn junction, with the resultant uncovered space charges, the electric eld and the drift currents/Inductiveload
146 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
carry current. When the diode is hooked up to a circuit, however, if the voltage is placed across the diode in one direction (left to right, for example, in the gure below) then it pulls some of the electrons back over to the n-doped side, which shrinks the space-charge region, allowing current to ow in that direction across the diode. If the voltage across the diode is in the other direction, however, more electrons will be pushed into the p-doped side and will simply ll the holes, and the circuit will not conduct current. One can also think of the voltage as causing the space-charge region to grow, strengthening
the blockade for current across the diode. The purpose of a diode is to allow current to ow in one direction but not the other. For diodes, and p-n junctions in general, the prop-
erties of the p- and n-doped regions must be controlled in order to work properly. AEC that causes degradation of either side, or of the space-charge region in the center, can either cause the blockade to break down and allow current to ow in both directions, or to persist when it should not and therefore block all current from owing.
By far the most common component in microelectronics is the transistor. A transistor acts like a gate for electrical current. When the gate is open, the transistor can conduct electrical current. When the gate is closed, current will not ow through it. To achieve this function, transistors use the advantages of doping, similarly to the p-n junctions used in diodes.
The most basic type of transistor is a bipolar junction transistor (B T), and it is formed by two similarly doped regions of a semiconductor separated by a thin region of oppositely doped semiconductor. It is very similar to placing two p-n junctions next to each other. The outer pieces can be electron doped, called an n-p-n type, or they can be hole doped, called a p-n-p type. Figure 2 shows the basic design of a B T. For explanation
The basic operation of an NPN B T in Active mode/Inductiveload
purposes, we will describe an n-p-n type B T. This type of transistor differs from two simple diodes connected to each other in opposite orientations in that one of the n-type re-gions is more heavily doped than its counterpart. The more heavily n-doped section is called the emitter and the less heavily n-doped section the collector, with the p-doped region in between called the base.
The mismatch in doping levels between the two electron rich regions means that current will naturally ow from the emitter to the collector, however the opposite doping in the base prevents this. The base is electrically connected to the rest of the circuit as well, and a voltage applied to it determines how high or low its resistance is to the ow of electrons from the emitter to the collector. When the resistance is low the gate is open, and when the resistance is high the gate is closed.
The amount of voltage needed to control the base in a B T is extremely small, especially compared to the voltage difference across the junction that can be achieved, meaning that a small change in voltage can control a much larger change in voltage, making B T transistors extremely useful for amplifying signals, as switches, or as components of logic circuits. Because the difference in doping of the n-regions is what makes the B T work, it is inherently designed to only work in one direction, different from the other basic type of transistor (the eld effect transistor), which can work with current owing either direction.
The gure below shows the layout of a eld effect transistor (FET). Instead of an emitter and collector, electricity ows through a transistor from the source region into the drain region. The source and drain regions are surrounded by what is commonly called the bulk region. ust as with the B T, we will describe the case when the source and drain re-gions are n-doped and the bulk is p-doped, but FETs can also have p-doped source and drains, with an n-doped bulk. A thin layer of insulating material is placed on the surface of the bulk between the source and drain. A conductive material is then placed on top of the insulating layer, forming what is called the “gate.”
Field effect transistor of the n-p-n type/ Cyril BUTTA
148 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Both electrons from the source and drain, and holes already present in the bulk, popu-late the region in the bulk directly between the source and drain. These opposing charg-es cancel each other out, so that no charge carriers remain to conduct current within that region, named the charge depletion region. Both the source and drain are equally doped, meaning that when the transistor is not connected to anything, there is no elec-tric eld that would cause current to ow between them. However, when voltage is ap-plied between the source and drain regions, a current can ow through the bulk, around the charge depletion region. Applying a voltage to the gate can have two different ef-fects on the transistor: negative voltage applied to the gate, brings more electrons near it, expanding the charge depletion region and cutting off the ow of current through the bulk; positive voltage applied to the gate pushes electrons away from it, shrinking the charge depletion region and allowing more current to ow. Electricity can ow either direction when the channel is open, and the source designates the region where the current ows into the transistor. Thus the n-doped region on the left in Figure 3 can be the source at one point in time, or the drain at a later point. The bi-directional nature of FETs makes them more versatile than B Ts.
A simpler, modi ed version of the FET, known as the junction eld effect transistor ( FET) uses the same principle described above, except the gate closes off a conducting channel instead of opening one. In the design of a FET, shown in the gure below the source and drain regions are not separated and, instead, are merely part of the bulk. The bulk region is made up of a doped semiconductor with a very narrow section, and the gate is merely a region of oppositely doped material next to the narrow section of the bulk. The gate is controlled by a voltage that, when increased, attracts the doped charge carriers in the narrow section of the bulk to the gate region, effectively pulling them out of the bulk and creating a charge depletion region that stops electrons from owing through the bulk.
Scheme of n-junction eld-effect transistor de/ Norro
No transistor works perfectly, meaning that the ow of electricity across the bulk or charge depletion region (CDR) can never be stopped completely, or open to the point of causing zero resistance. Furthermore, switching the base from closed to open requires that carriers be injected into or removed from it, and opening up the CDR requires that electrons travel through the bulk to that region, which does not happen instantaneously. Research in transistor technology seeks not only to make the transistors physically smaller, but also to improve how well the base can insulate in the “closed” state, how well it can conduct in the “open” state, and how reliably and quickly it can switch between those states.
Transistors perform different functions, such as gates or ampli ers, and their speci c func-tions are controlled by many different design parameters. Therefore it is important not only to understand how transistors function, but the different parts they play in system-level applications. There are entire books written on this topic; to illustrate it, let’ use the communications system in an unmanned aerial vehicle (UA ) as an example.
A drone’s rst step in communicating with its pilot is receiving the control signal. This sig-nal has been sent from some distance away and the signal strength is usually relatively small; also, the control signal is embedded in the surrounding “noise” of electromagnetic waves of many different frequencies from many other sources. Inductors and capacitors are used to isolate a single desired frequency from the cacophony the UA antenna picks up. If any of those components deteriorates signi cantly, then the antenna won’t be able to isolate the intended frequency, and therefore won’t even receive the com-munication from the pilot. Assume for the purpose that there has been no degradation, and the control signal is successfully detected. That signal will rst be ampli ed, most likely by serving as the controlling voltage for a larger current running through a B T. Once the signal has been boosted, it must be converted from an analog wave to a digital signal of ones and zeros, a process that heavily employs transistors and diodes. Failure at this step compromises the communications packet.
If the instructions from the pilot are successfully received, ampli ed, and converted, the digital signal must then be analyzed by the drone’s onboard computer. By far the most common use of transistors is as logic gates, which are the basic building blocks of processor chips. Metal Oxide Semiconductor Field Effect Transistors (MOSFETs) are most frequently used for this function. When any computer analysis job is performed, current ows through a series of logic gates, and the speci c computations determine which
gates are open and which are closed, which controls where the electrical current ows and thus the outcome the computer reaches. When a transistor inside a chip fails, that can affect one type of calculation or many, depending on where the transistor is placed and its role in the computation. A transistor failure could cause a slight miscalculation in the instructions received, or a complete failure of the communications system in the drone to interpret the pilot’s instructions. The results of the instructions control the com-ponents (e.g., motors that control the ight surfaces, or weapons release controls) within the drone. These components also include microelectronics that are involved in carrying out the instructions. So even if the central computer functions properly and can commu-nicate with its pilot, failures of the electronics in the motors that steer the drone or release its payload could have catastrophic results. Therefore the speci c use of the transistor, in addition to its design, determines the nature of failures that might happen.
150 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Fundamentally, an AEC-induced fault in a single micro component such as a transistor could result in a macro system failure. As we have already said, as the components in microelectronics become smaller, single or a few atomic effects could lead to that com-ponent failure. The future of microelectronics is nanoelectronics. Components of elec-tronic circuits are going to continue to decrease in size, and future DoD systems are go-ing to incorporate new electronic systems composed of nanomaterials that will be extremely susceptible to the impacts of AEC. The basic principles that govern the com-ponents (i.e., diodes, transistors, etc.) of current microelectronics will continue to be used in the nanoelectronic components of the future. As the DoD acquires future systems, a complete material sustainment strategy needs to consider how AEC can lead to failures in DoD systems due to changes in the underlying atomic properties of microelectronic components, as well as other “traditional” forms of corrosion.
Degradation of Microelectroincs By AEC
In this section, we present a more detailed discussion than that in chapter 2 regard-ing single event effects in microelectronics caused by AEC. These effects represent the “direct” types of damage that can be caused by AEC: that is, AEC that can lead to component failures. Following this description, we provide an example of how AEC in
a microelectronic circuit can catalyze degradation of that circuit, as well as showing how failure to consider such impacts can impair the ability to predict material failure with accuracy. These degradation events represent how “indirect” damage can also occur in microelec-tronics due to AEC, and these effects can become the catalysts for classical degradation.
Single Event Effects in Microelectronics
Currently, the main concern with radiation effects on microelectronics relates to “single event effects” (SEEs). These include single-event upsets (SEUs) wherein a bit within the microcircuit is changed from its correct value. In a memory chip, this can change the stored value. Multi-bit upsets are also possible, wherein a set of bits are changed. For the most part, SEEs are “soft errors,” meaning that the damage is limited to the error, and that any permanent damage is insigni cant and inconsequential. It is however possible, for a SEE to cause a “hard error,” wherein some part of the microcircuit is permanently dam-aged. For example, a “single event latchup” (SEL) can, in some instances, cause high currents that damage channels or junctions to cause a hard error. Single-event upsets (SEUs) are particularly problematic for SRAM Field Programmable Gate Arrays (FPGAs), and are becoming more signi cant as geometries continue to get smaller.14 A change to the stored bit stream that programs the FPGA can cause a program error, which might cause a failure upon execution. Whether a soft or hard error, radiation-caused events typically cause a degradation of the microelectronic device.
14. r. Keith E. olbert, “Single Event E ects,” Ari ona State niversity, 18 an 2006, Accessed 7 Oct 2015, h p:holbert. aculty.asu.edu eee560 see.html.
AEC can lead to component failures.
Most of the consequences of single-event effects are due to ionization tracks from charged particles that are emitted due to a nuclear event within the chip. These events are instigated by external radiation with a source typically from one of the following:
• A galactic cosmic ray that has made it through the atmosphere to arrive at the terrestrial level to interact with the microelectronic device, or a byproduct of a cosmic ray in a cascade event in the atmosphere. The particles of signi cance are generally neutrons.15
• Alpha particles emitted as radiation from a contaminating source in close proximity to the semiconductor. These can originate from uranium or thorium contaminants in packaging material, from an alpha emitter such as a byproduct of a lead isotope in solder, or an alpha particle cosmic ray.
• A decay product from an isotopic transmutation that has taken place by virtue of the absorption of a neutron within the active layers of the microcircuit (i.e., neutron activation within the microchip). For example, absorption of a cosmic neutron in an elastic collision with a silicon atom nucleus.
• Neutrons produced by radioactive materials or other sources of nuclear particles. Neutrons will pass through many materials, so special shielding is often required, and the shielding material can subsequently cause secondary emissions.
SEEs are typically instigated by linear energy transfer (LET), which is categorized ac-cording to a measure of energy deposited in a material. High-LET radiation is generally caused by protons, neutrons, or alpha particles. Low-LET radiation comes from photons (including -rays and gamma rays), electrons, positrons and muons.16 In either case, en-ergy is transferred to create a shower of ion charges deposited into the microelectronics material, creating electron-hole pairs, some of which can be trapped and change the properties of the electrical components such as diodes, capacitors, and transistors. At suf cient energy levels, transients in microelectronics at reverse bias junctions can cause irreparable damage. Exceeding the peak reverse bias on a diode can cause break-down, which is why static discharges are avoided with microelectronics. Both high and low LET events can cause problems as gate sizes in transistors become extremely ne.
Traditionally, the reliability of microelectronics is measured in Failures in Time (FIT). One FIT is equivalent to one error (hard or soft) per 109 hours (one billion hours) of operation. Soft error rates in microchips can vary from a few hundred to many thousands of FITs.17 At 100,000 FIT, one can expect roughly one error per year of continuous operation. Hard error rates are expected to be less than 10 FIT. For SRAM memory chips with gigabit capacities, soft error rates of 50,000 FIT are typical, according to one source.18 For most consumer applications, this is not a signi cant problem, especially given that most con-sumers replace their computers, cell phones and other devices every few years.
15. “Measurement and Repor ng o Alpha Par cle and Terrestrial Cosmic Ray-Induced So Errors in Semiconductor evices,” EDEC Solid State Technology Associa on (Arlington, A) 2001.
16. Claude Leroy and Pier-Giorgio Rancoita, rinciples o Radia on nterac on in Ma er and Detec on ( orld Scien c, Sep 2011).
17. Santosh Kumar, Shalu Agar al, and ae Pil ung, “So Error Issue and Importance o Lo Alpha Solders or Micro-electronics Packaging,” Rev. Advanced Materials Science 34 (2013): 185-202.
152 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
For certain DoD applications, this could be problematic, both due to their operating en-vironments and the extended life cycles we expect from military systems. For example, aircraft ying at an altitude of 30,000 feet or higher are subject to neutron densities hun-dreds of times higher than at sea level. One can expect FIT rates for soft errors to increase proportionately. For hard errors, greater scaling is possible as multiple events in proximity within a microchip might compound problems, causing a degradation that eventually results in failure. Much research relates to NASA and DoD satellite systems, where it is understood that microelectronic components are subject to various kinds of radiation ef-fects, both within the earth’s atmosphere and outer space. For NASA, a single event up-set (SEU) is de ned as “radiation-induced error in microelectronic circuits caused when charged particles (usually from the radiation belts or from cosmic rays) lose energy by ionizing the medium through which they pass, leaving behind a wake of electron-hole pairs.”19 As such, a SEU is typically a soft or recoverable problem, but can also cause degradation of the material. When an SEE causes a hard error, it is clearly a degrada-tion event. In space electronics, SEUs are caused by galactic cosmic rays, cosmic solar particles, and are often heavily in uenced by solar ares or protons trapped in radiation belts. There are various other kinds of single damage events including single event tran-sients (SETs), single event latchups (SELs) and single event burnouts (SEBs). Cumulative damage is also possible due to repeated ionizing events that overlap in critical areas.
In terrestrial applications, the radiation of consequence is most likely to be neutron events from cosmic rays and nearby radiation sources, and alpha particles from near-by materials. These events may be rare, but can cause upsets and reliability problems, and might become more consequential in new forms of microelectronics. Similarly, electronics con ned to the earth’s surface in close proximity to high neutron uxes can experience higher rates of SEEs, and potentially greater rates of hard errors, including degradation-induced failure. For example, electronics embedded deep within a nu-clear power plant might be well-shielded from gamma radiation, but still experience high neutron ux density.
U.S. industries are developing microchips with increasing numbers of nanometer-sized components, yet we counter that advantage by having to use “brute force” design techniques such as incorporating multiple redundancies into those chips so that if one component fails, a backup component is available to pick up its function. This design also introduces additional computational (processing) requirements to check whether or not
the primary component has failed so a backup needs to take over. If, however, we can understand the of AEC degradation and their implications on nanotechnol-ogy systems, then we may be able to devise other ways to overcome these AEC effects. As a result, we may no longer need to resort to building in redundancies, or may at least be able to reduce redundancies. This is one motivation behind addressing AEC as a degradation/corrosion mechanism – and
19. Claude Leroy and Pier-Giorgio Rancoita, rinciples o Radia on nterac on in Ma er and Detec on ( orldScien c, Sep 2011).
U.S. industries are developing microchips with increasing numbers of nanometer-sized components.
it is why this non-classical degradation phenomenology is important to understand in order to promote improved material sustainment policies.
AEC Catalyzed Electromigration in Microelectronics
The DoD has many assets that critically rely on microelectronics and thus identifying the various phenomena that can cause degradation in these systems is essential for proper material sustainment strategies. The goal of material sustainment is to ensure that acquired systems last for their expected lifetimes, require minimum maintenance, and remain reliable.
In order for the DoD to properly manage their systems to maximize their life cycles a thorough understanding of the effects that lead to their degradation is needed. In sys-tems that critically depend on microelectronics to operate it is important to understand the various chemical and physical phenomena that can lead to their degradation. An area of degradation effects that is receiving more attention as the line widths between electronic interconnects approaches single digit nanometers is material migration.20,21,22 Material migration can refer to metal atoms/ions diffusing due to chemical or tempera-ture gradients; as a result of mechanical stress; or as a result of an interaction with an applied electric eld.
The migration of materials due to an applied electric eld is also referred to as electromi-gration. Of the different mechanisms by which atoms in material materials can migrate, electromigration is likely the most in uenced by interactions of materials with radiation (i.e., AEC). In an electrical circuit, the interconnects are typically made of a conduct-ing metal such as Cu or Al and these are polycrystalline structures constructed of grains that are identical in their lattice structures, but arranged in different orientations (see the gure below).23
20. ens Lienig, “An Introduc on to Electromigra on-A are Physical esign” Proc. O the Int l Symposium on Physical esign, Dresden niversity o Technology ( resden, Germany: 2006).
21. iroka u Tanaka, “Factors leading to ionic migra on in lead- ree solder” ES EC Technology Report, No. 14 ( an 2007).
22. Shigeharu Yamamoto, “ o impuri es a ect ionic migra on, and ho to counter their impact” ES EC Technology Report, No. 22 (1 Sept 2006).
23. Lienig, . (2006), “An Introduc on to Electromigra on-A are Physical esign” Proc. O the Int l Symposium on Physical esign I.
A visual representation of grain boundaries/Wlytle1375
154 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
The consequence of this arrangement is that the areas where two grains touch (grain boundaries) represent a weakness in the entire polycrystalline structure because the metal atoms/ions at these edges are more weakly bound to the grain. As a result, these edge atoms/ions are susceptible to migration across the grain boundary when exposed to an appropriate force.
In microelectronics, the force that facilitates electromigration is caused by current ow-ing through the interconnects. The current is the ow of electrons moving through the conductive material, much like water that ows through a riverbed. This ow of electrons creates two forces that can act upon the metal ions/atoms, especially those at the grain boundaries, and dislodge them from or the change their orientation in their lattice struc-ture. The rst force is the force from the applied electric eld (F eld) in the interconnect and the second force is caused when the electrons owing through the conducting metal transfer some of their momentum to the metal ions/atoms in the polycrystalline lattice (Fwind). This force is commonly referred to as the “electron wind” and is typically the major force behind electromigration.24
When the force of the electron wind reaches a particular threshold, metal ions/atoms at the grain boundaries will begin to migrate in the direction of that force and typically in the direction of the grain boundary as well. Overtime, the migration of metal ions/atoms from the grain boundaries can lead to two types of formations that can facilitate the failure of the circuit known as hillocks and voids.
Hillocks are protrusions out from the surface of the crystal lattice that can cause shorts between adjacent interconnects and voids are holes within the polycrystalline lattice that reduce the current ow, increase current density, and eventually lead to intercon-nect failure (interconnect no longer conducts).
The likelihood an electronic interconnects will fail due to the accumulation of voids and/or hillocks is somewhat calculable thanks to the work of .R. Black who developed a model to estimate the mean time to failure (MTTF) of a wire.25 The equation derived from his work predicts the half life of a wire and is given as:
where A is a constant derived from the cross-sectional area of the wire (units ), is the current density (units ), n is a scaling factor determined to be 2 by Black, EA is the activa-tion energy needed to dislodge a metal ion/atom at the grain boundary in oules, k is
24. Lienig, . (2006), “An Introduc on to Electromigra on-A are Physical esign” Proc. O the Int l Symposium on Physical esign I
25. ames R. Black, “Electromigra on - A Brie Survey and Some Recent Results,” EEE Transac on on Electron Devices 16, No. 4 (April 1969): 338-347.
the Boltzman constant (1.38 x 10-23 /K) and T is the temperature in Kelvin. From looking at this equation it should be obvious that current density and the temperature of the wire are major factors in the MTTF.
The Black’s equation allows one to predict the lifetime of a particular circuit design with respect to failure from electromigration. The output of this equation is affected by many of the design choices for a particular circuit such as: the wire material, the wire tempera-ture, the wire size and metal slotting, the wire length, the via arrangements and corner bends, and the terminal connections. What is also evident from this equation is that additional energy added to the system in the form of radiation can also accelerate the degradation processes due to electromigration.
When radiation penetrates microelectronics they can interact with the environment and material in a number of ways (many which have been described extensively throughout this book). The exact nature of the interaction will depend on the type of radiation as particulate radiation, such as neutrons, and electromagnetic radiation, such as gamma photons, will cause different effects. The impact of particulate radiation can weaken the strength of the crystal lattice lowering the required energy needed to force a metal atom/ion at the grain boundary to migrate. Electromagnetic radiation can facilitate the Compton effect (and effects like it) that disrupt the ow of electrons leading to potential changes in the properties of the interconnect and could even increase the affect of the electron wind. The overall conclusion here is that the AEC caused by radiation can decrease the MTTF by accelerating the forces that lead to the degradation of the func-tion of circuit interconnects. Most important is that e e ua i n e n n ain a erm a in r ra e e re uen r ma ni u e ra ia i n e en an ere re
e la e ua i n un ere ima e e ra a i n im a in en ir nmen ere ma erial are u e e e en mena a au e .
Despite this limitation, people and organizations are trying to bring awareness to the important reality that future microelectronics designs are going to suffer more from deg-radation events such as electromigration. Strategies are being developed in an attempt to mitigate these effects in the design stage. One such proposal, referred to as the elec-tromigration-aware physical design ow, has already been implemented and veri ed in a commercial design for analog and mixed signal integrated circuits for automotive applications.26,27 While plans such as this are the important steps in material sustainment strategies, the current plans fail to address the role AEC plays in accelerating degradation events such as electromigration. More research into the exact role AEC induced by radiation needs to be per-formed in order to increase the predictive power of equations such as Black’s equation and lead to better design strategies to
26. G. erke, and . Lienig,“ ierarchical current-density veri ca on in arbitrarily shaped metalli a on pa erns oanalog circuits,” EE Transac ons on Computer Aided Design o ntegrate Circuits and Systems 23, No. 1 ( an2004): 80-90.
27. G. erke and . Lienig, “Reliability-driven layout decompac on or electromigra on ailure avoidance in complemi ed-signal IC designs, roc. Design Automa on Con (2004): 181-184.
Strategies for material sustainment
need to include bottom-up
models that include AEC.
156 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
mitigate the degradation events that will become more common in microelectronics as electronic components such as transistors and line widths between interconnects con-tinue to get smaller.
Planning the Future for AEC in Microelectroincs
As the Services continue to rely on microelectronics in their assets, and develop new systems that incorporate more state-of-the-art microelectronics, strategies for material sustainment will need to include “bottom-up” models that describe how materials deg-radation can occur through phenomena that cause AEC. As mentioned many times before in this book, the goal of material sustainment is material reliability throughout the material’s life cycle. When the materials are the components of microelectronics systems, a precise understanding of the atomic properties of each material and how the environment can manipulate and change these properties is needed. The CPO is cur-rently charged with ensuring material sustainment strategies aimed at preventing and controlling the degradation of DoD materials. Therefore, the CPO’s corrosion prevention and control strategies that are core to their material sustainment approach need to in-corporate the ways that materials such as those used in critical microelectronics systems can degrade due to AEC.
To date, there is insuf cient understanding of how the properties of microelectronic ma-terials change throughout their life cycle due to interactions with their environment. The microelectronics that will be built into future military avionics or other equipment will need to be understood from the bottom-up in order to ensure low failure rates can be designed into future systems, particularly as the importance of AEC increases with de-creasing microelectronic feature sizes. Currently, high-volume (and thus low cost) micro-electronics are developed for commercial applications, which have expected 3-7 year lifetimes.28 The requirements of most military assets containing microelectronics exceed these expected commercial lifetimes by factors of 3-10. Consequently, the DoD needs well-developed material sustainment strategies to ensure that microelectronics-depen-dent systems will continue to function reliably during their DoD life cycles. This strategy has to consider how the phenomena that cause AEC in microelectronics can impact the reliability of those microelectronics.
A major step towards this type of strategy was made in 1994 when then Secretary of De-fense William Perry issued a memorandum that stopped the use of MIL-HDBK-217 series, which was the military handbook used for reliability prediction of electronic equipment.29 This handbook utilized several different exponential models known as constant failure rate (CFR) models to explain when microelectronic components would fail. In the 1990s it became increasingly clear that the CFR models were unable to explain the unique ways complex IC designs were failing, and the “Perry Memo” was the response. In addition to
28. Mark hite and oseph B. Bernstein, “Microelectronics Reliability: Physics-o -Failure Based Modeling and Li e me Evalua on,” et ropulsion a oratory (Cali ornia Ins tute o Technology, CA: Feb 2008).
29. O ce o the Secretary o e ense, illiam . Perry, Memorandum or Secretaries o the Military Departments ( ashington, .C.: 29 une 1994), h p: s -eng. alls-church.va.us perry94.html
eliminating the use of the MIL-HDB-217 series, Secretary Perry’s memo encouraged the DoD to adopt industry standards for quality assurance of microelectronics.
Much of industry uses what is known as a physics-of-failure approach when it comes to reliability modeling for microelectronics components.30 This approach attempts to un-derstand the physics of failure (i.e., a bottom-up approach) that requires understanding how materials degradation leads to failure at the atomic scale. The CFR approach did not incorporate physical mechanisms because it modeled failure as a mathematical distribution wherein failures were due to random chance. Furthermore, these models failed to account for how multiple initiating events could eventually lead to failure; the CFR approach assumes microelectronic components only fail because of a single type of failure. The physics-of-failure approach considers all potential failure mechanisms that are chemical, electrical, physical, mechanical, structural, or thermal in nature. In doing this, a mathematical model founded in the physical structure of the material at the small-est possible scale is created through experimentation and computational modeling. The ultimate output of this approach is an equation for the dominant failure mechanism of the microelectronic system and its mean-time-to-failure (MTTF). Physics-of-failure ap-proaches include models such as Black’s equation discussed in the previous section. As discussed there, these models clearly have room for improvement to incorporate the impact of AEC on materials degradation in microelectronics.
Even though there are now better models that can be incorporated into material sus-tainment strategies for microelectronics, many engineers still rely on MIL-HDBK-217 when they go about designing new microelectronic circuits.31 Planning for the impact of AEC on microelectronic components is not a new concept or idea. Both NASA and DMEA are aware of the importance of physics-of-failure models in assessing microelectronics reli-ability. Both organizations have been engaged in efforts to ensure that microelectronics acquired by NASA or the DoD are resistant to the impacts of AEC.
The CPO can coordinate the research needed to expand these excellent efforts, with the goal of ensuring that bottom-up predic-tive models are being employed and developed assess all possible microelectronic failures due to AEC. This means coordinating mate-rial sustainment strategies for microelectronics with NASA and DMEA (and others working in similar areas) to ensure that the most bottom-up predictive models, founded in the laws of physics and represent-ed at the smallest scale possible, are being used by the Services as they consider the life cycles of existing and future microelectronic components.
30. Mark hite and oseph B. Bernstein, “Microelectronics Reliability: Physics-o -Failure Based Modeling and Li e me Evalua on,” et ropulsion a oratory (Cali ornia Ins tute o Technology, CA: Feb 2008).
The CPO can
158 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
indirect aec damage: loss of capability in nuclear reactor material properties on navy submarines through lattice defects
The purpose of this section is to provide a speci c example of the impact atomic ef-fects corrosion can have on a military platform that is critical to our national security. Navy nuclear submarines (SSNs, guided missile submarines – SSGNs, and ballistic missile submarines – SSBNs) use nuclear power to operate, and their materials, particularly in the vicinity of reactors, are exposed to highly irradiative environments. This expo-sure leads to materials experiencing atomic effects corrosion. For these materials, the atomic effects can start as nucleating or catalyzing events at the nanoscale that eventually lead to macroscopic property failure and the need to replace or decom-mission the nuclear reactor.32
In the near future, the Navy intends to replace its current Ohio-class (SSBN/SSGN) nuclear powered submarines.33 By combining both science and empirical exploration into nu-clear operations, the Navy has maintained an excellent historical track record of safety, reliability, and superior capability relative to other nations’ nuclear submarine programs. The Ohio-class replacement program offers the opportunity to design the next nuclear submarine from the “atom up” – a science-based, bottom-up approach to reactor se-lection and design that considers all associated reactor materials and potentially new reactor types. For example, the pressurized water reactors of the past were selected without knowledge of how materials in nuclear reactor environments degrade at the atomic scale. This knowledge is now available and can be incorporated into the design for the Navy’s new SSBN( ). The Navy has in the past demonstrated an ability to lead in the nuclear energy area34 and their choices with the SSBN( ) will have an impact on the future of nuclear energy. The Navy can, therefore, use this opportunity to set a prec-edent in designing future nuclear reactors to withstand and mitigate the impacts of AEC.
The description below overviews and highlights the historical use of pressurized water re-actors in Navy submarines. Then, we discuss the material properties of these reactors, how they degrade through AEC, and how the Navy can use this information to better mitigate and plan for the impact of AEC as they replace the Ohio-class ballistic missile submarine.
32. C.R.F. A evedo, “A Revie o Neutron-Irradia on- Induced ardening o Metallic Components,” Engineering ailure Analysis 18, No. 8 ( ec 2011): 1921-1942.
33. Ste Magnuson, “Nuclear Po er Plants on Ne Submarines May Last 40-Plus Years,” a onal De ense Magaine, Feb 2015, h p: .na onalde ensemaga ine.org archive 2015 February Pages NuclearPo erPlantson-
Ne SubmarinesMayLast40PlusYears.asp .34. “Nuclear Reactor esign Chosen Not Because It as Sa e But Because It orked on Navy Submarines,”
Washingtons log, 20 une 2011, h p: . ashingtonsblog.com 2011 06 nuclear-reactor-design-chosen-not-because-it- as-sa e-but-because-it- orked-on-navy-submarines.html.
History of Nuclear Reactors in Military
The United States Navy has been using nuclear propulsion in their submarines since the 1950s.35 Unlike their diesel counterparts, which required frequent surfacing (or near-sur-facing if they used snorkels) to charge the batteries used for propulsion while submersed, nuclear powered submarines can remain submersed for extended periods. The ability to remain submersed was a huge advantage because it meant the Navy could avoid exposing submarines on or near the surface. Admiral Hyman Rickover led the develop-ment of Naval nuclear power, including submarines, for over three decades;36 during the initial development, he had several options to choose from as different laboratories were working on prototype reactors that used different materials, different designs, and dif-ferent fuel sources.37 Admiral Rickover settled on a prototype built by the Westinghouse Electric Corporation that used a uranium fuel cycle in a pressurized light water reactor vessel called the Submarine Thermal Reactor. This prototype was developed into the S1W reactor that was used in the rst Navy submarine, the USS 38 Admiral Rick-over’s choice of pressurized water reactors with a uranium fuel cycle was likely based on two things: (a) the desire to use a fuel cycle that produced plutonium as a decay prod-uct that could be puri ed to create nuclear weapons, and (b) the fact the pressurized water reactor prototype met the size, safety, performance, and weight requirements for Navy submarines.39
Admiral Rickover’s decision had a profound impact on the future of nuclear energy within the United States as well as globally. At the time, no standards existed regarding the types of nuclear reactor to be employed for either land or sea based nuclear power. Multiple laboratories were working on different reactor types such as liquid metal reactors,40 molten salt reactors,41 and pressurized water reactors.42 Most of these reactors used uranium-based fuel cycles, but others used a fuel cycle based on thori-um. Different fuel cycles create different decay products, which cause different mech-anisms for degradation within the materials that contain these nuclear reactions. Ad-miral Rickover’s choice gave pressurized water reactors government backing, and as their advantages became apparent it was extremely dif cult for alternative reactors and fuels to break into the nuclear energy market.43 This choice also highlights the im-
35. “Nuclear-Po ered Ships,” World uclear Associa on, Modi ed Aug 2015, Accessed 22 Sept 2015, h p: .orld-nuclear.org in o Non-Po er-Nuclear-Applica ons Transport Nuclear-Po ered-Ships .
36. “ yman G. Rickover,” Wikipedia, Modi ed 20 Sept 2015, Accessed 24 Sept 2015, h ps: en. ikipedia.org ikiyman G. Rickover.
37. M. Ragheb, “Nuclear Marine Propulsion,” Rensselaer olytechnic ns tute, 14 April 2015, h p: mragheb.comNPRE 20402 20ME 20405 20Nuclear 20Po er 20Engineering Nuclear 20Marine 20Propulsion.pd .
38. “Nuclear Propulsion,” AS.org, Modi ed 29 Feb 2000, Accessed 26 Sept 2015, h p: as.org man dod-101 sysship eng reactor.html.
39. “Nuclear Reactor esign Chosen Not Because It as Sa e But Because It orked on Navy Submarines,” Washingtons log, 20 une 2011.
40. O ce o Technology Assessment, Technical p ons or the Advanced i uid Metal Reactor ( ashington, .C.: U.S. Government Prin ng O ce, May 1994).
41. “Thorium-Fuelled Molten Salt Reactors,” The Wein erg ounda on, une 2013, h p: .the- einberg-ounda on.org p-content uploads 2013 06 Thorium-Fuelled-Molten-Salt-Reactors- einberg-Founda on.pd .
42. O ce o Nuclear Energy, Science and Technology, This istory o uclear Energy ( ashington, .C.: U.S. epart-ment o Energy).
43. “Nuclear Reactor esign Chosen Not Because It as Sa e But Because It orked on Navy Submarines,” Washingtons log, 20 une 2011,
160 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
pact decisions the U.S. Military makes can have on civilian and commercial markets in terms of technology adoption.
Pressurized water reactors utilizing a uranium fuel cycle are still the main reactor design for the Navy’s nuclear submarine program. As of 2014, the U.S. Navy operates 75 sub-marines that are powered using pressurized water reactors. Decades of experience in multiple reactors offer the opportunity to leverage the science associated with their ma-terials degradation in new designs. Understanding how the materials used to build these reactors degrade at the atomic scale due to atomic effects corrosion can lead to better predictive models of reliability and safety. The next sections describe these reactors and explore some of the AEC mechanisms and their effects.
Pressurized Water Reactors
It was clear from the beginning that pressurized water reactors (PWR) were going to require unique material properties to deal with the harsh environments in which they operated. For example, it was quickly realized that the materials of the Submarine Ther-
mal Reactor (STR) were sensitive to classical corrosion caused by the extremely hot water reacting with the metal cladding that surrounded the fuel.44 From empirical studies, the rst solution used zirconium for the cladding because it resisted these classi-cal corrosion effects. A more sophisticated understanding of the mechanism causing this degradation led to the development of better materials for the cladding like ircaloy, a zirconium alloy that has better performance than its pure zirconium predecessor.
Most Naval nuclear submarines contain a miniaturized version of the land-based pres-surized water reactor (PWR) types used to provide commercial electrical power in the United States.45 These naval reactors differ in several ways from their land-based counter-parts. Land-based PWRs are much larger, produce more power, and use a less-enriched uranium fuel source made of uranium dioxide. Despite these differences, both the naval and land-based PWRs use the same principles to produce power.
Naval PWRs deliver a lot of energy from a very small volume of fuel. This fuel is made of highly-enriched uranium (93 U-235) alloyed with either zirconium or aluminum.46 This combination helps provide long core lives, and the reactors only need to be refueled after a decade or more of use. These cores are designed to last between 30-40 years. The long core life is due to the purity of the fuel and the introduction of “burnable poison particles” (BPPs) such as boron, which reacts with ssion products as the fuel is used up; the BPPs compensate for reactivity loss as the fuel is consumed, and thereby provide a means of long-term reactivity control.47
44. M. Ragheb, “Nuclear Marine Propulsion,” Rensselaer olytechnic ns tute, 14 April 2015.45. M.F. Ashby and Michael Smidman, “Materials or Nuclear Po er Systems,” RA TA Material nspira on ( anuary
2010), h p: .grantadesign.com do nload pd nuclear.pd .46. “Nuclear- Po ered Ships,” World uclear Associa on, Modi ed Aug 2015, Accessed 22 Sept 2015, h p: .
orld-nuclear.org in o Non-Po er-Nuclear-Applica ons Transport Nuclear-Po ered-Ships .47. .L. Kloosterman, “Applica on o boron and gadolinium burnable poison par cles in UO2 and PUO2 uels in
TRs,” Annals o uclear Energy 30 (2003): 1807-1819.
Pressurized water reactors are still the main reactor design for Navy nuclear submarines.
A schematic of a pressurized reactor plant schematic is shown in the gure below. The system consists of high-strength steel reactor vessel encased with shielding material, a heat exchanger, a primary coolant system, a secondary coolant system, and the associ-ated piping, pumps, and valves. The pressurized ow within the coolant system allows the water to extract heat from the core, and maintaining a constant ow prevents the water from boiling. This pressurized ow allows the water to act as both a coolant and neutron moderator.48 As the water passes through the heat exchanger steam is gener-ated, which is pumped through the secondary system in order to drive the turbines that propel the submarine. The steam then condenses back into water where it is fed back to the steam generators.
Reactor Plant Schematic/NNSA/DoE
The PWRs for all Naval submarines are housed in a central location within the submarine known as the reactor compartment (see gure page 162). The reactor compartment is cylindrical in shape and contains two shielded bulkheads at each end. The Ohio Class submarine reactor compartment, for example, is a large cylinder approximately 55-ft long, 42-ft in diameter and weighs roughly 2750 tons.49 The internal components of these reactors are not typically accessible during the life cycle of the core. The reactors must be able to withstand the extreme operating conditions at sea, plus the harsh internal environment characteristic of all PWRs. As a result, the PWRs’ material components ex-perience the long-term effects of radiation, classical corrosion, and mechanical stresses caused by high temperatures and pressures and temperature/pressure changes.
48. Massoud T. Simnad, “Nuclear Reactor Materials and Fuels,” niversity o Cali ornia, San Diego, 1992, h p: .cryptocomb.org Nuclear 20Reactor 20Materials 20and 20Fuels.pd .
49. “Nuclear Propulsion,” AS.org, Modi ed 29 Feb 2000, Accessed 7 Oct 2015, h p: as.org man dod-101 sysship eng reactor.html.
162 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
PWRs are constructed from a variety of different metals and ceramics, all designed to have speci c mechanical properties critical for the PWR to operate reliably and safely. The important components of a PWR from a material sustainment standpoint are the control rods, the pressure vessel, and the piping/internal components. The control rods are typically made of born carbide or a gold-indium-cadmium alloy. These rods are typi-cally clad in stainless steel tubes. The pressure vessel is made of steel, and most pressure vessels are encased in ircaloy cladding. The piping and internals, as well as the steam generators, are constructed from stainless steels. All of these different metal alloys were selected a e n eir in en e u e an e ire me ani al r er ie because the science to address their vulnerabilities to AEC did not exist.50 That is, the bottom-up sci-ence had yet to be seriously addressed. With recent scienti c advancements, however, this is no longer the case. Any good materials engineer would agree that materials se-lection should be based on both desirable mechanical properties their ability to function for the design lifetime. Now that the underpinning science exists to address not only materials’ mechanical properties but also material sustainment, it has become pos-sible to develop design strategies that ensure important PWR components not only have superior mechanical properties, but also are resistant to the impacts of AEC (as well as other forms of corrosion).
Degradation due to AEC in PWRs on Navy submarines can lead to a variety of failures. For example, AEC degradation can lead to the fracture of a metal alloy. A crack in the reaction vessel could lead to leakage of nuclear material, and potentially force shut-down. Mechanical failures in either of the coolant systems can lead to the PWR operat-ing at temperatures that promote further degradation of the reactor from classic cor-rosion or mechanical stresses, or could lead to lower ef ciencies in converting the heat of the nuclear reaction into propulsive force for the submarine’s propeller. Therefore, the primary materials of concern for AEC in PWRs are the metal alloys from which they are constructed. Because radiation-induced AEC contributes to materials degradation in nuclear reactors, a better understanding of degradation mechanisms at the atomic scale can help improve both selection of materials and reactor designs.
50. Mar uis A. Emmanuelle, “Nuclear reactor materials at the atomic scale,” Materials today 12, No. 11 (2009): 30-37.
AEC Mechanisms in Nuclear Reactors
Having introduced the impact of AEC in the section above, we now turn to a more detailed description of examples of AEC mechanisms. As stated earlier, a PWR reactor utilizes water as a coolant and thus its internal piping is subject to the classical corrosion mechanisms associated with water interacting with materials. In addition, the reactor core functions through the ssion of U-235, and this process releases energy in the form of heat, radiation; and fast, intermediate, and thermal neutrons.51 Most nuclear reactors on land operate at a steady state, meaning they operate at the same level, and pro-duce the same amount of power, over a 24-hr period.52 Naval reactors do not operate like land reactors because the demands of the submarine uctuate as the submarine changes depth, direction, and speed. To meet these demands, the reactor core must operate at different levels, which changes the rates at which it produces heat and ra-diation. As a result, the materials within the PWR will experience a range of temperatures, pressures, radiation levels and neutron uxes (see the gure below).53
Reactor essel/US Energy Information Agency. PD
51. C.R.F. A evedo, “A Revie o Neutron-Irradia on- Induced ardening o Metallic Components,” Engineering ailure Analysis 18, No. 8 ( ec 2011): 1921-1942.
52. M. Ragheb, “Nuclear Marine Propulsion,” Rensselaer olytechnic ns tute, 14 April 2015, h p: mragheb.comNPRE 20402 20ME 20405 20Nuclear 20Po er 20Engineering Nuclear 20Marine 20Propulsion.pd .
164 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
Atomic effects corrosion is concerned with those types of degradation events associ-ated with high-energy collisions, such as those caused by fast (0.1-10 Me ), intermedi-ate (10e -0.1 Me ), and/or thermal (0.025 e at 20 C) ssion-induced neutrons.54 Fast neutrons tend to be the most destructive because they cause displacements within the lattice structures of the PWR materials. These displacements are a consequence of the elastic collision between a neutron and atoms within the material lattice. When displacement occurs it is because the energy of the incoming neutron is suf ciently high to overcome the bonds holding the atom within a lattice. This energy is known as the displacement energy (ED) and is dependent on the composition of the material and the structure of the material lattice.55 For many metals this value is between 20-40 e .56 The amount of energy that can be transferred from a neutron to an existing lattice structure (Em) is dependent on the energy of the neutron and the atomic mass of the atoms within the material lattice.57 When a neutron strikes an atom within a material lattice, it creates what is referred to as a fast moving primary knock-on atom (PKA).58 This atom is ejected with energy equal to the difference between ED and EM (this difference is designated EPKA).59 The ejected atom (i.e., PKA) moves with this energy and eventually elastically collides with other atoms in the lattice.60 Other atoms will be ejected as long as the impacting atom has an Em higher than that atoms ED. The incoming neutron thereby creates a domino effect in which multiple atomic displacements are created producing vacancies and interstitial sites, which are called Frenkel defects.
The AEC resulting from the collision of the incoming neutron leads to what is referred to as a displacement cascade.61 It creates clusters of vacancies within the displacement cascade surrounded by self-interstitial atoms. The numbers of displacement cascades that form over a given unit of time can be estimated. The estimate depends on the total number of Frenkel defects generated by a single PKA (Nd 0.5 EPKA/Ed) and the total number of PKAs generated over a particular unit of time.62 The total number of PKAs is estimated by calculating the product of the ux of neutrons ( O) and the neutron elastic cross-section of an atom within a material lattice ( O). At a neutron ux of 1010 neutrons/cm2-s, for example, iron would experience approximately 5.1 x 1013 atomic displace-ments.63 The typical neutron ux in a reactor’s lifetime will almost certainly exceed this amount, meaning that a huge number of displacement cascades will occur in the pres-sure vessel throughout its life cycle. Therefore, it is important to consider AEC in pressure vessel designs.
The resulting PKA created from a fast neutron, and the corresponding displacement cascade that follows, is accompanied by a local temperature spike that last for a few
54. C.R.F. A evedo, “A Revie o Neutron-Irradia on- Induced ardening o Metallic Components,” Engineering ailure Analysis 18, No. 8 ( ec 2011): 1921-1942.
55. id.56. id.57. id.58. id.59. id.60. id.61. id.62. C. A. English and . M. yde, “Radia on Embri lement o Reactor Pressure essel Steels,” In: I. Milne, R. O.
Ritchie and B. Karihaloo, Comprehensive Structural ntegrity, (O ord, 2003): 351-398.63. C.R.F. A evedo, “A Revie o Neutron-Irradia on- Induced ardening o Metallic Components,” Engineering
ailure Analysis 18, No. 8 ( ec 2011): 1921-1942.
picoseconds. Depending on the material’s composition and structure, the local tem-perature increase can be higher than the melting temperature of the local lattice struc-ture, which can in turn cause further lattice defects. Other mechanisms that can impact the local lattice structure are the rebound effect that occurs as the lattice attempts to stabilize after the impact that initiated PKAs. The extent to which these effects take place within PWR materials, and their impact, depends on the reactor’s operating tem-perature, speci c chemical composition, and the microstructures that exist within the reactor’s material.64
It is not currently possible to follow the precise individual AEC mechanisms and chains of mechanisms produced by neutron bombardment of a material. The damage that can be induced through a neutron collision with an atom in a material lattice structure is dependent on both intrinsic and extrinsic factors. Much of what is known regarding the processes is determined through molecular dynamic computations based on atomic scale modeling.65 These simulations have helped understand that dislocations, grain boundaries and interfaces that naturally occur within the microstructures of PWR materi-als can act as defect sinks for radiation-induced defects.66 The material’s chemical com-position, microstructures, and crystal lattice structure all in uence the impact of atomic effects corrosion. The operating temperature, neutron radiation ux, exposure time, and other environmental stresses are also important factors in the creation and evolution of radiation-induced materials degradation (i.e., AEC).
Atomic scale modeling has also demonstrated that the type of crystal lattice packing can in uence the types of lattice defects that manifest following exposure to high speed neutrons. Metals with either body-centered cubic or face-centered cubic crys-tal structures will have different types and distributions of lattice defects.67 The extent to which radiation leads to degradation of mechanical properties within a PWR material depends on the type, size, spatial distribution, and mobility of the defects. This knowl-edge is currently limited to computational calculations, but as continued research makes it possible to design materials from the “atom up,” atomic scale models will be essential in designing new materials for reactors that are naturally resistant to the impacts of atomic effects corrosion.
A typical PWR on a Navy submarine experiences around 40 years of operation and can be expected to experience neutron uxes up to 1023 neutrons/ cm2-s.68 This ux over such a long time will result in many displacement cascades through the reactor’s life cycle: though individual collisions have effects at the atomic scale, the cumulative affect over time can result in changes observable on the macro scale. For example, displacement
64. Mar uis A. Emmanuelle, “Nuclear reactor materials at the atomic scale,” Materials today 12, No. 11 (2009): 30-37.
65. id.66. U.S. Nuclear Regulatory Commission, E pert anel Report on roac ve Materials Degrada on Assessment (O ce
o Nuclear Regulatory Research, ashington, C, 2006), h p: pbadup s.nrc.gov docs ML0707 ML070710257.pd .
67. C.R.F. A evedo, “A Revie o Neutron-Irradia on- Induced ardening o Metallic Components,” Engineering ailure Analysis 18, No. 8 ( ec 2011): 1921-1942.
68. U.S. Nuclear Regulatory Commission, E pert anel Report on roac ve Materials Degrada on Assessment (O ce o Nuclear Regulatory Research, ashington, C, 2006), h p: pbadup s.nrc.gov docs ML0707 ML070710257.pd .
166 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
cascades can lead to hardening or embrittlement of the material’s microstructures. Hardening/embrittlement increases the likelihood the material will fracture, particularly components that are made of metal alloys. Material hardening can lead to sudden
fracture, which in the high temperature and pressure environ-ment of a reactor that fracture can lead to structural failure. In short, what started as an AEC-induced cascade can become in effect a “macro cascade” causing the reactor to fail unexpect-edly. The PWR is the primary power source on a Navy submarine, and loss of this power source at the wrong time can be cata-strophic. A complete understanding regarding the precise mechanisms of atomic effects corrosion on materials is needed to reduce the potential of such losses.
The Future of AEC in Nuclear Reactors
The Navy’s nuclear submarines have speci c design requirements based on balancing the needed operational capabilities with the systems and technologies that provide them. For example, the overall size of the submarine and the variable buoyancy require-ment (among other things) drive the weight and size of the reactor. Originally, PWRs were selected for Navy nuclear submarines because they could meet these design require-ments. This choice was made at a time when the precise chemistry and physics regard-ing the interactions of radiation with matter were still immature. The relationships the ef-fects of nuclear radiation and materials degradation pathways remained largely unknown during the design, construction, operation, and disposal of the rst reactors on nuclear submarines. Safety and design improvements for submarine reactors were driv-en by empirical knowledge gained through operating experience. The designers simply could not address, a priori, atomic effects corrosion on the reactors because their ef-fects were largely unknown; designers were unaware they could cause problems until after those problems occurred – a posteriori. Now that the Navy has been operating nuclear-powered submarines (and surface ships) for decades, and science has contin-ued to advance during those same decades, this is no longer the case. A suf cient un-derstanding of the bottom-up science regarding the interaction of radiation with materi-als is emerging, thanks to advances in atomic-scale computational modeling and imaging techniques such as the scanning probe microscope. This knowledge can be incorporated into the design, construction, operation, and disposal strategies for future nuclear reactors in military platforms. Current scienti c knowledge already makes it clear that so doing, a priori, can lead to increased operational capabilities, safer submarines, and increased reactor life cycles.
The SSBN( ) is intended to replace the Ohio Class Navy subma-rines; SSBN( ) designs are already being developed. As with all ship designs, SSBN( ) ship architects will use a “design spiral” ap-proach that starts with design concepts and closes in on speci c details later in the process. Thus, there is still time to consider the impacts, including AEC, of the choices that will be made during the nal design process. In this book, we argue that a bottom-up science-based design approach can and should be used
A typical reactor on a Navy submarine is operated for 40 years and experiences high neutron uxes.
Navy nuclear submarine designs balance operational needs with systems and technologies.
to assist in designing future nuclear reactors. Employing a bottom-up design approach enables consideration of and planning for AEC-induced materials degradation in future reactors. Doing so can lead to selection and incorporation of more reliable materials into the reactor design. Along with improved predictive models, designs can assess safety, reliability, and potential failures. A “-up science approach is not limited to materials only; it can also address the radiation environment generated within the reactor. Both materi-als and radiation affect AEC degradation pathways.
Next-generation naval reactor designs may consider thorium-based reactors, or fuel al-ternatives such as relatively new low-enriched uranium fuel cycles.69 One argument for low-enriched fuels is that the current requirement for highly-enriched uranium fuel offers potential adversaries (e.g., Iran) a legitimate rationale for developing highly-enriched uranium , which can also be used to make nuclear weapons. The use of highly-enriched uranium is currently permitted under the nuclear non-proliferation treaty because the United States (and others) use these fuels. As long as countries like the United States use highly-enriched fuels and reactor designs, other countries who want to develop a nuclear submarine program can make a legitimate claim for needing their own nuclear programs that make highly-enriched uranium.70 The SSBN( ) is intended to remain in op-eration for 40 years, and the construction design phase set to begin in 2017.71 Thus, the choices made in SSBN( ) design and development will have major implications in both military and political arenas regarding global nuclear power.
Bryan Clark from the NNSA, a key gure in the design of the SSBN( ), has spoken about the new capabilities nanotechnologies can enable in nuclear reactor designs.72
In 2009, then U.S. Congressman oe Sestak (a former Navy admiral) sought to push the Pentagon to embrace thorium-based reactors for the design of a thorium-fueled ship.73,74 In some ways, this was a response to what nations like China were doing with these technologies. Congressman Sestak proposed that the Navy should be at least consider-ing reactor designs that use alternative fuel cycles like thorium as they move to replace
69. Nate Sans, “ hy the United States should redesign its nuclear submarines,” ulle n o the Atomic Scien sts, 3 Sept 2013, Accessed 6 Oct 2015, h p: thebulle n.org hy-united-states-should-redesign-its-nuclear-subma-rines.
70. ouglas Birch, “Navy should develop ne ship and sub reactors that don t use eapons-grade uranium, e perts say,” The Center or u lic ntegrity, 19 March 2015, Accessed 6 Oct 2015, h p: .publicintegrity.org 2015 03 19 16931 navy-should-develop-ne -ship-and-sub-reactors-don-t-use- eapons-grade-uranium.
71. Ste Magnuson, “Nuclear Po er Plants on Ne Submarines May Last 40-Plus Years,” a onal De ense Magaine, Feb 2015, Accessed 7 Oct 2015, h p: .na onalde ensemaga ine.org archive 2015 February Pages
NuclearPo erPlantsonNe SubmarinesMayLast40PlusYears.asp .72. id.73. avid Lague and Charlie Zhu, “Special Report: The U.S. government la behind Chain s nuclear po er push,”
Reuters, 20 ec 2013, Accessed 6 Oct 2015, h p: .reuters.com ar cle 2013 12 20 us-breakout-thorium-special-report-idINBRE9B 0R 20131220.
74. avid Lague and Charlie Zhu, “Special Report: The U.S. government la behind Chain s nuclear po er push,” Reuters, 20 ec 2013, Accessed 6 Oct 2015, h p: .reuters.com ar cle 2013 12 20 us-breakout-thorium-special-report-idINBRE9B 0R 20131220.
168 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
the Ohio Class, and that it would be unfortunate if a country like China was able to obtain a better nuclear submarine by using a reactor and materials designed around a thorium fuel cycle.75 Ironically, the Chinese obtained the information on how to build thorium nuclear reactors by engaging with Oak Ridge National Laboratories. Essentialy, a complete, bottom-up science-based approach can consider all alternatives, includ-ing different reactor types, to assess the potential of different methods to design systems with superior performance and resistance to the impacts of AEC.
Military and political considerations are not the only aspects a bottom-up design can address. Refueling a nuclear reactor core currently costs almost one billion dollars. If re-actors can be designed using a bottom-up approach to reduce the frequency of refuel-ing and increase their life-cycles, the result could signi cantly reduce the total cost of future reactors. The Navy will need to decide soon on the new design and development plan for SSBN( ). Some within the Navy have already expressed concerns that budget constraints will reduce the numbers of SSBN( ) in the eet.76 A more complete, bottom-up science based design of the nuclear reactor systems to be used in the SSBN( ) may lead to better, more precise cost estimations. In addition, if materials can be optimized – made better and more ef cient at lower total cost – by incorporating science-based design criteria for major systems (and addressing AEC and other degradation mecha-nisms), such designs might lead to more capable nuclear submarines, fewer problems during development, and thus fewer cost overruns. The result could offset some of the SSBN( ) development costs, and potentially lead to being able to procure more of the new submarines. In sum, the more the SSBN( ) program relies on the best available sci-ence regarding nuclear reactor designs, the less likely unexpected problems will arise. As a result, the Navy may be better able to control the cost, schedule and technical risks of developing the next generation of nuclear submarines.
The U.S. Nuclear Regulatory Commission (NRC) has developed a strategy that could help in the Navy’s search for new nuclear powered submarines.77 The Progressive Materi-als Degradation Approach attempts to develop a foundation for identifying appropriate actions to prevent materials degradation from leading to reactor failures. Part of this
approach is predicting which properties within material micro-structures could lead to future failures due to the AEC-prone environment of nuclear reactors. It would be bene cial for the Corrosion Policy Of ce (CPO) to investigate this approach and incorporate applicable principles into its corrosion prevention and control (CPC) strategies and policies throughout the cor-rosion spectrum.
75. “ ould Thorium Po ered Ships be be er or the Navy ” o a a s rom Thorium (blog), 2 Feb 2010, h p: yot-ta a sthorium.blogspot.com 2010 02 thorium-po ered-ships- or-navy.html.
76. “SSBNX Under Pressure: Submarine Chie Says Navy Can t Reduce,” edera on o American Scien sts, 24 uly2013, Accessed 7 Oct 2015, h p: as.org blogs security 2013 07 ssbn -numbers .
77. U.S. Nuclear Regulatory Commission, E pert anel Report on roac ve Materials Degrada on Assessment (O ceo Nuclear Regulatory Research, ashington, C, 2006), h p: pbadup s.nrc.gov docs ML0707 ML070710257.pd .
The U.S. NRC strategy could help the Navy’s new nuclear submarine design.
Acronym De nition
ACAT Acquisition CategoryAEC Atomic Effects CorrosionAFCAD Alternative Futures for Corrosion and Degradation ASTM American Society for Testing and Materials ATOX Atomic OxygenBJT Bipolar Junction TransistorBPP Burnable Poison ParticleCDR Charge Depletion RegionCFR Constant Failure Rate (model)CME Coronal Mass EjectionCPC Corrosion Prevention and ControlCPO Of ce of Corrosion Policy and Oversight Corrosion Policy Of ce DARPA Defense Advanced Research Projects AgencyDD Displacement DamageDMEA Defense Microelectronics Activity DNA Deoxyribonucleic AcidDoD Department of DefenseDoDI Department of Defense InstructionDoE Department of EnergyELF Early Life FailuresFET Field Effect TransistorFIT Failure in TimeFPGA Field Programmable Gate ArrayHCI Hot Carrier InjectionIC Integrated CircuitIR InfraredJFET Junction Field Effect TransistorLED Light Emitting DiodeLEP Life Extention ProgramLET Linear Energy TransferMEMS Micro-Electro-Mechanical SystemsMIL-HDBK Military HandbookMOSFET Metal Oxide Semiconductor Field Effect TransistorMRI Magnetic Resonance Imaging or ImagersMTTF Mean Time to FailureNASA National Aeronautics and Space AdministrationNEMS Nano-Electro-Mechanical SystemsNNSA National Nuclear Security Administration
GLOSSARY OF ACRONYMS
170 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
NRC Nuclear Regulatory CommissionOSD Of ce of the Secretary of DefensePIPS Potomac Institute for Policy StudiesPKA Primary Knock-on AtomPV PhotovoltaicPVC Polyvinyl ChloridePWR Pressurized Water ReactorRAM Random Access MemoryRDT E Research, Development, Test and EvaluationSEB Single Event BurnoutSEE Single Event EffectSEL Single Event LatchupSET Single Event TransientSEU Single Event UpsetSRAM Static Random Access MemorySSBN U.S. Navy NuclearBallistic-missile SubmarineSSGN U.S. Navy Nuclear Guided-missile SubmarineSSN U.S. Navy Nuclear SubmarineSTR Submarine Thermal ReactorTID Total Ionizing DoseTOW Tube-launched, Optically-tracked, Wire-guided (missile)UAV Unmanned Aerial VehicleUHV Ultrahigh VacuumUV UltravioletVHSIC Very High-Speed Integrated CircuitVSEPR Valence Shell Electron Pair Repulsion (theory)WWII World War II
IMAGE CREDITS“Artist’s conception of a gamma ray collision in a semiconductor lattice”, on cover and title page by Alex Taliesen.
by Alex Taliesen.
“Evolution of lighting” vexworldwide/Image ID: 280630649/www.shutterstock.com.
“Jet Fighter Aircraft Mesh. Part of a series” by Nuno Andre/Image ID: 120354058/www.shutterstock.com.
“computer motherboard closeup” by chungking/Image ID: 258734219/www.shutter-stock.com.
“Artist’s conception of a gamma ray collision in a semiconductor lattice” by Alex Taliesen.
by Alex Taliesen.
“Laptop” by Alex Taliesen.
“The Atom” by Alex Taliesen.
“The three isotopes of hydrogen” “Protium deuterium tritium” by Lamiot for french ver-sion, from Dirk H nniger - self, translation from Dirk H nniger (german wikipedia). Licensed under CC B -SA 3.0 via Wikimedia Commons. https://commons.wikimedia.org/wiki/File:Periodic trends.svg.
“Diagram of the various periodic trends” by Mirek2 (Own work) CC0 1.0 Universal. , via Wikimedia Commons https://commons.wikimedia.org/wiki/File:Periodic trends.svg.
“Forming and dissolving of table salt” by Alex Taliesen.
“Oxidation and Reduction” by Alex Taliesen.
“Chemical reaction” by Aushulz (Own work) CC B -SA 3.0 (http://creativecommons.org/licenses/by-sa/3.0) , via Wikimedia Commons. https://commons.wikimedia.org/wiki/File:Chemical reactions.svg.
electrons.” Image creator: Lucas Taylor. CERN. http://cds.cern.ch/record/628469.
“Lightning” by Timothy Kirkpatrick (Lightning pics) Public domain , via Wikimedia Com-mons. https://commons.wikimedia.org/wiki/File:Lightning.0257.jpg.
active decay.” Generated by Kieran Maher using Aldus SuperPaint. Public domain , via Wikimedia Commons. https://en.wikibooks.org/wiki/File:Radioactive decay.gif.
172 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
by Cmglee (Own work) CC B -SA 3.0 , via Wikimedia Commons https://commons.wikimedia.org/wiki/File:Comparison semicon-ductor process nodes.svg.
by Robert Steffens (alias RobbyBer 8 Novem-ber 2004), S G: Marlus Gancher, Antonsusi (talk) using a le from Marlus Gancher. See File talk:Schema Siedewasserreaktor.svg License history GFDL (http://www.gnu.org/copyleft/fdl.html) , via Wikimedia Commons. https://commons.wikimedia.org/wiki/File:Boiling water reactor english.svg.
“Nuclear Waste Barrels” Flickr, Iwan Gabovitch CC0 Public Domain, (CC B 2.0) https://www. ickr.com/photos/qubodup/6992896138/in/photostream.
Image credit: National Weather Service. http://www.srh.noaa.gov/srh/jetstream/atmos/atmpro le.htm.
“Experience in microchip life cycles” by Alex Taliesen.
Illustration by Kristian Molhave. Opensource Handbook of Nanoscience and Nanotechnology. https://com-mons.wikimedia.org/wiki/File:SPM overview.jpg.
by Alex Taliesen.
“ClipartOf.com.” 3d rendered single red cube at the bottom of a crumbling tower of white cubes by Tonis Pan, COLLC0042.
“Forcing atoms into dense spaces can lead to the creation of unique electrons.” Image credit: Alex Taliesen.
“Vibrations of Atoms.”. Image credit: Alex Taliesen.
“Magnetic Moments from Orbital Movement and Spin.” Image credit: Alex Taliesen.
”Ruby Laser Beam” by Mcgill Mcgill - self-made. Licensed under Public Domain via Wiki-books - https://en.wikibooks.org/wiki/File:Ruby laser beam.png /media/File:Ruby la-ser beam.png.
“Periodic Table of Elements” Periodic Table Of Elements With Color Delimitation/Maximil-ian Laschon/ Image ID: 172309694/www.shutterstock.com.
“Microscopic structure of steel.” Webcorr. https://commons.wikimedia.org/wiki/File:Microstructure of a sensitized type 304 stainless steel.jpg.
(CC B -SA 3.0) https://commons.wikimedia.org/wiki/ SEPR.
“Critical Radius Ratio” by Matthew Rollings. PD. https://commons.wikimedia.org/wiki/File:Criticalradiusratio.png.
“Spinel Structure” by Perditax, PD. https://commons.wikimedia.org/wiki/File:Spinel struc-ture.png.
y Wimmel (Own work) Public domain , via Wikimedia Commons. https://commons.wikimedia.org/wiki/File:SiO C2 B2 uartz.svg.
“The by Wimmel (Own work) Public domain , via Wikimedia Commons. https://commons.wikimedia.org/wiki/File:Silica.svg.
“Crystal Lattice Point Defects” by Alex Taliesen.
“Examples of traditional ceramics.” Attribution 4.0 International (CC B 4.0) http://www.scielo.br/img/revistas/ce/v60n354/a16 g05.jpg.
“MEMS microcantilever resonating in an SEM” by Pc et01 at en.wikipedia CC B -SA 3.0 (http://creativecommons.org/licenses/by-sa/3.0) from Wikimedia Commons. https://up-load.wikimedia.org/wikipedia/commons/3/34/MEMS Microcantilever in Resonance.png.
“The effect of applied by Creepin475 (Own work) CC B -SA 3.0 (http://creativecommons.org/licenses/by-sa/3.0) https://commons.wiki-
media.org/wiki/File:Piezoelectric. PG via Wikimedia Commons.
translated from Ger-man “Prinzipieller Aufbau eines n-Kanal-MOSFETs im uerschnitt” by PNG- ersion: Markus A. Hennig (17. Dezember 2005) S G-Umsetzung Cepheiden (:Datei:N-Kanal-MOSFET.png) GFDL (http://www.gnu.org/copyleft/fdl.html) or CC-B -SA-3.0 (http://creative-commons.org/licenses/by-sa/3.0/) , via Wikimedia Commons https://upload.wikimedia.org/wikipedia/commons/a/ad/N-Kanal-MOSFET 28Schema 29.svg.
” by W2raphael (Own work) Public domain , via Wikime-dia Commons. https://commons.wikimedia.org/wiki/File:Nanotubos enrolamento.PNG.
“Ethane three dimensional bonding structure” by Alex Taliesen.
“Differing ethane rotational orientations” by Alex Taliesen.
“Different linkages of copolymers” by Alex Taliesen.
174 ALTERNATIVE FUTURES FOR CORROSION AND DEGRADATION RESEARCH
“Schematic of an by Materialscientist - Own work. Licensed under CC B -SA 3.0 via Wikimedia Commons - https://commons.wikimedia.org/wiki/File:OfetEng.png /media/File:OfetEng.png.
Diagram of the es, the by Inductiveload (Own work (Own Drawing)) Public domain , via Wikimedia Commonsorg/wiki/File:Pn unction Diffusion and Drift.
The basic operation of an NPN BJT in Active mode. By Inductiveload https://commons.wikimedia.org/wiki/File:NPN B T Basic Operation (Active).svg PD .
by Cyril BUTTA CC B -SA 3.0 https://cre-ativecommons.org/licenses/by-sa/3.0/deed.en. https://commons.wikimedia.org/wiki/File:Lateral mosfet.svg.
by Norro. CC B -SA 2.5. https://com-mons.wikimedia.org/wiki/File:Scheme of n-junction eld-effect transistor de.svg /me-dia/File:Scheme of n-junction eld-effect transistor de.svg.
“A visual representation of grain boundaries” by Wlytle1375 https://upload.wikimedia.org/wikipedia/commons/4/40/Grain boundary diagram.jpg PD .